This book contains information obtained from authentic and highly regardedsources. Reprinted material is quoted with permission, and sources are indicated.Reasonable efforts have been made to publish reliable data and information, butthe author and the publishers cannot assume responsibility for the validity of allmaterials. Neither the author nor the publishers, nor anyone else associated withthis publication, shall be liable for any loss, damage or liability directly orindirectly caused or alleged to be caused by this book.
Neither this book nor any part may be reproduced or transmitted in any formor by any means, electronic or mechanical, including photocopying, microfilmingand recording, or by any information storage or retrieval system, withoutpermission in writing from the publishers.
The consent of Woodhead Publishing and CRC Press does not extend tocopying for general distribution, for promotion, for creating new works, or forresale. Specific permission must be obtained in writing from Woodhead Publishingor CRC Press for such copying.
Trademark notice: Product or corporate names may be trademarks or registeredtrademarks, and are used only for identification and explanation, without intent toinfringe.
British Library Cataloguing in Publication DataA catalogue record for this book is available from the British Library.
Library of Congress Cataloging in Publication DataA catalog record for this book is available from the Library of Congress.
Woodhead Publishing ISBN 1 85573 567 9CRC Press ISBN 0-8493-1551-4CRC Press order number: WP1551
Typeset by SNP Best-set Typesetter Ltd., Hong KongPrinted by TJ International, Padstow, Cornwall, England
Engineering is not an exact science and, of the many disciplines within engi-neering, welding is probably one of the most inexact – rather more of anart than a science. Much of the decision-making is based on experience anda ‘gut feel’ for what is or is not acceptable. When the difficulties of shopfloor or site control are taken into account and the occasional vagaries ofthe welder and the sometimes inadequate knowledge of supervisory staffare added, the problems of the practising shop floor engineer can appearoverwhelming. I hope that some of this uncertainty can be dispelled in thisbook, which is aimed at those engineers with little or no knowledge of metallurgy and perhaps only the briefest acquaintance with the weldingprocesses. It does not purport to be a metallurgical or processes textbookand I make no apology for this. Having lectured fairly extensively onwelding technology, I have come to realise that most engineers think ofmetals as being composed of a large number of small billiard balls heldtogether by some form of glue. I have attempted to describe the metallur-gical aspects of the aluminium alloys in these terms. I have therefore keptthe contents descriptive and qualitative and have avoided the use of mathematical expressions to describe the effects of welding.
The book provides a basic understanding of the metallurgical principlesinvolved in how alloys achieve their strength and how welding can affectthese properties. I have included sections on parent metal storage and prepa-ration prior to welding and have also described the more frequently encoun-tered processes. There are recommendations on welding parameters thatmay be used as a starting point for the development of a viable welding pro-cedure. Also included are what I hope will be useful hints and tips to avoidsome of the pitfalls of welding these sometimes problematic materials.
I would like to thank my colleagues at TWI, particularly Bob Spiller,Derek Patten and Mike Gittos, for their help and encouragement duringthe writing of this book – encouragement that mostly took the form of‘Haven’t you finished it yet?’. Well, here it is. Any errors, inaccuracies oromissions are mine and mine alone.
1 Introduction to the welding of aluminium 1
1.1 Introduction 11.2 Characteristics of aluminium 41.3 Product forms 61.4 Welding: a few definitions 6
2 Welding metallurgy 10
2.1 Introduction 102.2 Strengthening mechanisms 102.3 Aluminium weldability problems 182.4 Strength loss due to welding 31
3 Material standards, designations and alloys 35
3.1 Designation criteria 353.2 Alloying elements 353.3 CEN designation system 363.4 Specific alloy metallurgy 403.5 Filler metal selection 46
4 Preparation for welding 51
4.1 Introduction 514.2 Storage and handling 514.3 Plasma-arc cutting 524.4 Laser beam cutting 584.5 Water jet cutting 634.6 Mechanical cutting 644.7 Cleaning and degreasing 66
5 Welding design 69
5.1 Introduction 695.2 Access for welding 705.3 Welding speed 715.4 Welding position 725.5 Edge preparation and joint design 725.6 Distortion 845.7 Rectification of distortion 885.8 Fatigue strength of welded joints 89
6 TIG welding 97
6.1 Introduction 976.2 Process principles 976.3 Mechanised/automatic welding 1146.4 TIG spot and plug welding 115
7 MIG welding 116
7.1 Introduction 1167.2 Process principles 1167.3 Welding consumables 1307.4 Welding procedures and techniques 1357.5 Mechanised and robotic welding 1417.6 Mechanised electro-gas welding 1437.7 MIG spot welding 144
Appendix A British and ISO standards related to welding and aluminium 216
Appendix B Physical, mechanical and chemical properties at 20°C 226
Appendix C Principal alloy designations: cast products 227Appendix D Alloy designations: wrought products 228
The existence of aluminium (Al) was postulated by Sir Humphrey Davy in the first decade of the nineteenth century and the metal was isolated in1825 by Hans Christian Oersted. It remained as somewhat of a labora-tory curiosity for the next 30 years when some limited commercial pro-duction began, but it was not until 1886 that the extraction of aluminiumfrom its ore, bauxite, became a truly viable industrial process. The methodof extraction was invented simultaneously by Paul Heroult in France and Charles M. Hall in the USA and this basic process is still in use today.Because of its reactive nature aluminium is not found in the metallic state in nature but is present in the earth’s crust in the form of differentcompounds, of which there are several hundreds. The most important and prolific is bauxite. The extraction process consists of two separatestages, the first being the separation of aluminium oxide, Al2O3 (alumina),from the ore, the second the electrolytic reduction of the alumina atbetween 950°C to 1000°C in cryolite (Na3AlF6). This gives an aluminium,containing some 5–10% of impurities such as silicon (Si) and iron (Fe),which is then refined either by a further electrolytic process or by a zone-melting technique to give a metal with a purity approaching 99.9%.At the close of the twentieth century a large proportion of aluminium wasobtained from recovered and remelted waste and scrap, this source alonesupplying almost 2 million tonnes of aluminium alloys per annum in Europe(including the UK) alone. The resulting pure metal is relatively weak andas such is rarely used, particularly in constructional applications.To increasemechanical strength, the pure aluminium is generally alloyed with metalssuch as copper (Cu), manganese (Mn), magnesium (Mg), silicon (Si) andzinc (Zn).
One of the first alloys to be produced was aluminium–copper. It wasaround 1910 that the phenomenon of age or precipitation hardening in thisfamily of alloys was discovered, with many of these early age-hardening
1Introduction to the welding of aluminium
alloys finding a ready use in the fledgling aeronautical industry. Since thattime a large range of alloys has been developed with strengths which canmatch that of good quality carbon steel but at a third of the weight.A majorimpetus to the development of aluminium alloys was provided by the twoWorld Wars, particularly the Second World War when aluminium becamethe metal in aircraft structural members and skins. It was also in this periodthat a major advance in the fabrication of aluminium and its alloys cameabout with the development of the inert gas shielded welding processes ofMIG (metal inert gas) and TIG (tungsten inert gas). This enabled high-strength welds to be made by arc welding processes without the need foraggressive fluxes. After the end of the Second World War, however, thereexisted an industry that had gross over-capacity and that was searching forfresh markets into which its products could be sold. There was a need forcheap, affordable housing, resulting in the production of the ‘prefab’, a prefabricated aluminium bungalow made from the reprocessed remains ofmilitary aircraft – not quite swords into ploughshares but a close approxi-mation! At the same time domestic utensils, road vehicles, ships and struc-tural components were all incorporating aluminium alloys in increasingamounts.
Western Europe produces over 3 million tonnes of primary aluminium(from ore) and almost 2 million tonnes of secondary or recycled aluminiumper year. It also imports around 2 million tonnes of aluminium annually,resulting in a per capita consumption of approximately 17kg per year.Aluminium now accounts for around 80% of the weight of a typical civil-ian aircraft (Fig. 1.1) and 40% of the weight of certain private cars. If pro-duction figures remain constant the European automotive industry isexpected to be consuming some 2 million tonnes of aluminium annually bythe year 2005. It is used extensively in bulk carrier and container ship super-structures and for both hulls and superstructures in smaller craft (Fig. 1.2).The new class of high-speed ferries utilises aluminium alloys for both thesuper-structure and the hull. It is found in railway rolling stock, roadsidefurniture, pipelines and pressure vessels, buildings, civil and military bridg-ing and in the packaging industry where over 400000 tonnes per annum isused as foil. One use that seems difficult to rationalise in view of the generalperception of aluminium as a relatively weak and soft metal is its use inarmoured vehicles (Fig. 1.3) in both the hull and turret where a combina-tion of light weight and ballistic performance makes it the ideal materialfor fast reconnaissance vehicles.
This wide range of uses gives some indication of the extensive numberof alloys now available to the designer. It also gives an indication of the difficulties facing the welding engineer. With the ever-increasing sophis-tication of processes, materials and specifications the welding engineer must have a broad, comprehensive knowledge of metallurgy and welding
2 The welding of aluminium and its alloys
Introduction to the welding of aluminium 3
1.1 BAC 146 in flight. Courtesy of TWI Ltd.
1.2 A Richardson and Associates (Australia) Ocean Viewer all-aluminium vessel. The hull is 5mm thick A5083. Courtesy TWI Ltd.
processes. It is hoped that this book will go some way towards giving thepractising shop-floor engineer an appreciation of the problems of weldingthe aluminium alloys and guidance on how these problems may be over-come. Although it is not intended to be a metallurgical textbook, some metallurgical theory is included to give an appreciation of the underlyingmechanisms of, for instance, strengthening and cracking.
1.2 Characteristics of aluminium
Listed below are the main physical and chemical characteristics of aluminium, contrasted with those of steel, the metal with which the bulk ofengineers are more familiar.As can be seen from this list there are a numberof important differences between aluminium and steel which influence thewelding behaviour:
• The difference in melting points of the two metals and their oxides. Theoxides of iron all melt close to or below the melting point of the metal;aluminium oxide melts at 2060°C, some 1400°C above the melting pointof aluminium. This has important implications for the welding process,as will be discussed later, since it is essential to remove and disperse thisoxide film before and during welding in order to achieve the requiredweld quality.
• The oxide film on aluminium is durable, highly tenacious and self-healing. This gives the aluminium alloys excellent corrosion resistance,enabling them to be used in exposed applications without additionalprotection. This corrosion resistance can be improved further by anodising – the formation of an oxide film of a controlled thickness.
• The coefficient of thermal expansion of aluminium is approximatelytwice that of steel which can mean unacceptable buckling and distor-tion during welding.
• The coefficient of thermal conductivity of aluminium is six times that ofsteel. The result of this is that the heat source for welding aluminiumneeds to be far more intense and concentrated than that for steel. Thisis particularly so for thick sections, where the fusion welding processescan produce lack of fusion defects if heat is lost too rapidly.
• The specific heat of aluminium – the amount of heat required to raisethe temperature of a substance – is twice that of steel.
• Aluminium has high electrical conductivity, only three-quarters that ofcopper but six times that of steel. This is a disadvantage when resistancespot welding where the heat for welding must be produced by electri-cal resistance.
• Aluminium does not change colour as its temperature rises, unlike steel. This can make it difficult for the welder to judge when melting is about to occur, making it imperative that adequate retraining of the welder takes place when converting from steel to aluminiumwelding.
• Aluminium is non-magnetic which means that arc blow is eliminated asa welding problem.
• Aluminium has a modulus of elasticity three times that of steel whichmeans that it deflects three times as much as steel under load but canabsorb more energy on impact loading.
• The fact that aluminium has a face-centred cubic crystal structure (seeFig. 2.2) means that it does not suffer from a loss of notch toughness asthe temperature is reduced. In fact, some of the alloys show an improve-ment in tensile strength and ductility as the temperature falls, EW-5083(Al Mg 4.5Mn) for instance showing a 60% increase in elongation afterbeing in service at -200°C for a period of time. This crystal structurealso means that formability is very good, enabling products to be pro-duced by such means as extrusion, deep drawing and high energy rateforming.
• Aluminium does not change its crystal structure on heating and cooling,unlike steel which undergoes crystal transformations or phase changesat specific temperatures. This makes it possible to harden steel by rapidcooling but changes in the cooling rate have little or no effect on thealuminium alloys (but see precipitation hardening p 16–17).
Introduction to the welding of aluminium 5
1.3 Product forms
Aluminium is available in both wrought and cast forms. The wrought formscomprise hot and cold rolled sheet, plate, rod, wire and foil. The ductilityand workability of aluminium mean that extrusion is a simple method ofproducing complex shapes, particularly for long, structural members suchas I and H beams, angles, channels,T-sections, pipes and tubes. Forging, bothhot and cold, is used extensively as a fast, economical method of producingsimple shapes. Precision forging is particularly suitable for aluminiumalloys, giving advantages of good surface finish, close tolerances, optimumgrain flow and the elimination of machining.
The four most commonly used methods of casting are sand casting, lostwax casting, permanent steel mould casting and die-casting. The require-ment for high fluidity in a casting alloy means that many are based on aluminium–silicon alloys although heat-treatable (age-hardening) alloysare often used for sand, lost wax and permanent mould castings. Lost waxand die-casting give products with smooth surfaces to close tolerances andare processes used extensively for aerospace products. A number of alloys,their product forms and applications are listed in Table 1.1.
1.4 Welding: a few definitions
Before dealing with the problems of welding aluminium alloys there are afew definitions required, not least of which is welding itself. Welding can bedescribed as the joining of two components by a coalescence of the surfacesin contact with each other. This coalescence can be achieved by melting thetwo parts together – fusion welding – or by bringing the two parts togetherunder pressure, perhaps with the application of heat, to form a metallicbond across the interface. This is known as solid phase joining and is oneof the oldest of the joining techniques, blacksmith’s hammer welding havingbeen used for iron implement manufacture for some 3500 years. The moremodern solid phase techniques are typified by friction welding. Brazing,also an ancient process, is one that involves a braze metal which melts at atemperature above 450°C but below the melting temperature of the com-ponents to be joined so that there is no melting of the parent metals. Sol-dering is an almost identical process, the fundamental difference being thatthe melting point of the solder is less than 450°C. The principal processesused for the joining of aluminium are listed in Table 1.2. Not all of theseprocesses are covered in this book as they have a very limited applicationor are regarded as obsolescent.
Welding that involves the melting and fusion of the parent metals onlyis known as autogenous welding, but many processes involve the addition
6 The welding of aluminium and its alloys
Introduction to the welding of aluminium 7
Table 1.1 Typical forms and uses of aluminium alloys
Aluminium Product form Applicationalloy Grade
Pure aluminium Foil, rolled plate, Packaging and foil, roofing, extrusions cladding, low-strength corrosion
resistant vessels and tanks2000 series Rolled plate and sheet, Highly stressed parts, aerospace
(Al-Cu) extrusions, forgings structural items, heavy duty forgings, heavy goods vehicle wheels, cylinder heads, pistons
3000 series Rolled plate and sheet, Packaging, roofing and cladding,(Al-Mn) extrusions, forgings chemical drums and tanks,
architectural purposes5000 series Rolled plate and sheet, Cladding, vessel hulls and
(Al-Mg) extrusions, forgings, superstructures, structural tubing and piping members, vessels and tanks,
vehicles, rolling stock, architectural purposes
6000 series Rolled plate and sheet, High-strength structural members,(Al-Si-Mg) extrusions, forgings, vehicles, rolling stock, marine
tubing and piping applications, architectural applications.
7000 series Rolled plate and sheet, High strength structural members, (Al-Mg-Zn) extrusions, forgings heavy section aircraft forgings,
military bridging, armour plate, heavy goods vehicle and rollingstock extrusions
Table 1.2 Principal processes for the welding of aluminium
Tungsten inert gas High-quality, all position welding process that utilises a non-consumable electrode; may be used with or without wire additions; may be manual, mechanised or fully automated; low deposition rate, higher with hot wire additions; straight or pulsed current.
Metallic arc inert High-quality, all position welding process that utilises gas shielded a continuously fed wire; may be manual,
mechanised or fully automated; can be high deposition rate; twin wire additions; straight or pulsed current.
8 The welding of aluminium and its alloys
Table 1.2 (cont.)
Manual metal arc Limited application; uses a flux-coated consumable electrode; non- or lightly stressed joints; obsolescent.
and electronic equipment; high capital cost.Electro-gas, electro-slag, Limited applications, e.g. large bus bars; porosity
submerged arc problems; largely obsolescent.
Welding with fusion and pressure
Magnetically impelled Butt joints in pipe; capital equipment required but arc butt welding lower cost than flash butt; fully automated.
Resistance and flash welding
Spot, projection spot Lap joints in sheet metal work, automotive, seam welding holloware, aerospace industry; high capital cost;
high productivity.Weld bonding Combination of spot welding through an adhesively
bonded lap joint; automotive industry; very good fatigue strength.
High-frequency Butt joints; production of pipe from strip; high capital induction seam cost; high production rates.
Flash butt welding In line and mitre butt joints in sheet, bar and hollow sections; dissimilar metal joints, e.g. Al-Cu; high capital cost; high production rates.
Condenser, capacitor Stud diameters 6mm max, e.g. insulating pins, pan discharge handles, automotive trim, electrical contacts.
Drawn arc Stud diameters 5–12mm.
Solid phase bonding
Friction welding Butt joints in round and rectangular bar and hollow sections; flat plate and rolled section butt welds (friction stir); dissimilar metal joints; capital equipment required.
Explosive welding Field pipeline joints; dissimilar metal joints, surfacing.
Ultrasonic welding Lap joints in foil; thin to thick sections; Al-Cu joints for electrical terminations.
Cold pressure welding Lap and butt joints, e.g. Al-Cu, Al-steel, Al sheet and wire.
Hot pressure welding Roll bonded lap joints, edge to edge butt joints.
of a filler metal which is introduced in the form of a wire or rod and meltedinto the joint. Together with the melted parent metal this forms the weldmetal. Definitions of the terms used to describe the various parts of awelded joint are given in Chapter 5.
Introduction to the welding of aluminium 9
Ideally a weldment – by this is meant the complete joint comprising the weldmetal, heat affected zones (HAZ) and the adjacent parent metal – shouldhave the same properties as the parent metal.There are, however, a numberof problems associated with the welding of aluminium and its alloys thatmake it difficult to achieve this ideal.The features and defects that may con-tribute to the loss of properties comprise the following:
• Gas porosity.• Oxide inclusions and oxide filming.• Solidification (hot) cracking or hot tearing.• Reduced strength in the weld and HAZ.• Lack of fusion.• Reduced corrosion resistance.• Reduced electrical resistance.
This chapter deals with the first four of these problem areas, i.e. those ofporosity, oxide film removal, hot cracking and a loss of strength. Before dis-cussing these problems, however, there is a brief introduction as to howmetals achieve their mechanical properties. Some of the terms used todescribe specific parts of a welded joint are shown in Fig. 2.1.
2.2 Strengthening mechanisms
There are five separate strengthening mechanisms that can be applied tothe aluminium alloys. These are grain size control, solid solution alloying,second phase formation, strain hardening (cold work) and precipitation orage hardening.
2.2.1 Structure of metals
Before discussing the principles by which metals achieve their mechanicalstrength it is necessary to have an appreciation of their structure and howthese structures can be manipulated to our benefit. The simple model of anatom is of a number of electrons in different orbits circling a central nucleus.In a metal the electrons in the outer orbit are free to move throughout thebulk of the material. The atoms, stripped of their outer electrons, becomepositively charged ions immersed in a ‘cloud’ of negatively charged elec-trons. It is the magnetic attraction between the positively charged ions andthe cloud of mobile, negatively charged electrons that binds the metaltogether. These atomic scale events give metals their high thermal and
Welding metallurgy 11
Weld face Heat affected zone
Single sided butt weldWeld toesface androot
Root pass orpenetration bead
Double sided weld
Root Fillet weld
2nd side welded
1st side welded
2.1 Definition of weld features.
electrical conductivity and the ability to deform extensively before fractur-ing by a process known as slip, where one plane of atoms slides over itsneighbours.
In metals the atoms are arranged in a regular three-dimensional patternrepeated over a long distance on what is termed a space lattice. Conven-tionally, these atoms are visualised as solid spheres. The smallest atomicarrangement is the unit cell, the least complicated unit cell being the simplecube with an atom at each corner of the cube. In metals the three mostcommon arrangements are body-centred cubic (BCC), face-centred cubic(FCC) and hexagonal close packed (HCP). Schematic views of the threestructures are given in Fig. 2.2.
Each crystal structure confers certain physical properties on the metal.The face-centred cubic metals, of which aluminium is one, are ductile,formable and have high toughness at low temperatures. Although singlecrystals can be obtained it is more common for metals to be polycrystalline,that is, made up of a very large number of small grains. Each grain is acrystal with a regular array of atoms but at the boundaries between thegrains there is a mismatch, a loss of order, in the orientation of these arrays.Both the grain boundaries and the size of the grains can have a markedeffect on the properties of the metal.
2.2.2 Grain size control
Grain size is not generally used to control strength in the aluminium alloys,although it is used extensively in reducing the risk of hot cracking and incontrolling both strength and notch toughness in C/Mn and low-alloy steels.In general terms, as grain size increases, the yield and ultimate tensilestrengths of a metal are reduced.The yield strength sy, is related to the grainsize by the Hall–Petch equation:
s sy I y= + -k d 1 2
12 The welding of aluminium and its alloys
(a) (b) (c)
2.2 The three crystalline forms of metals: (a) body-centred cubic; (b)face-centred cubic; (c) close-packed hexagonal. (From John Lancaster,Metallurgy of Welding, 6th edn, 1999.)
where d is the average grain diameter, and sI and ky are constants for themetal. Typical results of this relationship are illustrated in Fig. 2.3.
The practical consequence of this is that a loss of strength is often encoun-tered in the HAZ of weldments due to grain growth during welding. A lossof strength may also be found in the weld metal which is an as-cast struc-ture with a grain size larger than that of the parent metal. In the aluminiumalloys the strength loss due to grain growth is a marginal effect, with othereffects predominating. Grain size does, however, have a marked effect onthe risk of hot cracking, a small grain size being more resistant than a largegrain size.Titanium, zirconium and scandium may be used to promote a finegrain size, these elements forming finely dispersed solid particles in the weldmetal. These particles act as nuclei on which the grains form as solidifica-tion proceeds.
2.2.3 Solid solution strengthening
Very few metals are used in the pure state, as generally the strength is insufficient for engineering purposes. To increase strength the metal isalloyed, that is mixed with other elements, the type and amount of the alloying element being carefully selected and controlled to give the desiredproperties. An alloy is a metallic solid formed by dissolving, in the liquidstate, one or more solute metals, the alloying elements, in the bulk metal, the solvent. On cooling the alloy solidifies as a solid solution whichcan exist over a range of compositions, all of which will be homogeneous.Depending upon the metals involved a limit of solid solubility may be
Welding metallurgy 13
2.3 General relationship of grain size with strength, ductility andtoughness.
reached. Microscopically a solid solution is featureless but once the limit of solid solubility is reached a second component or phase becomes visible. This phase may be a secondary solid solution, an inter-metallic compound or the pure alloying element.The introduction of a second phaseresults in an increase in strength and hardness, for instance iron carbide(Fe3C) in steels, copper aluminide (CuAl2) in the aluminium–copper alloysand silicon (Si) in the aluminium–silicon alloys.
In solid solution alloying the alloying element or solute is completely dissolved in the bulk metal, the solvent. There are two forms of solid solution alloying – interstitial and substitutional – illustrated in Fig. 2.4.Interstitial alloying elements fit into the spaces, the interstices, between thesolvent atoms, and substitutional elements replace or substitute for thesolvent atoms, provided that the diameter of the substitutional atom iswithin ±15% of the solvent atomic diameter. The effect of these alloyingelements is to distort the space lattice and in so doing to introduce a straininto the lattice. This strain increases the tensile strength but as a generalrule decreases the ductility of the alloy by impeding the slip between adja-cent planes of atoms.
Many elements will alloy with aluminium but only a relatively small number of these give an improvement in strength or weldability.The most important elements are silicon, which increases strength and fluidity; copper, which can give very high strength; magnesium whichimproves both strength and corrosion resistance; manganese, which gives both strength and ductility improvements; and zinc, which, in com-bination with magnesium and/or copper, will give improvements in strengthand will assist in regaining some of the strength lost when welding.
14 The welding of aluminium and its alloys
Substitutionalor solutealloying atom
Main alloyor solventatom
Main alloyor solventatom
Interstitial orsolute alloyingatom
2.4 Schematic illustration of substitutional and interstitial alloying.
2.2.4 Cold working or strain hardening
Cold work, work hardening or strain hardening is an important process used to increase the strength and/or hardness of metals and alloys thatcannot be strengthened by heat treatment. It involves a change of shape brought about by the input of mechanical energy. As deformationproceeds the metal becomes stronger but harder and less ductile, as shownin Fig. 2.5, requiring more and more power to continue deforming the metal.Finally, a stage is reached where further deformation is not possible – themetal has become so brittle that any additional deformation leads to frac-ture. In cold working one or two of the dimensions of the item being coldworked are reduced with a corresponding increase in the other dimen-sion(s). This produces an elongation of the grains of the metal in the direc-tion of working to give a preferred grain orientation and a high level ofinternal stress.
The increase in internal stress not only increases strength and reducesductility but also results in a very small decrease in density, a decrease inelectrical conductivity, an increase in the coefficient of thermal expansionand a decrease in corrosion resistance, particularly stress corrosion resis-tance. The amount of distortion from welding is also likely to be far greaterthan from a metal which has not been cold worked.
Welding metallurgy 15
Amount of cold work
2.5 Illustration of the effect of cold work on strength, hardness andductility.
If a cold worked metal is heated a temperature is reached where theinternal stresses begin to relax and recovery begins to take place. Thisrestores most of the physical properties of the unworked metal but withoutany observable change in the grain structure of the metal or any majorchange in mechanical properties. As the temperature is increased, recrys-tallisation begins to occur where the cold worked and deformed crystals arereplaced by a new set of strain-free crystals, resulting in a reduction instrength and an increase in ductility. This process will also result in a finegrain size, perhaps finer than the grain size of the metal before cold workingtook place. It is possible therefore to grain refine a metal by the correctcombination of working and heat treatment. On completion of recrystalli-sation the metal is said to be annealed with the mechanical properties ofthe non-cold-worked metal restored.
At temperatures above the recrystallisation temperature the new grainsbegin to grow in size by absorbing each other. This grain growth will resultin the formation of a coarse grained micro-structure with the grain sizedepending upon the temperature and the time of exposure. A coarse grainsize is normally regarded as being undesirable from the point of view ofboth mechanical properties and weldability.
2.2.5 Precipitation (age) hardening
Microstructures with two or more phases present possess a number of waysin which the phases can form. The geometry of the phases depends on theirrelative amounts, whether the minor phase is dispersed within the grains oris present on the grain boundaries and the size and shape of the phases. Thephases form by a process known as precipitation, which is both time andtemperature controlled and which requires a reduction in solid solubility asthe temperature falls, i.e. more of the solute can dissolve in the solvent ata high temperature than at a low temperature. A simple analogy here is saltin water – more salt can be dissolved in hot water than in cold. As the tem-perature is allowed to fall, the solution becomes saturated and crystals ofsalt begin to precipitate.
A similar effect in metals enables the microstructure of a precipitationhardenable alloy to be precisely controlled to give the desired mechanicalproperties. To precipitation or age harden an alloy the metal is first of allheated to a sufficiently high temperature that the second phase goes intosolution.The metal is then ‘rapidly’ cooled, perhaps by quenching into wateror cooling in still air – the required cooling rate depends upon the alloysystem. Most aluminium alloys are quenched in water to give a very fastcooling rate.This cooling rate must be sufficiently fast that the second phasedoes not have time to precipitate. The second phase is retained in solutionat room temperature as a super-saturated solid solution which is metastable,
16 The welding of aluminium and its alloys
that is, the second phase will precipitate, given the correct stimulus. Thisstimulus is ageing, heating the alloy to a low temperature. This allows dif-fusion of atoms to occur and an extremely fine precipitate begins to form,so fine that it is not resolvable by normal metallographic techniques. Thisprecipitate is said to be coherent, the lattice is still continuous but distortedand this confers on the alloy extremely high tensile strength. In this world,there is no such thing as a free lunch, so there is a marked drop in ductil-ity to accompany this increase in strength.
If heating is continued or the ageing takes place at too high a tempera-ture the alloy begins to overage, the precipitate coarsens, perhaps to a pointwhere it becomes metallographically visible.Tensile strength drops but duc-tility increases. If the overageing process is allowed to continue then thealloy will reach a point where its mechanical properties match those of theannealed structure.
Too slow a cooling rate will fail to retain the precipitate in solution. Itwill form on the grain boundaries as coarse particles that will have a verylimited effect on mechanical properties.The structure is that of an annealedmetal with identical mechanical properties.The heat treatment cycle and itseffects on structure are illustrated in Fig. 2.6.
Welding metallurgy 17
Alloy at solution treatment temperature.Precipitates taken into solution
Rapid cool by quenching in water
Time at ageing temperatureHeating tosolution treatmentfollowed by aslow cool
Correctly aged– fine dispersionof precipitateswithin thegrains
Overaged –coarseprecipitateswithin thegrains
2.6 Illustration of the solution treatment and age-(precipitation)hardening heat treatment cycle.
This chapter is only the briefest of introductions to the science of metals,how crystal structures affect the properties and how the fundamental mech-anisms of alloying, hardening and heat treatment, etc., are common to allmetals. Table 2.1 gives the effects of solid solution strengthening, coldworking and age hardening. It illustrates how by adding an alloying elementsuch as magnesium, the strength can be improved by solid solution alloy-ing from a proof strength of 28N/mm2 in an almost pure alloy, 1060, to 115N/mm2 in an alloy with 4.5% magnesium, the 5083 alloy. Similarly, theeffects of work hardening and age hardening can be seen in the increasesin strength in the alloys listed when their condition is altered from theannealed (O) condition. Note, however, the effect that this increase instrength has on the ductility of the alloys.
2.3 Aluminium weldability problems
2.3.1 Porosity in aluminium and its alloys
Porosity is a problem confined to the weld metal. It arises from gas dis-solved in the molten weld metal becoming trapped as it solidifies, thusforming bubbles in the solidified weld (Fig. 2.7).
Porosity can range from being extremely fine micro-porosity, to coarsepores 3 or 4mm in diameter. The culprit in the case of aluminium is hydro-gen, which has high solubility in molten aluminium but very low solubilityin the solid, as illustrated in Fig. 2.8. This shows a decrease of solubility tothe order of 20 times as solidification takes place, a drop in solubility so
18 The welding of aluminium and its alloys
Table 2.1 Summary of mechanical properties forsome aluminium alloys
1060 O 28 68 431060 H18 121 130 65083 O 155 260 145083 H34 255 325 56063 O 48 89 326063 TB(T4) 100 155 156063 TF(T6) 180 200 82024 O 75 186 202024 TB(T4) 323 468 20
UTS: ultimate tensile strength
pronounced that it is extremely difficult to produce a porosity-free weld inaluminium.
Porosity tends to be lowest in autogenous welds.When filler metal is usedporosity levels tend to increase because of contamination from the wire. Ofthe conventional fusion welding processes TIG has lower levels of porositythan MIG due to this hydrogen contamination of the wire. Increasing thearc current increases the temperature of the weld pool and therebyincreases the rate of absorption of hydrogen in the molten metal. Con-versely, in the flat welding position increasing the heat input can reduceporosity when the rate of gas evolution from the weld exceeds the rate ofabsorption – slowing the rate at which the weld freezes allows the
Welding metallurgy 19
2.7 Finely distributed porosity in TIG plate butt weld 6mm thickness.Courtesy of TWI Ltd.
300 400 500 600 700
Tm 660 °C
2.8 Solubility of hydrogen in aluminium.
hydrogen to bubble out of the weld. A similar effect can be achieved byreducing the travel speed. Increasing arc voltage and/or arc length increasesthe exposure of the molten metal to contamination, and porosity willthereby increase. The alloy composition can also influence the amount ofporosity by changing the solubility of hydrogen – magnesium in particularhas a beneficial effect. It is thought that magnesium raises the solubility andreduces absorption of hydrogen by as much as twice at 6% Mg. Copper andsilicon have the opposite effect. A conclusion that can be drawn from thisis that when porosity is encountered the use of Al-Mg filler can assist inreducing the problem.This assumes of course that such filler metal is accept-able in the specific application.
The sources of hydrogen are many and varied but one of the primarysources is the welding consumables. Moisture is an intrinsic part of the fluxin any of the flux shielded processes such as manual metallic arc (MMA)or SMA (shielded metal arc), and submerged arc (SA) welding. Duringwelding this moisture decomposes in the arc to give hydrogen, resulting ina large amount of porosity. This is one reason why these processes are notwidely used to weld aluminium.
The gas used in the gas shielded processes is another source of moisturewhich is easy to overlook. Ideally gas with a dew point of less than -50°C (39ppm water) should be used. To achieve such a high purity it is essential topurchase the gas with a guaranteed low dew point. It is also necessary to ensure that when it is delivered to the weld pool it has maintained thishigh degree of purity. This means that the gas supply system should bechecked at regular intervals for leaks, that damaged hoses are replacedimmediately and joints are sound. When faced with a porosity problem thegas purity should be checked first of all at the torch nozzle before workingback along the gas delivery system in a logical manner to locate the sourceof contamination. If the workshop layout permits it is recommended that thegas is supplied from a bulk tank rather than from cylinders and distributedaround the workplace in copper or steel piping. Despite the best efforts ofthe gas suppliers it is not always possible to guarantee completely the purityof individual bottles except at great expense. Bulk supplies are generally ofsuperior quality.Screwed or bolted flanged connections are potential sourcesof contamination and leaks and are best avoided by the use of a brazed orwelded system.
A further source of contamination may come from the gas hoses them-selves. Many of the plastics used for gas hoses are porous to the waterpresent in the air. This results in moisture condensing on the inside of thehose and being entrained in the shield gas. A number of reports publishedrecently have identified the permeability of hose compositions and asummary of the results is presented in Table 2.2. From this it can be seenthat only a limited number of hose compositions will maintain gas purity.
20 The welding of aluminium and its alloys
Of the plastic tubing the most porous is neoprene rubber, the least porouspolytrifluoro-chloroethylene. The best of all is an all-metal system. Anyplastic hoses should be kept as short and as small a diameter as possibleconsistent with the application.
Also important is the fact that the moisture collects in the tube over aperiod of time when no gas is flowing. The implication of this is that ifwelding equipment is left idle for long periods of time the first few weldsto be made on recommencing welding may contain unacceptable porosity.A systematic porosity problem always occurring, for example, at the com-mencement of the first shift after a weekend break may be an indication ofthis problem. Flushing the hoses through for a short time by operating thetorch trigger may help to reduce the amount of porosity. If this is done withthe MIG (GMAW, gas metal-arc welding) torch do not forget to slacken offthe wire drive rolls!
TIG welding wire should be cleaned with a lint-free cloth and a gooddegreasant before use. Once the wire has been cleaned do not handle thewire with bare hands but use a clean pair of gloves, store the wire in cleanconditions and weld within a short time of cleaning. For the MIG processthere are devices available that can be fitted around the wire where it entersthe torch liner in the wire feed unit and that will clean the wire as it passesthrough. Best of all the wire should be shaved to remove any contaminantsand oxides that may have been pressed into the surface during the wiredrawing operation.
Cleanliness of the parent metal is also extremely important in achievinglow levels of porosity – it cannot be emphasised too strongly how impor-tant this is. Thorough degreasing is essential, followed by a mechanicalcleaning such as stainless steel wire brushing to remove the oxide layerwhich may be hydrated. Once degreased and wire brushed the parent mate-rial should be welded within a short period of time, a period of four hoursfrequently being regarded as acceptable. Further details of mechanicalcleaning, degreasing and workshop conditions are given in Chapter 4.
A last source of porosity may be hydrogen dissolved within the alu-minium. Although solubility of hydrogen is low in the solid phase there canbe sufficient in the parent metal to give a problem on welding. This isunlikely in wrought products but may arise when welding castings or sin-tered products. For this reason some purchasers specify in their purchaseorders a limit on hydrogen, typically 2ppm. Avoidance of porosity whenhydrogen is present in the parent metal is impossible to avoid.
Table 2.3 summarises the causes and prevention of porosity.
2.3.2 Oxide film removal during welding
The need to remove the oxide film prior to welding to reduce the risk ofporosity has been covered above. It is also necessary to disperse this film
22 The welding of aluminium and its alloys
Table 2.3 Summary of causes and prevention of porosity
Mechanism of Potential causes Remedial measuresporosity formation
Hydrogen Oxide film, grease, drawing soap Clean wire, use high-entrapment on filler wire; oxides, grease, quality gas, change
dirt on parent plate; dirt/grease liner, protect wirein liner; contaminated shield from contamination,gas; water leaks in torch; spatter change torch, cleanon weld face. plate, minimise
spatter.Gas/air (a) Weld pool turbulence due to (a) Use lower
entrapment high current. current, reduce(b) Gas expanding from root of travel speed,
(b) Use full penweld, allow gapin fillet weldroot, use highheat input.
Rapid freezing Heat input too low, rapid heat Increase current,trapping gas loss, viscous weld pool, cold slow travel speed,
backing bar. consider preheat,heat backing bar,replace argon shieldgas with helium.
Erratic wire feed Kinked, blocked or wrong size Straighten wireliner, incorrect or badly adjusted conduit, replacedrive rolls, damaged contact tip, contact tip, adjustunstable power supply. drive roll pressure,
fit correct liner, fitgrooved rolls.
during welding if defects such as lack of fusion and oxide film entrapmentare to be avoided. Figure 2.9 illustrates oxide filming in a fillet weld thatwill obviously have a pronounced effect on joint strength.
Aluminium oxide (Al2O3) is a very tenacious and rapid-forming oxidewhich gives aluminium its excellent corrosion resistance. Aluminium oxidehas a very high melting point, 2060°C compared with the pure metal which melts at 660°C. The oxides of most other metals melt at tempera-tures at or below that of their metals and during welding will float on top of the weld pool as a molten slag. Heating aluminium to its meltingpoint without dispersing the oxide film will result in a molten pool of aluminium enclosed in a skin of oxide, rather like a rubber toy balloon filled with water. This skin has to be removed by some suitable means.With fluxed processes, soldering, brazing, MMA and SA welding, the fluxneeds to be very aggressive to dissolve the film. Failure to remove thesefluxes on completion can give rise to service failures from corrosion and, inaddition to porosity, is a further reason why MMA and SA welding arerarely used.
Fortunately, in gas shielded arc welding there is a phenomenon known ascathodic cleaning which can be employed to give the desired result. Whenthe electrode is connected to the positive pole of the power source anddirect current is passed there is a flow of electrons from the workpiece tothe electrode with ions travelling in the opposite direction and bombard-ing the workpiece surface. This ion bombardment breaks up and dispersesthe oxide film and permits the weld metal to flow and fuse with the parentmetal. The MIG welding process uses only DC electrode positive (DCEP)current – using DC electrode negative (DCEN) results in an unstable arc,
Welding metallurgy 23
2.9 Oxide entrapment in fillet weld. Courtesy of Roland Andrews.
erratic metal transfer and poor weld quality. Oxide film removal is there-fore an intrinsic part of the MIG process.
TIG welding, on the other hand, conventionally uses DCEN, which, ifused on aluminium, can result in poor weld quality. Using DCEP with TIG,however, results in the tungsten electrode overheating as some 60–70% ofthe heat generated in a TIG welding arc may be produced at the positivepole. (Conventionally a rule of thumb for the heat balance in a TIG arc isregarded as being two-thirds at the positive pole, one-third at the negativepole. This, however, varies widely depending upon the shield gas, current,arc length, etc.) This can cause melting of the electrode and bring thewelding operation to a premature end. A compromise is therefore reachedby using AC where oxide film removal takes place on the positive half cycleand electrode cooling on the negative half cycle as illustrated in Fig. 2.10.TIG welding of aluminium is therefore normally carried out with AC,although there are a couple of techniques that use either DCEP or DCEN.These will be discussed in Chapter 6 on TIG welding.
2.3.4 Hot cracking
Hot cracking is a welding problem that does not occur in pure metals butmay be found in certain alloy systems. It is not confined to the aluminiumalloys but is also encountered in steels, nickel and copper alloys. The funda-
24 The welding of aluminium and its alloys
TIGDC – ve
DC + veTIGAC
IONS ELECTRONS IONS
2/3 Heat 1/3 Heat 1/2 Heat+ve 1/2 Cycle
–ve 1/2 Cycle
2.10 Effect of polarity on cathodic cleaning and heat balance.
mental mechanism is the same in all of the alloy systems and is a function of how metal alloy systems solidify. As the name suggests, this is a high-temperature cracking mechanism which, because of its prevalence, is knownby a number of different names – hot cracking, hot fissuring, hot shortness,liquation cracking, centre-line cracking or solidification cracking.
The addition of alloying elements to a pure metal will cause a change inthe freezing temperature of the alloy from that of the pure metal and mayresult in a number of different phases – a solid solution, a eutectic and anintermetallic compound, for instance, being produced. These changes ofstate and the relative proportions of each phase are represented on phasediagrams. It is not intended to go into any greater detail than this – forfurther information refer to the books listed in the Bibliography.The lowestmelting point composition of the alloy is known as the eutectic compositionwhich freezes at one specific temperature. The other non-eutectic compo-sitions freeze over a range.
It is necessary next to look at how a metal solidifies. Figure 2.11 showsthe way in which the lowest melting point constituents are pushed to thegrain boundaries by the solidification fronts as the solid particles grow insize.
The first solid to form is a unit cell that acts as a nucleus to which atomsattach themselves, forming what is known as a dendrite. The dendriteincreases in size until such time as it begins to collide with its neighboursthat have been nucleating and growing in a similar manner. The point atwhich this collision takes place becomes the boundary between adjacentdendrites, crystals or grains – the grain boundary. Since almost all alloysystems, except eutectics, solidify over a range of temperatures, it is commonsense to expect that the first metal to solidify will be the highestmelting/freezing point alloy and the last to be the lowest melting point com-position, always the eutectic if one has formed. The consequence of thissolidification process is that the lowest melting point alloy composition ispushed ahead of the solidifying dendrite until it becomes trapped betweenthe adjacent dendrites, i.e. along the grain boundaries. If the difference inmelting point between the low melting point eutectic and the bulk of themetal is sufficiently great then the liquid film along the grain boundariesmay part as the metal cools and contracts. The results of this are illustratedin Fig. 2.12.
In most metals this effect is caused by tramp elements or impurities.Sulphur in steel and nickel alloys is a good example where low melting pointsulphide eutectics are formed. In the aluminium alloys, however, it is thedeliberately added alloying elements themselves that form a range of eutec-tics with freezing points substantially lower than the bulk metal.This meansthat all aluminium alloys are susceptible to some degree to this form ofcracking, differing only in their degree of susceptibility. Cracking tests have
Welding metallurgy 25
First solidto form
Increasingarea of solid
Increasing amounts of solid phase
Small amounts of liquid surroundinglarge islands of solid
Small amount of lowest melting point liquid along the grain boundaries
Note that a largedifference in melting pointbetween the bulk of themetal and the ‘low’melting point films resultsin an increased sensitivityto hot or solidificationcracking
2.11 Solidification of a metal.
determined what is termed the hot short range, the range of compositionwithin which the alloy has a high risk of hot cracking. The hot short rangeof the common alloying elements is given in Table 2.4.
These results are produced by performing standard cracking tests. Thesetests are designed to load the weld transversely under controlled conditionsto give cracks, the length of which will be a measure of the crack sensitiv-ity of the specific alloy being tested. This enables the alloys to be ranked inorder of sensitivity and characteristics such as the hot short range to bedetermined.
Welding metallurgy 27
2.12 Solidification cracking: (a) in the finish crater of a TIG weld inA5083 alloy; (b) in a 3mm thick A6082 plate/4043 filler metal TIG weld.Courtesy of TWI Ltd.
The aluminium alloys all exhibit a peak in sensitivity with a high resis-tance to hot cracking at both low and high alloy content, as shown in Fig. 2.13. At low levels of alloy content there is only a small amount of eutectic present.This results in the liquid film on the grain boundaries being
28 The welding of aluminium and its alloys
Table 2.4 Hot short range and eutectic characteristics
Alloy system Hot short range Eutecticcomposition %
Temp. (°C) Composition (%)
Al-Si 0.5 to 1.2 577 12.6Al-Cu 2.0 to 4.0 548 33Al-Mn 1.5 to 2.5 658 1.5Al-Mg 0.5 to 2.5 450 36Al-Zn 4.0 to 5.0 381 94Al-Fe 1.0 to 1.5 655 2Al-Li Not available 596 7.5Al-Ni Not available 640 5.7
0 1 2 3 4 5 6
Percentage of alloying element
2.13 Effect of solute concentration on crack sensitivity.
either discontinuous or very thin. The strength of a liquid film can bederived from
where F = force required to tear the liquid;k = a constant;g = the liquid/solid interfacial tension;A = cross-sectional area;t = liquid film thickness.
Therefore, as the liquid film thickness t increases, the force required to tearthe film F reduces. The force required for cracking begins to increase,however, once there is sufficient eutectic available that it can begin to flowinto and fill any cracks that form. The crack sensitivity therefore drops, thecracks heal themselves and a crack-free structure results. This is a veryuseful feature when welding alloys that are sensitive to liquation crackingin the HAZ. Figure 2.14 illustrates this graphically, where it can be seen thatthe shape of the curve is essentially the same as that in Fig. 2.13.
The practical consequence of this is that the crack susceptibility of theweld metal is very sensitive to changes in composition. In very many situ-ations when welding aluminium alloys, the filler metal does not match theparent material. It is most important that this fact is realised and thataccount is taken of the composition of the resultant weld metal. There area number of other factors, apart from filler metal and parent metal com-position, which affect the weld metal composition. Fit-up of the componentparts can affect the amount of dilution in a joint, dilution being the amountof parent metal dissolved into the weld metal during welding. In the rootpass a wide gap will give low dilution, a narrow gap high dilution, as illus-trated in Fig. 2.15.
Back filling ofdefects due to largeamount of eutectic
2.14 Generalised picture of crack sensitivity.
A steep weld preparation bevel angle will give lower dilution than a wideshallow weld preparation because of the change in the angle of the elec-trode to the weld bevel, as shown in Fig. 2.16. Changing the welding processor the welding parameters, particularly the welding current, may also affectpenetration and therefore dilution. From a shop-floor point of view thismeans that weld bevel angles, joint fit up and welding parameters need tobe controlled far more closely than in the case of steel welding if problemsof hot cracking are to be avoided.
In summary, if hot cracking is encountered it may be eliminated by oneor more of the following:
• A small grain size. It has been found that small additions of elementssuch as titanium, zirconium or scandium will act as nuclei for the for-mation of a very fine grain during solidification. Filler metals can be pur-chased that are alloyed with titanium and/or zirconium.
• Control the composition of the weld pool by adding filler metal toproduce an alloy that is not in the hot short range.
• Use an edge preparation and joint spacing to permit sufficient fillermetal to be added to achieve a weld metal composition outside the hotshort range.
• Use the highest welding speed. High speeds reduce the length of timethe weld is within the hot short temperature range. High welding speeds
30 The welding of aluminium and its alloys
Small gap – high dilution
Large gap – low dilution
2.15 Effect of variations in root gap.
Weld preparationsurface Deep
2.16 Effect of electrode angle on dilution.
also reduce the size of the HAZ and consequently the shrinkage stressesacross the joint.
• Use high-speed, small-volume multi-run procedures instead of largevolume, single run deposits.
• Select welding and assembly sequences that minimise restraint andresidual stresses.
• Apply an external force to maintain the weld in compression while it isin the hot short range.
• Select a filler metal with a melting point close to that of the parent metal,see Appendixes C and D.
2.4 Strength loss due to welding
In order to effect a weld the components to be joined are heated to a hightemperature, in the case of fusion welding above the melting point of theparent metals, and brought together to enable the components to coalesce.The heat of the welding operation is conducted into the parent metal suchthat in any welded joint there are three distinct areas – the weld metal ina fusion welded joint, the HAZ in the parent material and the unaffectedparent metal. The HAZ may be further subdivided into areas with partic-ular properties depending upon the alloy system involved. Since the HAZwill have experienced one or more cycles of heating and cooling the prop-erties may be radically different from those of the unaffected parent metal.This is particularly the case with those aluminium alloys that have beenstrengthened by either cold working or precipitation hardening. One aspectof this is the width of the HAZ, a function of the high thermal conductiv-ity of aluminium and the consequent size of the area where there has beena substantial loss of strength.Only when the alloy is in the as-cast or annealedcondition will the properties of the HAZ match those of the parent metal.
2.4.1 Weld metal
In a fusion weld the weld metal is an as-cast structure consisting of amixture of the filler metal, if added, and the parent metal(s). The proper-ties of this weld depend upon the composition, the quality and the grainsize of the deposit. These in their turn depend on the parent and filler metalcompositions, the amount of dilution, the quality of the welding process andthe welder and, lastly, the rate of solidification. With the exception of acouple of 2XXX filler wires most filler metals available are not capable ofbeing age hardened, although dilution with parent metal may enable someage hardening to take place. Fast solidification rates will give a finer grainsize and hence better mechanical properties than slow solidification rates.Small weld beads therefore generally have better properties than large weld
Welding metallurgy 31
beads and a higher resistance to hot cracking. In the root pass, however, asmall cross-section weld bead may increase the risk as it will be required tocarry the contractional stresses and restraint.
There is very little that can be done to improve the properties of the weldmetal. Solid solution strengthening can be useful and the selection of theappropriate filler metal can significantly contribute to a high weld metalstrength.As a general rule the weld metal will match the parent metal prop-erties only when the parent metal itself is in either the as-cast or annealedcondition. Where cold work has been used to increase the strength of theparent metal it is not practicable to match these by cold working the weld.The lower strength in the weld metal must therefore be accepted and com-pensated for in the design. With some of the precipitation-hardening alloysa post-weld ageing treatment can be carried out to increase the strength ofthe weld metal, provided that the weld metal contains those alloying ele-ments which will give precipitation hardening as mentioned above. Theeffectiveness of this heat treatment will depend upon the filler metal com-position and dilution. For example, a single pass AC-TIG weld in a 6061series alloy made with a 4043 filler metal will give an ultimate tensilestrength of around 300N/mm2 in the post-weld aged condition, a multi-passMIG weld made with a 4043 filler will give approximately 230N/mm2.Changing the 4043 filler to a 4643, which contains only 0.2% of magnesium,will improve the strength after post-weld ageing to match that of the auto-genous AC-TIG weld. This is a further example of the importance of thecorrect selection of filler metals and the control of consistency duringwelding of the aluminium alloys.
2.4.2 Heat affected zone
As mentioned earlier, alloys in the as-cast or annealed condition may bewelded without any significant loss of strength in the HAZ, the strength ofthe weldment matching that of the parent metal. Where the alloy has hadits strength enhanced by cold work or precipitation hardening then theremay be a substantial loss of strength in the HAZ.
The cold worked alloys will experience a loss of strength due to recrys-tallisation in the HAZ. Recrystallisation begins to take place when the tem-perature in the HAZ exceeds 200°C and progressively increases with fullannealing taking place over 300°C as illustrated in Fig. 2.17. This shows a1XXX alloy cold worked to different amounts and heat treated at a rangeof temperatures, showing how the annealing heat treatment results in amajor loss of strength. The result of this in practice is illustrated in Fig. 2.18which shows a 5XXX alloy TIG welded.
A similar picture can be seen in the heat-treatable alloys. The situationhere is somewhat more complex than with the work-hardened alloys but
32 The welding of aluminium and its alloys
Welding metallurgy 33
100 150 200 250 300 350 Temperature, ∞C
Cold work 80 60 40 20
2.17 Effect of annealing temperature on cold work and strength.
75 50 25 0Distance from centre of weld (mm)
25 50 75
Hardness andstrength of weldmetal
Hardness andstrength of work-hardened alloy
Hardness andstrength ofHAZ
2.18 Effect of welding on strength in cold worked alloy.
similar losses in tensile strength can be found. The loss is caused by a dis-solution of the precipitates in the 2XXX series alloys and a coarsening oroverageing of the precipitates in the 6XXX and 7XXX alloys. These effectsare illustrated in Fig. 2.19. Greater detail on these effects for individualalloys can be found in Chapter 3.
One last comment is the potential for the loss of alloying elements fromthe weld pool that may result in a reduction in strength. It is true that someelements, mainly magnesium with its low boiling point and lithium which ishighly reactive with oxygen, may be lost or oxidised during welding. Thereis, however, a dearth of information quantifying any effects, which suggeststhat it is not perceived as being a problem. Loss of magnesium is worst whenMIG welding, resulting in the sooty deposit occasionally seen along theweld toes but in this case, and in the case of lithium, careful attention to gasshielding will minimise any problem.
34 The welding of aluminium and its alloys
30 20 10 0Distance from centre of weld (mm)
10 20 30
Hardness andstrength of weldmetal
Hardness andstrength of fullyage-hardenedalloy
Hardness andstrength in theHAZ
2.19 Effect of welding on 6061 T6 age-hardened alloy – as welded.
3.1 Designation criteria
Aluminium alloys may be divided into two broad classes, cast and wroughtproducts. These two classes can be further subdivided into families of alloysbased on chemical composition and finally on temper designation. Temperdesignations are used to identify the condition of the alloy, in other wordsthe amount of cold work the alloy has undergone or its heat treatment con-dition. There are a number of schemes available for identification of thealloy and its condition. In this book the numeric method adopted by theEuropean Committee for Standardisation (CEN) will be used as standard.This system uses four digits to identify the wrought alloys and five digits to identify the cast alloys, and is broadly the same as the ISO and US nu-merical methods of identification where a four digit number identifies theunique alloy composition. This is in agreement with the recommendationmade in the early 1970s for an International Designation System issued bythe Aluminum Association in the USA. The chemical composition limitsspecified in the CEN specifications are identical with those registered withthe Aluminum Association for the equivalent alloys. This should simplifythe sourcing of alloys and remove the confusion that can surround the iden-tification of specific grades. One perennial problem for the welding engi-neer is the use of superseded specification designations to identify alloycompositions. As an aid to identification a table of comparative specifica-tion designations is included as Appendices C and D.
3.2 Alloying elements
The principal alloying elements are copper, silicon, manganese, magnesium,lithium and zinc. Elements such as nickel, chromium, titanium, zirconiumand scandium may be added in small amounts to achieve specific proper-ties. Other elements may also be present in small amounts as unwantedimpurities. These elements, known as tramp or residual elements, have no
3Material standards, designations and alloys
36 The welding of aluminium and its alloys
beneficial effects on mechanical properties and the aluminium producersattempt to eliminate these from their products. The main effects of thealloying elements are as follows:
• Magnesium (Mg) increases strength through solid solution strengthen-ing and improves work hardening ability.
• Manganese (Mn) increases strength through solid solution strengthen-ing and improves work hardening ability.
• Copper (Cu) gives substantial increases in strength, permits precipita-tion hardening, reduces corrosion resistance, ductility and weldability.
• Silicon (Si) increases strength and ductility, in combination with mag-nesium produces precipitation hardening.
• Zinc (Zn) substantially increases strength, permits precipitation hard-ening, can cause stress corrosion.
• Iron (Fe) increases strength of pure aluminium, generally residualelement.
• Chromium (Cr) increases stress corrosion resistance.• Nickel (Ni) improves elevated temperature strength.• Titanium (Ti) used as a grain-refining element, particularly in filler
metals.• Zirconium (Zr) used as a grain-refining element, particularly in filler
metals.• Lithium (Li) substantially increases strength and Young’s modulus,
provides precipitation hardening, decreases density.• Scandium (Sc) substantially increases strength by age hardening, grain-
refining element particularly in weld metal.• Lead (Pb) and bismuth (Bi) assist chip formation in free machining
3.3 CEN designation system
3.3.1 Alloy composition identification
A full listing of all of the British and European specifications dealing withany aspect of aluminium alloys, product forms, supply conditions andwelding is given in Appendix A at the end of the book.
There are two methods in the CEN system for identifying aluminiumalloys, one based on the numerical designation adopted by ISO and as recommended by the Aluminum Association, the other on the basis ofchemical composition. The details of the European system are contained in the specification BS EN 573. This is divided into four parts as follows:
• Part 1 Numerical Designation System.• Part 2 Chemical Symbol Based Designation System.
Material standards, designations and alloys 37
• Part 3 Writing Rules for Chemical Composition.• Part 4 Form of Products.
In the European system the prefix ‘AB’ denotes ingots for remelting, ‘AC’denotes a cast product, ‘AM’ a cast master alloy, the prefix ‘AW’ a wroughtproduct. For the wrought alloys this is followed by the four digit numberwhich uniquely identifies the alloy. The first digit indicates the main alloy-ing element, with numbers 1 to 9 being used as follows:
• AW 1XXX – commercially pure aluminium.• AW 2XXX – aluminium–copper alloys.• AW 3XXX – aluminium–manganese alloys.• AW 4XXX – aluminium–silicon alloys.• AW 5XXX – aluminium–magnesium alloys.• AW 6XXX – aluminium–magnesium–silicon alloys.• AW 7XXX – aluminium–zinc–magnesium alloys.• AW 8XXX – other elements e.g. lithium, iron.• AW 9XXX – no alloy groups assigned.
Except in the case of the commercially pure aluminium alloys, the last threedigits are purely arbitrary and simply identify the specific alloy. In the caseof the pure aluminium, however, the last two digits indicate the minimumpercentage aluminium in the product to the nearest 0.01%, e.g. AW-1098-99.98% Al, AW-1090-99.90% Al. The second digit gives the degree ofcontrol on impurities: a zero indicates natural impurity limits, a figurebetween 1 and 9 that there is special control of one or more of the indi-vidual impurities or alloying elements.
There are a total of 36 separate compositions of casting alloys, dividedinto 11 subsections as follows. It is worth mentioning that 29 of the alloysare based on the Al-Si system.
• AC 2 1 XXX – Al Cu.• AC 4 1 XXX – Al SiMgTi.• AC 4 2 XXX – Al Si7Mg.• AC 4 3 XXX – Al Si10Mg.• AC 4 4 XXX – Al Si.• AC 4 5 XXX – Al Si5Cu.• AC 4 6 XXX – Al Si9Cu.• AC 4 7 XXX – Al Si(Cu).• AC 4 8 XXX – Al SiCuNiMg.• AC 5 1 XXX – Al Mg.• AC 7 1 XXX – Al ZnMg.
As with the wrought alloys the third and fourth digits identify the specificalloy in the group and are arbitrary.
Master alloys, which will not concern the shop-floor welding engineer,are identified with the prefix ‘AM’ followed by the number ‘9’, the secondand third figures are the atomic number of the main alloying element,e.g. 14 for silicon, 29 for copper, the last two digits being chronological and issued in the order of registration of the alloy. For example, an aluminium–silicon master alloy could carry the designation AM 91404,identifying the alloy as being the fourth Al-Si alloy to be registered.
3.3.2 Temper designations
The mechanical properties of the alloys are affected not only by their chemical composition but also by their condition, e.g. annealed, coldworked, precipitation hardened. It is obviously important that this condi-tion is clearly and unequivocally identified for both the designer and thewelding engineer. To do this CEN has developed a system of suffixes thatidentify the amount of strain hardening the alloy has undergone or its heattreatment condition. There are five basic designations identified by a singleletter which may be followed by one or more numbers to identify theprecise condition.
The basic designations are as follows:
• F – as fabricated. This applies to wrought products where there is nocontrol of the amount of strain hardening or the thermal treatments.There are no mechanical properties specified for this condition.
• O – annealed. This is for products that are annealed to produce thelowest strength. There may be a suffix to indicate the specific heat treatment.
• H – strain hardened (cold worked). The letter ‘H’ is always followed byat least two digits to identify the amount of cold work and any heattreatments that have been carried out to achieve the required mechani-cal properties.
• W – solution heat treated. This is applied to alloys which precipitationharden at room temperature (natural ageing) after a solution heat treat-ment. It is followed by a time indicating the natural ageing period, e.g.W 1h.
• T – thermally treated. This identifies the alloys that are aged to producea stable condition. The ‘T’ is always followed by one or more numbersto identify the specific heat treatment.
The first digit after ‘H’ identifies the basic condition:
• H1 – strain hardened only.• H2 – strain hardened and partially annealed. This applies to the alloys
that are hardened more than is required and that are then annealed at
38 The welding of aluminium and its alloys
Material standards, designations and alloys 39
a low temperature to soften them to the required degree of hardnessand strength.
• H3 – strain hardened and stabilised. Stabilisation is a low-temperatureheat treatment applied during or on completion of fabrication. Thisimproves ductility and stabilises the properties of those strain-hardenedalloys that soften with time.
• H4 – strain hardened and painted. This is for alloys that may be sub-jected to low-temperature heat treatment as part of a paint baking oradhesive curing operation.
The second digit after ‘H’ indicates the amount of strain hardening in thealloy. H18 is strain hardened only and in the most heavily cold worked con-dition. It is therefore the hardest and highest strength condition. Ductilitywill be very low and further cold work may cause the component to crack.Intermediate conditions are identified by the numbers 1 to 7 and are basedon the strength relative to that of the annealed alloy, O condition and theH18 condition, e.g. an H14 alloy will have a strength halfway between theannealed and fully hard condition, H12 halfway between O and H14. Thereis an H9 condition in which the ultimate tensile strength exceeds that of theH8 condition by a minimum of 10N/mm2.
The third digit after ‘H’ is not mandatory and is used when the alloyrequires special control to achieve the specific temper identified by thesecond digit or when some other characteristic of the alloy is affected.Examples of such characteristics are exfoliation corrosion resistance, seamwelded tube or additional working after the final temper has been achieved,e.g. by embossing.
The ‘T’ designations are applied to those alloys that are age hardened,the first digit identifying the basic heat treatment:
• T1 – cooled from an elevated temperature-shaping treatment and naturally aged.
• T2 – cooled from an elevated temperature-shaping process, cold workedand naturally aged.
• T3 – solution heat treated, cold worked and naturally aged.• T4 – solution heat treated and naturally aged.• T5 – cooled from an elevated temperature-shaping process and artifi-
cially aged.• T6 – solution heat treated and artificially aged.• T7 – solution heat treated and overaged or stabilised.• T8 – solution heat treated, cold worked and artificially aged.• T9 – solution heat treated, artificially aged and cold worked.
More digits may be added to the designation to indicate variations in heattreatments or cold work. For example, TX51, 510, 511, 52 or 54 all indicate
those alloys that are stress relieved after heat treatment by some form ofcold working such as stretching or restriking cold in the finish die. Theseadditional digits are also used to indicate the temper condition of thosealloys designated ‘W’.
The T7, artificially aged, temper designation may be supplemented by a second digit to indicate if the alloy is overaged and by how much. Othernumbers are used to identify underaged conditions and increasing degreesof cold work etc.
The full details of these designations are contained in the specificationEN 515 ‘Aluminium and Aluminium Alloys – Wrought Products – TemperDesignations’.
3.4 Specific alloy metallurgy
3.4.1 Non-heat treatable alloys
188.8.131.52 Pure aluminium (1XXX series)
The principal impurities in ‘pure’ aluminium are silicon and iron, residualelements remaining from the smelting process. Copper, manganese and zincmay also be present in small amounts. The maximum impurity levels varywith the specified purity, e.g. 1098 (Al99.98) contains a maximum impuritycontent of 0.02%, comprising 0.010% Si max., 0.006% Fe max., 0.0035% Cumax. and 0.015% Zn max. The 1050 (Al99.5) alloy contains a maximum of0.05% of impurities. In the high-purity grades of these alloys the impuritiesare in such low concentrations that they are completely dissolved. From thewelding viewpoint the alloys can be regarded as having no freezing rangeand a single phase microstructure which is unaffected by the heat ofwelding. The less pure alloys such as 1200 (Al99.0) can dissolve only smallamounts of the impurity elements and, as the metal freezes, most of the ironcomes out of solution to form the intermetallic compound FeAl3. Whensilicon is present in more than trace quantities, a ternary or three-elementcompound, Al-Fe-Si phase, is formed. With higher silicon contents freeprimary silicon is formed. All of these phases contribute to an increase instrength, attributed to slight solution hardening and by a dispersion of thephases.
The effects of welding on the structure of a fusion welded butt joint inan annealed low-purity aluminium such as 1200 is to produce three distinctzones. The unaffected parent material will have a fine-grained structure ofwrought metal with finely dispersed particles of Fe-Al-Si. The heat affectedzones show no significant change in microstructure except close to thefusion boundary where partial melting of the low melting point constituentsalong the grain boundaries occurs, leaving minute intergranular shrinkage
40 The welding of aluminium and its alloys
Material standards, designations and alloys 41
cavities that result in a slight loss of strength. There will also be a loss ofstrength in the cold work alloys where the structure has been annealed andsoftened. The weld metal has an as-cast structure. When the filler metal hasthe same nominal composition as the parent metal the low melting pointconstituents such as Fe-Al-Si are the last to solidify and will be located atthe grain boundaries.
184.108.40.206 Aluminium–manganese alloys (3XXX series)
When iron is present as an impurity the solubility of manganese in alu-minium is very low. The rate of cooling from casting or welding is suffi-ciently rapid for some manganese to be left in supersaturated solution.Further processing to provide a wrought product causes the manganese toprecipitate as FeMnAl6, this precipitate giving an increase in strength dueto dispersion hardening. Any uncombined iron and silicon impurities maybe present as an insoluble Al-Fe-Mn-Si phase.
The weld zones are similar to those seen in pure aluminium, the onlymajor difference being the composition of the precipitates. The heat ofwelding has the same effect on the structure as on pure aluminium, withthe precipitates arranged along the grain boundaries and a loss of strengthin the annealed regions of cold worked alloys.
The 3103 (AlMn1)alloy is more hot short (see Section 2.5) than pure alu-minium, despite having a similar freezing range. In practice, however, hotcracking is rarely encountered. Those alloys containing copper (alloy 3003)or magnesium (alloys 3004, 3005 and 3105) are more sensitive to hot crack-ing. Weld cracking may be sometimes encountered when autogenouswelding but this is easily prevented by the use of an appropriate filler metalcomposition.
220.127.116.11 Aluminium–silicon alloys (4XXX series)
The aluminium silicon alloys form a binary eutectic at 11.7% silicon with amelting point of 577°C, the two phases being solid solutions of silicon inaluminium, 0.8% maximum at room temperature, and aluminium in silicon.There are no intermetallic compounds. Sodium may be added in smallamounts to refine the eutectic and increase the strength by improved dis-persion hardening. Iron, even in small amounts, can seriously degradetoughness although manganese may be added to reduce this effect.
The 4XXX series has very high fluidity and is extensively used for castingpurposes, often being alloyed with copper and magnesium to provide somedegree of precipitation hardening and with nickel to improve high temper-ature properties. Because of its high fluidity and low sensitivity to hot short-ness it is commonly used as a weld filler metal.
18.104.22.168 Aluminium–magnesium alloys (5XXX series)
Up to about 5% magnesium can be dissolved in aluminium to provide asubstantial amount of solid solution strengthening: the higher the magne-sium content, the higher the strength. The amount of magnesium that canbe dissolved under equilibrium conditions at ambient temperature is onlysome 1.4%, meaning that there is always a tendency for the magnesium tocome out of solution when the higher magnesium content alloys are heatedand slowly cooled. This reaction is very sluggish and welding processes donot cause any appreciable change in the microstructure except in the coldworked alloys where mechanical strength will be reduced.
The standard aluminium–magnesium alloys have iron and silicon asimpurities and deliberate additions of around 0.4–0.7% of manganese toincrease strength further, mainly by dispersion hardening. Chromium maybe added in place of or in addition to manganese to achieve the samestrength increase, 0.2% chromium being equivalent to 0.4% manganese.The iron forms FeMnAl6; the silicon combines with magnesium to formmagnesium silicide, Mg2Si, most of which is insoluble.
The magnesium alloys may all have their microstructure changed by theheat of welding. The microstructure of a butt weld in 5083 (AlMg4.5Mn0.7)in the annealed condition, welded with a 5356 filler shows the following fea-tures. The parent metal will have a fine-grained structure composed of amatrix of a solid solution of magnesium in aluminium, dispersion strength-ened with a fine precipitate of the compound Mg2Al3 together with coarserparticles of Al-Fe-Si-Mn. In the HAZ where the temperature has beenraised to around 250°C further Mg2Al3 will be formed which may begin tocoalesce and coarsen. Where temperatures begin to approach 400°C someof the Mg2Al3 will be redissolved and closer to the weld, where tempera-tures are above 560°C, partial melting occurs, causing some shrinkage cavitation. The weld metal is an as-cast structure of a supersaturated solu-tion of magnesium in aluminium with particles of the insoluble inter-metallics such as Mg2Si. The cooling rates of the weld metal are generallyfast enough to prevent the precipitation of Mg2Al3.
The strength of aluminium–magnesium weld metal is generally close to that of the annealed wrought parent metal of the same composition andit is not difficult to achieve joint strengths at least equal to the annealedcondition. Butt joints in parent metal with more than 4% magnesium sometimes show joint strengths less than that of the annealed parent alloy.In MIG welding this may be due to the loss of magnesium in the arc and it may be advisable to use a more highly alloyed filler such as 5556(AlMg5.2Cr).
5083 is normally welded with a filler metal of similar composition becausethe higher magnesium contents increase the risk of stress corrosion
42 The welding of aluminium and its alloys
Material standards, designations and alloys 43
cracking. A continuous network of Mg2Al3 along the grain boundaries maymake the alloy sensitive to stress corrosion in the form of intergranular cor-rosion. The alloy can be sensitised by prolonged exposure to temperaturesabove 80°C. In service at or above this temperature in mildly corrosiveenvironments the magnesium content should be limited to a maximum of3%. Alloys for service in these conditions are generally of the 5251 or 5454type, welded with a 5554 (AlMg3) filler metal. In multi-pass double-sidedwelds a 5% Mg filler may be used for the root passes to reduce the risk ofhot cracking, followed by 5554 filler for the filling and capping passes.
The 5XXX alloys containing between 1% and 2.5% magnesium may besusceptible to hot cracking if welded autogenously or with filler metal of a matching composition. The solution is to use more highly alloyed fillermetal containing more than 3.5% magnesium.
3.4.2 Heat-treatable alloys
22.214.171.124 Aluminium–copper alloys (2XXX series)
The aluminium–copper alloys are composed of a solid solution of copperin aluminium which gives an increase in strength, but the bulk of thestrength increase is caused by the formation of a precipitate of copper alu-minide CuAl2. To gain the full benefits of this precipitate it should bepresent as a finely and evenly distributed submicroscopic precipitate withinthe grains, achieved by solution treatment followed by a carefully controlledageing heat treatment. In the annealed condition a coarse precipitate formsalong the grain boundaries and in the overaged condition the submicro-scopic precipitates coarsen. In both cases the strength of the alloy is lessthan that of the correctly aged condition.
The early aluminium–copper alloys contained some 2–4% of copper.Thiscomposition resulted in the alloys being extremely sensitive to hot short-ness, so much so that for many years the 2XXX were said to be unweld-able. Increasing the amount of copper, however, to 6% or more, markedlyimproved weldability owing to the large amounts of eutectic available toback-fill hot cracks as they formed. The limit of solid solubility of copperin aluminium is 5.8% at 548°C; at ambient this copper is present as a saturated solid solution with particles of the hardening phase copper alu-minide, CuAl2, within the grains as a fine or coarse precipitate or at thegrain boundaries.
The effect of welding on the age-hardened structure is to re-dissolve theprecipitates, giving up to a 50% loss in ultimate tensile strength in a T6 condition alloy. The weldable alloy 2219 (AlCu6) can recover some of thisstrength loss by artificial ageing but this is usually accompanied by a reduc-tion in ductility. The best results in this alloy are obtained by a full solution
treatment and ageing after welding, not often possible in a fully fabricatedstructure. The less weldable alloy 2014 (AlZnMgCu) may also be heattreated to recover some tensile strength but the improvement is not as great as in 2219 (AlCu6) and may exhibit an even greater reduction in ductility.
Filler metals of similar composition such as 2319 (AlCu6) are availableand weld metal strengths can therefore be matched with the properties inthe HAZ.
The hardening constituent in 6XXX series alloys is magnesium silicideMg2Si. These alloys contain small amounts of silicon and magnesium, typi-cally less than 1% each, and may be further alloyed with equally smallamounts of manganese, copper, zinc and chromium. The alloys are sensitiveto weld metal cracking, particularly when the weld metal is rich in parentmetal such as in the root pass of the weld. Fortunately the cracking can bereadily prevented by the use of filler metals containing higher proportionsof silicon such as 4043 or, with a slightly increased risk of hot cracking, thehigher magnesium alloys such as 5356.
With these heat-treatable alloys the changes in the structure and mechani-cal properties, briefly discussed in Chapter 2, are complex and stronglydependent on the welding conditions employed. Welding without filler metal or with filler metal of parent metal composition is rarely practisedbecause of the risk of weld metal hot cracking. A weld metal with a com-position close to that of the parent metal may age-harden naturally or maybe artificially aged to achieve a strength approaching, but never matching,that of the aged parent metal.
In the overheated zone in the HAZ closest to the fusion line, partialmelting of the grain boundaries will have taken place. Temperatures havebeen high enough and cooling rates sufficiently fast that solution treatmenthas taken place, enabling some ageing to occur after welding. Adjacent tothis is the partially solution-treated zone where some of the precipitateshave been taken into solution, enabling some post-weld hardening to occur,but those not dissolved will have been coarsened. Outside this will be theoveraged zone where precipitate coarsening has taken place and there hasbeen a large drop in strength.
The strength losses in the 6000 alloys are less in the naturally aged metalthan in the artificially aged alloys. The strength of the weld and HAZ in theartificially aged condition generally drop to match that of the naturally agedalloy with a narrow solution-treated zone either side of the weld and anoveraged zone beyond this, which is weaker than the T6 condition. Withcontrolled low-heat input welding procedures the strength of the weldment
44 The welding of aluminium and its alloys
Material standards, designations and alloys 45
will not drop to that of an annealed structure but will be close to that ofthe T4 condition.
7XXX series alloys may, from a welding point of view, be convenientlydivided into two groups. The first group is the high-strength alloys contain-ing more than 1% copper, normally used in the aerospace industry andjoined by non-welding methods. The second group is the medium strengthalloys which have been developed for welding.
Aluminium and zinc form a eutectic containing solid solutions of 83%zinc in aluminium and 1.14% aluminium in zinc. The addition of magne-sium complicates the situation with additional ternary eutectics andcomplex intermetallics being formed, these intermetallics providing dis-persion hardening and precipitates of composition MgZn2. Copper providesfurther precipitation hardening, forming CuAl2 and an intermetallic of thecopper–zinc system.
Welding of the hardened high-strength alloys results in a major loss ofstrength, the high-strength alloys such as 7022 (AlZn5Mg3Cu) or 7075(AlZn5.5MgCu1.6) in particular suffering a considerable reduction instrength. Although almost all of this strength loss can be recovered by a fullheat treatment, the loss in ductility is so great that brittle failure is a realpossibility. The alloys are also very prone to hot cracking and the combi-nation of these adverse features is such that the high-strength alloys arerarely welded. Joining techniques such as riveting or adhesive bonding areoften used to avoid these problems.
The lower-strength non-copper-containing alloys such as 7017(AlZn5Mg2.5Mn0.7), 7020 (AlZn4.5Mg1) and 7039 (AlZn4Mg2.5Mn0.7)are more readily weldable. The response of these alloys is very similar tothat of the 6XXX series, with a loss of strength in the heat affected zones,some of which can be recovered by suitable heat treatment. The alloys willage naturally but it may take up to 30 days for ageing to proceed to com-pletion. The strength loss in the 7XXX alloys is less than that in the 6XXXseries and this, coupled with the natural ageing characteristic, makes thisalloy a popular choice for structural applications where on-site repair andmaintenance work may be required.
One problem peculiar to the 7XXX series is that the zinc rapidly formsan oxide during welding, affecting the surface tension of the weld pool andincreasing the risk of lack of fusion defects. This requires the use of weldingprocedures in which the welding current is some 10–15% higher than wouldbe used for a 5XXX alloy. It has also been found to be beneficial to use ashorter arc than normal so that metal transfer is almost in the globularrange.
126.96.36.199 Unassigned (or other alloys) (8XXX series)
The 8XXX series is used to identify those alloys that do not fit convenientlyinto any of the other groups, such as 8001 (Al-Ni-Fe) and 8020 (Al-Sn).However, contained within this 8XXX group are the aluminium–lithium(Al-Li) alloys, a relatively new family that gives substantial weight savingsof up to 15% and a higher Young’s modulus compared with some of theother high-strength alloys. Each 1% of lithium added results in an approx-imate 3% reduction in weight. These advantages mean that significantweight savings can be achieved in the design of aerospace structures andthat the very high-strength unweldable alloys, such as those in the 2XXXseries, may be replaced by the weldable, lighter Al-Li alloys.
The Al-Li alloys generally contain some 2–3% of lithium and smallamounts of copper and magnesium. They are fully heat treatable, with anumber of different precipitates, the principal one being Al3Li. Typical ofthese alloys are 8090 (AlLi2.5Cu1.5Mg0.7Zr) and 8091 (AlLi2.6Cu1.9Mg0.8Zr). Lithium has a great affinity for oxygen and this reactivity requiresgreat care to be taken during any process that involves heating the alloy.These processes comprise melting, casting, high-temperature heat treat-ment and welding. Failure to remove the oxidised layer will result in grossporosity – some 0.2mm should be machined off to be certain of completeremoval. It may also be necessary to purge the back face of the weld withan inert gas to prevent oxidation and porosity. As with the 7XXX alloys theAl-Li alloys have a similar response to the heat of welding, losing strengthin the HAZ, although a post-weld artificial ageing treatment can restore alarge proportion of this strength.
A further family of alloys that may fall into this group once they havebeen assigned a designation are those containing scandium. These are newalloys, still to a great extent in the development phase. Scandium is a rareearth element that has been found to be highly effective in increasingstrength by age hardening and by grain refinement, the latter being particu-larly useful in weld metal. Scandium is likely to be used in conjunction withother alloying elements such as zirconium, magnesium, zinc or lithiumwhere tensile strengths of over 600N/mm2 have been achieved in labora-tory trials.
3.5 Filler metal selection
Filler metal specifications are to be found in BS 2019 Part 4, although thiswill be replaced in the near future by a CEN specification. The BS specifi-cation lists 11 filler metal types in the 1XXX, 3XXX, 4XXX and 5XXXseries and details the delivery conditions. BS 2901 does not include any fillermetals capable of being age hardened. The American Welding Society has
46 The welding of aluminium and its alloys
Table 3.1 General guidance on filler metal selection
7XXX NR 5XXX 5XXX NR 5XXX 5XXX 5XXX 5XXX 5XXXNR NS NS NR NS 4XXX NS NS NSNR NS NS NR NS NS NS NS NS
published a similar specification, AWS A5.10 ‘Specification for Bare Alu-minium and Aluminium Alloy Welding Electrodes and Rods’, which fulfilsa similar role. This specification includes 15 separate filler metal composi-tions, comprising alloys in the 1XXX, 2XXX, 4XXX and 5XXX series. Inaddition there are five age-hardening filler metals designed for use in thewelding of castings. AWS A5.10 also includes delivery conditions and thetesting requirements for usability and soundness.
As mentioned earlier, filler metal selection is crucial to producing crack-free, optimum strength welded joints but there are other considerations that may need to be included when making the choice. Unlike selecting consumables for welding steel, where the composition of the filler metalgenerally matches that of the parent metal with respect to composition,mechanical properties, corrosion resistance and appearance, aluminiumalloys are often welded with filler metals that do not match the parent metalin some or all of these properties. This presents the engineer with someproblems when it comes to deciding on the optimum filler metal composi-tion. In addition to strength and crack resistance the choice may also needto include colour match, corrosion resistance, response to anodising and
48 The welding of aluminium and its alloys
Table 3.2 Guidance on filler metal selection – dissimilar metal joints for specific alloys
creep strength. Guidance on suitable fillers can be found in Table 3.1, forspecific alloys, in Table 3.2 and to achieve specific properties in some of thecommoner structural alloys in Table 3.3. In Table 3.1 there are three re-commendations based on the best strength, the upper figure; the highestcrack resistance, the middle figure; and an acceptable alternative, the lowerfigure. Note that the alloys are arranged in families – for a recommenda-tion on filler metal read directly across and down from the alloys of interest.
There are a number of specific points to be made to amplify the guid-ance given in Tables 3.1–3.3:
• When welding alloys containing more than 2% magnesium avoid theuse of fillers containing silicon as the intermetallic compound magne-sium silicide, Mg3Si, is formed. This embrittles the joint and can lead tofailure in joints that are dynamically loaded. The converse is also true,that Mg3Si will be formed when welding alloys containing more than2% silicon with 5XXX fillers.
• 5XXX filler metals with more than 5% Mg should be avoided if theservice temperature exceeds 65°C as Al2Mg is formed, which makes thealloy susceptible to stress corrosion. Filler metals such as 5454 or 5554containing less than 3% Mg should be used.
• High-purity 5654 is preferred for the welding of high-purity aluminiumin hydrogen peroxide service.
• 4643 may be used to weld the 6XXX alloys as the small amount of magnesium improves the response to solution treatment.
Material standards, designations and alloys 49
Table 3.3 Filler metal selection to achieve specific properties for the commonerstructural alloys
Base Highest Best ductility Salt water Least cracking Best formaterial strength corrosion tendency anodising
• The pure aluminium 1XXX alloys are very soft and wire feeding prob-lems can be experienced.
• Low magnesium (<2%) 5XXX alloys such as 5251 may suffer hot crack-ing if matching composition fillers are used. Use Al-Mg5 type instead.
• When welding the 7XXX alloys 5039 filler metal may give more effec-tive age hardening in low-dilution applications.
• 6XXX alloys exhibit solidification cracking if welded autogenously.• Titanium and zirconium are sometimes added to filler metals to reduce
the risk of weld metal hot cracking by means of grain refinement.• 4047 may be used to prevent weld metal cracking in joints involving high
dilution or restraint but remember the first point above.• The 2XXX series of copper containing alloys were generally regarded
as unweldable until the higher (>4%) copper alloys such as 2219 becameavailable. If it is necessary to weld the lower copper-containing alloysthen 4047 is the best choice as a filler metal.
50 The welding of aluminium and its alloys
The need for degreasing and oxide removal has been covered in Chapter2. This chapter will review both the handling and storage of aluminium andthe options available for cutting, machining and pickling and cleaning ofthe alloys prior to welding. There are a number of thermal processes avail-able to the fabricator for either cutting or weld preparing, as discussed inthis chapter. One process that is not available for the cutting of aluminium,however, is the oxy-gas process used so widely to cut the carbon and low-alloy steels. Instead, arc or power beam processes or machining mustbe used to provide the correct edge preparations for welding.
Correct and accurate edge preparations are essential for the productionof sound, defect-free welds in aluminium. Edge preparations are requiredto achieve full penetration to the root of the joint, to enable the correctanalysis of weld metal to be achieved, to assist the welder to produce defect-free joints and to do this at an acceptable cost. The design of edge prepa-rations for specific welding processes will be dealt with in the chaptersdealing with the individual processes.
4.2 Storage and handling
Good handling practices are required if aluminium components are to besupplied to the customer in an unmarked condition. Aluminium is a rela-tively soft material and is easily scored or dented by clumsy handling or theuse of inappropriate lifting equipment. Over-centre edge clamps, commonlyused on steels, can score plate edges and steel chains can produce scratchesand dents. A solution to marking by clamps is to face the jaws with a softmaterial – wood or polythene blocks are excellent as packing materials.Lifting should be carried out with nylon ropes or webbing straps. Remem-ber that these softer materials are far more easily damaged than steel andmore regular maintenance of any lifting equipment will be necessary. Hard
4Preparation for welding
particles can also become embedded in the packing or lifting strops, result-ing in marking of the components.
Storage is important if the surface condition of the aluminium is not tosuffer. Ideally, items should be stored indoors in a dry, clean and well-ventilated storage area. Storing plates flat may give rise to water stainingfrom condensation collecting on the surface. This can be particularly dam-aging if the plates are stacked directly one on top of another, when a thicklayer of hydrated oxide can rapidly form at the interface. Plates shouldalways be separated in storage and ideally stacked on edge to provide goodair circulation. This reduces the risk of accumulating water and dirt on theflat surfaces and prevents other items being stored on top. It also assists inreducing the risk of scratches from dragging plates off the stack.
4.3 Plasma-arc cutting
Plasma-arc may be used for either cutting or welding and is the most widely used thermal process for cutting of aluminium alloys in manual,mechanised or fully automated modes (Fig. 4.1). In the latter case cuts ofexcellent quality can be achieved in material of up to 250mm thickness at high cutting speeds.
Plasma-arc utilises a specially designed torch in which a tungsten elec-trode is recessed inside a water-cooled copper annulus, through which ispassed the plasma gas.An arc is struck between the electrode and the work-piece, transferred arc plasma-arc, or between the electrode and the annulus,non-transferred arc plasma-arc. Transferred arc plasma-arc is used forcutting purposes (Fig. 4.2). The plasma gas is heated by the arc to anextremely high temperature within the annulus and is ionised – it becomesa plasma. At the same time it expands in volume due to the high tempera-ture and, being forced through the constriction of the nozzle, reaches veryhigh velocity. The heat for welding and cutting is therefore provided by a ‘flame’ or plasma jet of high-velocity gas at temperatures of up to 15000°C, which has the characteristics of being highly concentrated, virtu-ally insensitive to stand-off distance and extremely stiff. This makes it anideal candidate for cutting purposes.
The cut is made by the plasma jet piercing the component to be cut toform a keyhole, a hole that penetrates completely through the item. This isfilled with the gas and is surrounded by molten metal. The force of theplasma jet alone may be sufficient to remove this molten metal but withthicker material a secondary cutting gas may be required to assist in metalremoval. This secondary gas is supplied via a series of holes around theplasma nozzle designed to blow away the molten metal to give a clean,
Preparation for welding 53
4.2 Schematic illustrating the principles of plasma-jet cutting.Courtesy of TWI Ltd.
high-quality and narrow cut. Plasma gases include air, argon, argon–hydrogen, nitrogen and carbon dioxide. Cutting can be performed manu-ally or mechanised with higher cutting speeds being achievable with mech-anised and automated systems.
A plasma cut edge is generally not completely square. The top edge ofthe cut may be rounded by some 1 or 2mm, particularly if the cutting energyis high for the thickness of plate being cut or when high-speed cutting ofthin material is being carried out.The plasma jet also tends to remove moremetal from the upper part of the component than the lower part, resultingin a cut wider at the top than the bottom with non-parallel sides.This ‘bevel’angle may be between 3° and 6°. The cut surface may also be rough. Thequality of the cut is affected by gas type, gas flow rate, cutting speed andoperating voltage. High gas flow rates and high voltages will improve the squareness of the cut and mechanised cutting will give an improvedappearance.
Arc cutting produces a HAZ and may cause melting at the grain bound-aries. This results in micro-cracking, primarily of the heat-treatable alloys –the 7000 series being particularly sensitive. As the thickness increases, thelikelihood of such cracking also increases. For this reason it is advisable to machine back the plasma cut edges by about 3mm, particularly if thecomponent is to be used in a dynamic loading environment.
The composition of the gas for plasma cutting depends on the requiredquality of the cut, the thickness of the metal to be cut and the cost of thegas. Air is the cheapest option and single gas systems utilising air and ahafnium electrode have been developed for the cutting of materials up toapproximately 6mm in thickness (Fig. 4.3).
Above this thickness nitrogen, carbon dioxide, argon–hydrogen or mixtures of these gases may be used. For the thicker materials over, say,
54 The welding of aluminium and its alloys
4.3 Air plasma cutting. Courtesy of TWI Ltd.
12.5mm, argon–hydrogen is regarded as the best choice for the plasma gas,this gas mixture giving the best quality cut, irrespective of thickness. Thesecondary cutting gas may be carbon dioxide or nitrogen. Table 4.1 lists therecommended cutting/shielding gases and typical parameters for plasmacutting the aluminium alloys. Water injection into the nozzle can be used inaddition to the orifice gas. This restricts the plasma jet further and producesa better quality, more square, cut, although above 50mm thickness theseadvantages are reduced.
A development of the process known as high-tolerance plasma-arccutting (HT-PAC), also known as plasma-constricted arc, fine plasma orhigh-definition plasma, has been developed and is being used as a cheaperalternative to laser cutting of material less than 12mm in thickness. Thisvariation to the plasma-arc process achieves a better quality cut with more perpendicular faces, a narrower kerf and a less rough finish than the
Preparation for welding 55
Table 4.1 Suggested parameters for plasma-jet cutting
Metal Plasma Gas Shield Gas Current Voltage Cutting Methodthickness gas flow gas flow (amps) (volts) speed
(l/min) (l/min) (mm/min)
1.0 Air 98 4800 Manual1.5 Air 98 6300 Manual3 Air 98 3000 Manual6.5 Air 98 1000 Manual6.5 N2 34 CO2 100 1800 Manual6.5 Ar + H2 25 200 50 1500 Manual
10 N2 35 CO2 100 200 1250 Manual12.5 Ar + H2 28 280 55 1000 Manual25 Ar + H2 33 330 70 500 Manual50 Ar + H2 45 400 85 500 Manual6 Ar + H2 55 300 140 7500 Mechanise6 N2 32 CO2 100 115 1800 Mechanise
10 N2 32 CO2 100 120 900 Mechanise12.5 N2 32 CO2 100 120 480 Mechanise12.5 N2 32 CO2 100 300 3200 Mechanise12.5 Ar + H2 60 300 140 5000 Mechanise25 N2 70 CO2 100 400 1800 Mechanise25 Ar + H2 60 375 160 2300 Mechanise50 N2 32 CO2 100 400 800 Mechanise50 Ar + H2 60 375 165 500 Mechanise75 Ar + H2 95 420 170 380 Mechanise75 Ar + H2 45 N2 100 400 500 Mechanise75 Ar + H2 45 N2 100 700 650 Mechanise
100 Ar + H2 95 450 180 750 Mechanise125 Ar + H2 95 475 200 250 Mechanise
plasma-arc cut by a combination of a redesigned nozzle and a constrictingmagnetic field (Fig. 4.4). Typical cutting parameters are given in Table 4.2.
A variation to the conventional plasma cutting process is the plasmagouging technique. This utilises a plasma-jet torch which, as shown in Fig.4.5, is presented to the surface at a glancing angle. In doing so the surfaceis blown away and a groove is formed. The technique may be used toremove excess metal, to excavate for defect removal, to back-gouge thereverse side of welds and to establish a weld preparation. Needless to sayit requires a skilled operator to achieve an acceptable surface and shouldnot be entrusted to unskilled personnel since it is capable of removing largeamounts of metal very rapidly.
4.3.1 Health and safety
The plasma-arc process uses higher open circuit and arc voltages than doesthe TIG process, with operating voltages as high as 400 volts in some appli-cations. These voltages present a serious risk of electric shock and suitable
56 The welding of aluminium and its alloys
Cooling water – inand out
Magnetic field coil Plasma
4.4 HT-PAC torch. Courtesy of TWI Ltd.
Table 4.2 Suggested parameters for HT-PAC
Metal thickness Plasma Shield Current Stand off Cutting (mm) gas gas (A) (mm) speed
1.2 Air Air 70 2 38002 Air Air 70 2.5 25404 Air Air 70 2 1800
precautions must therefore be taken to ensure that cutting operations arecarried out in a safe manner. Only fully trained operators should be per-mitted to operate the cutting equipment. All frames, casings, etc., should beconnected to a good electrical earth and all electrical connections and terminals must be adequately protected. Any equipment maintenance ormodification must be carried out by suitably trained and qualified staff andconnections, insulation, etc. inspected at regular intervals for soundness anddeterioration.
The plasma-arc produces large amounts of infra-red and ultra-violet radi-ation. All personnel in the vicinity of plasma-arc cutting operations there-fore need to be provided with protective clothing, goggles and helmets toprotect both eyes and skin. The operator must use the correct filter lensesfor electric arc welding, with shade numbers ranging from 9 to 14, depend-ing upon the current.
As with any thermal cutting process copious amounts of fume are pro-duced. The fume will contain not only aluminium oxide but the oxides of the other elements present in the alloy, ozone, oxides of nitrogen,any surface plating or coating, any contamination and the cutting gases.These present a health hazard that is best dealt with at source by local fume extraction. Fume extraction, either local or general, will almost certainly be mandatory if the fume and gas limits set by the Control of Substances Hazardous to Health (COSHH) Regulations are to be com-plied with. Cutting in confined spaces presents a particular problem. Fumeextraction and ventilation must be provided in these circumstances. Itshould be remembered that many of the cutting gases, although not toxic,are asphyxiant, are heavier than air and can accumulate in low-lying areas
Preparation for welding 57
Power inletShielding gas inletPlasma gas inlet
Tungsten electrodeShielding gas shroud
Direction of gouge
4.5 Plasma-arc gouging principles. Courtesy of TWI Ltd.
such as pits and wells. Forced ventilation should be considered in such circumstances.
When plasma-arc cutting is carried out under water the dross that is produced may build up on the tank bottom. Over a period of time this drossreacts with the water, producing hydrogen which may accumulate under theitem being cut, leading to a risk of explosion. This is best avoided by clean-ing the tank of the dross at regular intervals or using a forced circulationwater supply to carry away any gas as it is formed.
Plasma-arc cutting is a very noisy process, the noise level increasing asthe cutting current is increased. Ear protection is required for the operatorand personnel working in the vicinity to avoid discomfort or ear damage.
4.4 Laser beam cutting
A laser (light amplification by the stimulated emission of radiation) gener-ates a coherent beam of light at an essentially constant wavelength. Whenthis beam is focused on a surface there is sufficient energy concentrated inthis focused spot that the material may be melted or vaporised (Fig. 4.6).This enables the laser to be used for either welding or cutting. The laserlight is produced by exciting a lasing medium, this being either a suitablegas or solid. The excitation is provided by the passage of an electric currentor by means of high-intensity light. There are two commonly used lasers tobe found in industrial applications: the gas CO2 laser and the solid statecrystal laser, the neodymium-doped yttrium–aluminium–garnet (Nd-YAG)laser. Of the two, the CO2 laser is the most powerful with average poweroutputs of up to 50 kilowatts. Both types of laser can be designed to provide
58 The welding of aluminium and its alloys
Pressurised assistgas inlet
Focused laser and gas jet
4.6 Laser cutting principles. Courtesy of TWI Ltd.
a steady output, continuous wave (CW) laser light or in a pulsed outputmode. In this latter case the power output on the peak pulse may be asmuch as 20 times the average power.
The wavelength of light from the CO2 laser is 10.6 microns (micro-metres) and at this wavelength is easily absorbed by most solids, enabling the CO2 laser to be used on a wide variety of materials. This long wave-length has a disadvantage, however, in that it cannot be transmitted by glassor fibre optics but requires reflecting metal mirrors for manipulating thebeam and materials such as zinc selenide or gallium arsenide for focusinglenses.The Nd-YAG laser light is an order of magnitude less at 1.06 microns,allowing the use of glass lenses for focusing and fibre optic cable for beamtransmission. This offers a clear advantage over the CO2 laser, since itpermits the marriage of commercially available manipulating equipmentsuch as NC (numerically controlled) gantries and robots with the laser.The power output of currently available Nd-YAG lasers is limited to around6 kilowatts, however, restricting the thickness of materials that can be cut.
The laser cutting process consists of focusing the beam through a cuttingnozzle onto the surface to be cut, the concentration of energy being suffi-cient to vaporise the material, creating a ‘keyhole’. With continuous wavelasers there is generally more melting than vaporisation and an assist gas isused to blow away the vapour and any molten metal, creating a narrowclean cut as the beam is traversed along the item. The pulsed lasers gener-ally provide enough energy that the laser beam imparts sufficient force tothe vapour that the vapour itself removes any molten metal. The assist gas,introduced either through the cutting nozzle or co-axially with it, is usednot only to blow away any molten metal but also to protect the lens fromspatter or debris ejected from the cut.
The assist gas for cutting aluminium may be oxygen, nitrogen or air.Oxygen is a reactive gas with aluminium and will give higher cutting speedsthan nitrogen. Nitrogen, however, will give a better quality cut in terms ofsquareness and roughness than will oxygen. Air is a compromise but is thecheapest of the gases. Gas pressure is an important variable that needs tobe controlled to give the best quality of cut – high gas pressures give themost effective metal removal but too high a pressure may damage the focus-ing lens, since this forms part of the pressure system. As the assist gas pres-sure is increased the lens also needs to be thickened in order to carry theincreased pressure. The pressure of gas in the cut is also influenced by thedistance between the nozzle and the workpiece. For example, high-pressurecutting may require a stand-off distance of only some 2.5mm. The rela-tionship between stand-off and pressure in the kerf is not simple, however,as most laser cutting is done with supersonic gas velocities. It is essentialthat the nozzle stand-off distance and nozzle condition are closely
Preparation for welding 59
controlled to provide consistent and high-quality cuts. Typical laser cuttingparameters are given in Table 4.3.
A number of advantages accrue from using a laser for the cutting of weldpreparations:
• Low heat input, resulting in minimal distortion and narrow heat affectedzones.
• Edges that are smooth and perpendicular to the surface and oftenrequire no further cleaning before welding.
• Narrow kerfs and heat affected zones, meaning that more efficientnesting can be achieved, resulting in material savings.
• Very thin materials can be cut without distortion.• Very accurate cuts can be made, resulting in more easy assembling for
welding, this giving reduced fit-up time, more accurate fit-up and fewerweld defects.
• The process is easily automated and can be readily interfaced with otherNC equipment (Fig. 4.7).
The main drawbacks to the use of lasers for the cutting of aluminium areas follows:
• The capital cost of equipment, which may be in the order of several hundreds of thousands of pounds for a laser interfaced with suitablemanipulating equipment. A 1.5kW CW Nd-YAG laser interfaced witha robotic system, together with its appropriate safety equipment willcost in the region of £250k to £300k at today’s (2002) prices.
• The coupling of the beam with the work surface is not very good sincealuminium can be highly reflective. This means that higher power isneeded to cut an aluminium component than a similar item in steel.Aluminium may also reflect the beam back into the lens, resulting indamage, although this problem has lessened with the development ofmore accurate lenses and focusing systems.
• Laser cut aluminium may have a heavy dross on the underside of thecut. Removal of this can make the process non-competitive with otherprocesses. Higher gas pressures will assist in reducing or eliminating theproblem.
• The cut edges of the age-hardening alloys may contain microfissuresthat will need to be removed.
4.4.1 Health and safety
The laser cutting process is a thermal process and therefore metal fumemixed with the assist gas will be generated. This fume will need to beremoved, preferably by local fume extraction at source. As laser cutting is
60 The welding of aluminium and its alloys
Table 4.3 Parameters for laser cutting
Process Thickness Average power Pulse frequency Pulse width Assist gas Gas pressure Cutting speed(mm) (kW) (Hz) (ms) (mm/min)
CW Nd-YAG2 2 na na oxygen 45002 2 na na nitrogen 300
1.2 1.41 na na oxygen 38002 1.2 na na oxygen 30004 1.5 na na oxygen 1200
performed with mechanised or automated systems using remote controlthere is only a limited risk of fume exposure for the operator. However, alaser cutting system generally has a very high usage and fume extractionwill be required to control the general fume level within the shop.
The voltages used in laser equipment are sufficiently high to present aserious risk of electric shock. Access panels should be secured and suitablymarked to highlight the risks. Only authorised and trained personnel shouldbe permitted access to the equipment for repair and maintenance purposes.A typical laser work cell is illustrated in Fig. 4.8.
There are two hazards associated with laser radiation which, dependingupon the wavelength, can damage either the eye or the skin. The radiationcan damage the retina and/or the cornea, particularly the shorter wave-length radiation which can be focused by the lens of the eye on to the retina.Exposure of the skin can result in burns.With high-power lasers these burnsmay be deep and can cause permanent damage. To prevent such damage itis generally necessary to position the laser inside a suitable enclosure withinterlocks to prevent access when the laser is operating. Screening of theCO2 laser beam can be provided by clear glass or acrylic screens. Tintedwelding screens are required for the solid state lasers since the radiation iscloser to the wavelength of visible light than that of the gas laser. Personaleye protection for the operator is also recommended, selected to filter outthe appropriate wavelength of laser light.
62 The welding of aluminium and its alloys
4.7 CNC CO2 laser cutting machine. Courtesy of Messer Griesheim.
Visible radiation is also emitted during laser cutting, this light being similarto that produced from a welding arc containing both ultra-violet and infra-red light.To filter this out requires tinted filter glasses,the density of the shadebeing sufficient that no discomfort is felt when viewing the bright plume asso-ciated with the beam. This radiation may also cause skin reddening. It goeswithout saying that all personnel involved in laser processing operationsshould be fully trained in the use of eye and skin protection equipment.
4.5 Water jet cutting
Water jet cutting uses an abrasive powder introduced into a very high-pressure and velocity water jet and is capable of cutting both metallic andnon-metallic materials essentially by a process of erosion. Water velocity isin the region of 2500km/h (1600mph) and water pressure between 2000 bar (30000psi) and 4000 bar (60000psi). One of the most important usesof water jet cutting is the roughing out of parts prior to finish machining.The great advantage that water jet cutting has over the laser or plasma-arcis that no heat is used in the process. There are therefore no heat affectedzones and no thermal distortion. Parts can be cut very accurately and closelynested, resulting in material savings. Cut part tolerances are very small,simplifying the task of fitting up for welding.
Although aluminium up to 450mm in thickness can be cut using theprocess, the limitations with water jet cutting are the cutting speed, which
Preparation for welding 63
4.8 Laser welding and cutting work cell. Courtesy of TWI Ltd.
may be only a quarter the speed of a laser cut component, particularly inthin sections. The other limitation is the bevel or taper of the cut face whichmay be twice that of laser cutting, some 25% of the nozzle diameter oraround 0.2mm at the optimum cutting speed. The bevel can be reduced byslowing the cutting speed with the penalty of an increased cost.
4.6 Mechanical cutting
Although the methods mentioned above can be applied to many fabricat-ing activities, mechanical cutting techniques are used by most welding work-shops as being the most cost-effective and versatile method. Cutting andmachining equipment is freely available in most fabrication shops and isfrequently less capital intensive than the sophisticated laser or plasmacutting systems discussed above. Furthermore, the systems described in Sections 4.2, 4.3 and 4.4 are capable of straight or simple bevel cuts only –if double bevel preparations are required then two or more cuts are nec-essary and J-preparations are not feasible. Edge preparations can be pro-duced in a number of ways such as high-speed milling machines, edgeplaners, routers and various types of saws. Where air-powered equipmentis used care needs to be taken to ensure that the air supply is clean, dry andoil-free to prevent contamination of the surfaces, which would give rise toporosity during welding.
Routers, planers and edge millers are capable of producing J- and U-preparations when fitted with the correct shape of tools. The equipment forthese tasks can be hand-held and similar to that used for wood working,the only requirement being the need for slightly greater power or floormounts for greater capacity. High cutting speeds can be used without theneed for lubricants or coolants, although this does not remove the need forthorough cleaning. Hand-held rotary cutting machines are ideally suited toback-gouging and for removing excess weld metal. The depth of cut can beadjusted and various cutter forms are available, including V-blades for bevelling and flat blades for weld cap removal.
The guillotine can be used to shear sheets of up to 6mm thickness withoutthe need for further preparation work. Over this thickness some dressingof the sheared edges is necessary if the best weld quality is to be achieved.Shearing of the edges of alloys containing more than 3.5% Mg is not recommended if the edges are to enter service ‘as sheared’ because of therisk of the work-hardened edges suffering from stress corrosion cracking.Edges that are welded after shearing do not suffer from this problem.
Sawing is a very effective method of cutting and bevelling aluminiumusing either portable or floor-mounted equipment. To achieve a goodquality cut high cutting speeds are necessary, around 2500 metres perminute (mpm) peripheral surface speed for high-speed steel circular saw
64 The welding of aluminium and its alloys
blades, 3500mpm for tungsten-tipped blades and 1800mpm for band sawblades. It is usual for band saw blades to have wider spacing on the teeththan for steel to prevent snagging, 8 to 16 teeth per centimetre being rec-ommended. Band and circular saws can produce straight cuts and, whenequipped with a tilting table, bevelled cuts. The saw cut surface tends to berough and readily traps grease and dirt, making cleaning and degreasingdifficult. It is recommended that the sawn faces are milled or filed toproduce a smooth surface when the best quality of weld is required.
Grinding is best performed with high-speed, semi-flexible aluminiumoxide grinding discs. Care needs to be taken to ensure that the grinding iscontrolled and is not heavy handed. Over-enthusiastic grinding can give atorn and rough surface which will be difficult to clean. Material may alsobe smeared over the surface, physically trapping dirt and grease and givingrise to porosity on welding. Rotational speed of the discs needs to be in the region of 8500rpm. Care should be taken that the grinding machinesare capable of maintaining these speeds when under load – some machinesare incapable of attaining or maintaining these speeds in operation. Gritsizes range from 24 to 120 and the discs selected should be of the non-loading type. Under these conditions the discs should not become cloggedand the speed of metal removal should not be affected. Grinding can be used to clean the weld preparation prior to welding, to blend the weldinto the parent metal, to remove excess weld metal and to back-grind a partially penetrated weld to sound metal. To achieve the best results this requires suitable and well-maintained equipment operated by trained personnel.
Hand-held abrasive belt sanders are readily available and enable finish-ing operations to be carried out without too great a risk of damage owingto incorrect manipulation of the sander. Belt widths of 3–100mm can bepurchased; the narrow belts in conjunction with sander arms of up to 500mm in length enable dressing operations to be carried out when accessis very restricted.
Most machining and grinding operations can be carried out without lubri-cation. Dust may therefore be a problem and operators may need to beequipped with dust masks or respirators and the equipment with dust collectors. Noise can also be a problem and ear defenders will be neededfor some of the machining and grinding tasks.
One last but very important point to be made before ending this sectionon the cutting and machining of weld preparations is that the equipmentmust not be used on aluminium if it has been used on other metals. Cross-contamination of aluminium with copper, iron, etc., may result in weldingor service problems. Wire brushes, grinding discs, cutters and milling headsmust only be used on aluminium and should be identified as such if thereis any possibility of cross-contamination. Machining equipment should be
Preparation for welding 65
thoroughly cleaned of any foreign metals before being used on aluminiumalloys.
4.7 Cleaning and degreasing
Components for welding may be flat, preformed, sheared, sawn or milledto give the desired shape or to provide the weld preparation. Lubricantsused during these processes must be removed if weld quality is to be main-tained. Degreasing may be accomplished by wiping, brushing, spraying orvapour degreasing with commercially available solvents. This is best donebefore any mechanical cleaning takes place. Mechanically cut edges maycarry burrs along the cut edge that will trap dirt and grease. These burrsshould therefore be removed from weld preparations by scraping with adraw tool – do not wire brush only as this may fail to remove them com-pletely. Scraping is also an excellent method for removing the oxide film.Stainless steel wire brushes, stainless steel wire wool or files may also beused to remove the oxide. As mentioned above in Section 4.6, under no circumstances should carbon steel, brass or copper brushes be used. Makesure that any cleaning tools are segregated and are used only on aluminium,otherwise cross-contamination can occur.
In certain cases, particularly when striving to achieve freedom fromporosity, chemical cleaning or pickling may be required. A pickling shop isillustrated in Fig. 4.9 and a schedule of chemical cleaning treatments is givenin Table 4.4.
66 The welding of aluminium and its alloys
4.9 Typical pickling shop. Courtesy of R. Andrews.
Table 4.4 Chemical treatments for cleaning and oxide removal
Solution Concentration Temp (°C) Procedure Container material Purpose
Nitric acid 50% water 18–24 Immerse 15min Stainless steel Removal of thin oxide film 50% HNO3 Rinse in cold water for fusion welding
(technical Rinse in hot watergrade) Dry
Sodium hydroxide 5% NaOH in 70 Immerse 10 to 60s Mild steel Removal of thick oxide film followed by nitric water Rinse in cold water Stainless steel for all welding andacid brazing operations
Concentrated 18–24 Immerse 30sHNO3 Rinse in cold water
Rinse in hot waterDry
Sulphuric – chromic 5 litres H2SO4 70–80 Dip for 2 to 3min Antimonial lead lined Removal of films and stains acid 1.4kg CrO3 Rinse in cold water steel tank from heat treating and
40 litres water Rinse in hot water oxide coatingsDry
Phosphoric – chromic 1.98 litres of 95 Dip for 5–10min Stainless steel Removal of anodic coatingsacid 75% H3PO3 Rinse in cold water
0.65kg of CrO3 Rinse in hot water45 litres of water Dry
Once degreased and cleaned the parent material should be welded withina short period of time; typically four hours would be regarded as reason-able. The component must be maintained in a clean condition during thistime and this may require the item to be covered with polythene sheets orbrown paper. If the item is left standing overnight the joints may requirean additional cleaning operation so it is advisable to clean only those partsthat can be welded within a four or five hour production period.
There are a couple of points concerning cleanliness that are worth men-tioning. If the chemical cleaning has been extremely good then it is possi-ble to leave the components for a longer period of time, perhaps overnightif the storage conditions are clean and dry. It has also been noticed thatwhen the items are ‘super clean’ the TIG or MIG welder can experiencearc starting and stability problems. The reason for this is not clear but isprobably associated with the complete absence of any oxide. It is thoughtthat a small amount of oxide assists in the formation of an active anodespot, resulting in a more stable arc.
The aluminium fabrication area ideally should be separated physicallyfrom other fabrication areas. For example, dust from activities such as grinding, settling on the surface will cause problems, particularly if this isfrom the grinding of steel items in adjacent bays. Aluminium and steelshould never be welded in the same welding booth. It cannot be empha-sised too strongly how important attention to cleanliness is if sound, defect-free welds are to be made consistently.
68 The welding of aluminium and its alloys
In all constructional applications where welded connections are used eithera stress analysis is carried out or ample experience of acceptable perfor-mance exists for the specific joint design. The principles of stress analysisare outside the scope of this chapter – it deals instead with those shop-floorfabrication activities that the designer directly influences. There are manynational and international specifications dealing with the design aspects ofspecific structures. For instance, BS 8118 deals with the structural use of alu-minium, as does the US specification D 1.2. Pressure vessel design iscovered by BS PD 5500 and ASME VIII. For advice on the design of suchstructures the designer can do no better than consult the relevant specifi-cations. For a list of relevant specifications see Appendix A at the end ofthis book.
The objective of the designer is to provide an assembly with adequatestrength for the specific application with the least amount of weld metaland the minimum number of joints. This requires the designer to plan fora smooth flow of stresses through the joint, to compensate for any strengthloss due to welding, to design the component such that there is sufficientaccess for welding and to select the metal to be welded with optimum weld-ability in mind. As mentioned in Chapter 2 there is little that can be doneto improve the strength of the weldment to match that of the cold workedor precipitation-hardened alloy. All that the designer can do to compensatefor the loss is to thicken the component, either overall or locally, or to movethe weld to an area of low stress. For advice consult British Standard BS8118 or the AWS Structural Design Code D 1.2, as mentioned above.
There are a number of factors that the designer needs to take intoaccount that are specific to designs in aluminium. Some of these have beenmentioned in earlier chapters and include such physical properties as thehigh coefficients of thermal conductivity and expansion, the major loss of strength of certain alloys in the HAZ and the low Young’s modulus. In
addition, the designer must consider access for both welding and inspec-tion, joint design to enable high-quality welds to be made, the effects andminimisation of distortion and the effect of welding on stress concentra-tions and fatigue.
The ease with which a weld can be made is crucially dependent on jointdesign and this will have a direct effect on fabrication costs. It is thus essen-tial that the designer is aware of certain fundamentals of welding practicein order to achieve the objectives of the lightest structure capable of per-forming its desired function at the lowest cost.
There are a number of ‘golden rules’ that the designer should keep inmind when detailing the drawings:
• Remember that weld metal is very expensive. Do not over-specify filletweld throat thickness and specify the narrowest weld preparation anglethat is consistent with quality. Specify these sizes clearly.
• Keep welding to a minimum – use formed sections instead of weldedplate, keep stiffeners to a minimum. The cheapest weld of all is the oneyou do not make!
• Specify welds to be made in the flat position.• Allow adequate access for the welder – see below.
5.2 Access for welding
The two most common design faults are failing to recognise that full visionof the weld pool is essential for manual welding and that the weld must beat a comfortable distance from the operator, neither too close nor at a dis-tance where the welder’s arm is at full stretch. These errors can frequentlybe recognised at the design stage and the benefits of requiring an ex-perienced welding engineer to review draft drawings cannot be over-emphasised. The distance from the operator’s head to the weld can easilybe checked on drawings. Ideally this distance should be in the region of 200mm minimum to 450mm maximum. It should be remembered that thediameter of the welder’s helmet is about 300mm and that this will affectthe access requirements.
For a joint to be accessible for manual welding welders must be able com-fortably to position themselves and their equipment if high-quality weldsare to be produced. This requires sufficient space to permit free movementof the welding torch or electrode and to enable the torch to be presentedto the weld pool at the correct angle. Detail design must also take intoaccount the proximity of adjacent material which should be such that thewelder is allowed an unrestricted view of the arc. The amount of spacerequired will depend on the size of the equipment to be used, in particularthe size of the torch. Welding aluminium with the gas shielded processes
70 The welding of aluminium and its alloys
requires a large diameter gas shroud and a short arc length.This means thatthe welder’s view of the weld pool is more restricted than when welding asimilar configuration in steel. The sketch in Fig. 5.1 illustrates a situationthat is often encountered in practice where the designer has failed to takeinto account the need for adequate access. As a rule of thumb the distancebetween the plates should be as shown.A further limitation for TIG weldingis the need to add a filler wire that restricts further the welder’s view of thearc and the ease of manipulation as both of the welder’s hands need to bein the work area.
The welding of attachments or nozzles to plates or pipes can presentproblems when the nozzle is presented to the surface at an angle less than45°.Access into the acute angle is difficult, resulting in lack-of-fusion defectsin the root of the weld as illustrated in Fig. 5.2.
5.3 Welding speed
Aluminium is normally welded at higher travel speeds than when weldingsteels, particularly when using the MIG process. The implication of this isthat abrupt changes of direction are to be avoided. It is, for example, impos-sible to weld around a 90° corner as the MIG torch cannot be moved rapidlyenough to keep the correct lead angle. It is also difficult to weld aroundsmall diameter bosses fixed in position. In this sort of application the bossneeds to be rotated with the torch held stationary. Such comments do notnecessarily apply when fully mechanised or robotic equipment is used.
Welding design 71
x For adequate access to the filletwelds between the two upright platesy should always be less than x
5.1 Access requirements for welding.
Face side weldRoot sealing pass
Inability to achieve correct arc length MIG torchgas shroud
5.2 Access problems of angled plates or pipes.
Automation or the use of robots enables torch positioning and motion tobe controlled with the precision required for the production of qualitywelds.
5.4 Welding position
Welding in the flat or downhand position is preferred for all arc weldingactivities. It is easier for the welder to deposit high-quality weld metal athigh deposition rates in the flat position than in any of the other positions.The weld pool is larger in this position with slower solidification and coolingrates, permitting gases to evolve from the pool and reducing the amount ofporosity. The force of gravity in positions such as the horizontal–vertical,however, means that the weld pool tends to sag, making it more difficult toachieve an acceptable weld profile. These effects are more marked withMIG than with TIG. Flat position welding therefore gives the best qualityweld metal at the lowest cost.
The designer should take these points into account when considering thedesign of a structure. Wherever possible welding should be performed inthe flat position.This may require the fabrication of sub-assemblies that aremore easily manipulated. Manipulating equipment such as rotators or face-plate manipulators are useful for items too large for manual handling. Theuse of this equipment, however, may require the welding of temporaryattachments to the component to facilitate fitting the component to themanipulator. As much care must be taken with the welding and removal ofthese attachments as is applied to the permanent joints – formal weldingprocedures should be considered in order to exercise control over thissometimes haphazard activity.
5.5 Edge preparation and joint design
There are few more important decisions that affect the success of weldingthan that of correct joint design. Problems with weld quality or performancecan often be attributed to the wrong design of edge preparation. Jointdesign is determined by the strength requirements, the alloy, the thicknessof the material, the type and location of the joint, the access for weldingand the welding process to be used.
There are three fundamental forms of weld, the butt, the fillet and theedge weld, illustrated in Fig. 5.3, from which can be developed six basic joint types. These are the butt, T-joint, corner, cruciform, edge and lap joint,illustrated in Fig. 5.4.
The static tensile strength of these weld types is determined by the throatthickness (Fig. 5.5). The size of a fully penetrated butt weld is determinedby the thickness of weld metal deposited within the plane of the plate or
72 The welding of aluminium and its alloys
Welding design 73
5.3 Butt, fillet and edge welds.
(a) BUTT joint
(c) LAP joint
(d) CRUCIFORM joint (f) CORNER joint
(e) EDGE joint
5.4 Joint types developed from the butt, fillet and edge weld.
pipe, t1 in Fig. 5.5. No credit is taken in calculating permissible static designstress of either a butt or fillet weld for the excess weld metal, i.e. that abovethe surface of the parent metal for a butt or outside the isosceles triangleof a fillet weld as given by (t2 - t1).
74 The welding of aluminium and its alloys
5.5 Throat thickness in a butt weld: (a) full pen butt weld; (b) partialpen butt weld; (c) T-butt weld.
t1 = t2
5.6 Throat thickness in a fillet weld: (a) fillet weld; (b) mitre andconvex fillet weld.
For the fillet weld the shape of the weld and the amount of penetrationinto the root will affect the throat thickness. The effective throat thicknessis t1 in Fig. 5.6.The size of the fillet weld must be determined by the designerand should be of sufficient size to carry the load. The throat may thereforebe completely different from the material thickness.
The fillet weld may also be described as a mitre, a concave or a convexfillet. In addition the fillet weld may have unequal leg lengths. These fourtypes of fillet weld are illustrated in Fig. 5.7.
5.5.1 The butt weld
The butt weld, typical forms of which are illustrated in Fig. 5.8, is a simpleand easily designed joint which uses the minimum amount of material.Figure 5.8 also includes definitions of some of the features of a weld prepa-ration such as ‘root face’, ‘angle of bevel’ and ‘included angle’. Butt welds,as illustrated in Fig. 5.5, may also be classified as full penetration or partialpenetration.
With the conventional fusion welding processes of TIG and MIG pene-tration of weld metal into the surface of a flat plate from a bead-on-platerun is typically 3mm and 6mm respectively. To achieve a full penetrationbutt weld at thicknesses over these it is necessary for the two close square-butted edges to be bevelled, although leaving a small gap between the edgeswill increase penetration. Typical weld preparations for the variousprocesses will be found in the relevant process chapter. Butt joints may besingle or double sided – if double sided it is often necessary to back-gougeor back-grind the first side to be welded to achieve a joint that is free ofany lack of penetration.
5.7 Mitre, convex, concave and unequal leg length fillet.
76 The welding of aluminium and its alloys
Single – V
Double – V
Single – V
Double – V
Angle of bevel
Angle of bevel
Root radius Root gap
5.8 Various forms of the butt weld.
The effective size of a full penetration butt weld equals the design throatthickness, essentially the plate/pipe thickness of the thinner component. Asmentioned elsewhere no credit is taken for the weld metal cap height orroot penetration bead. Although not often used in aluminium fabricationsbecause of the need to match joint strength and base metal strength, inlightly loaded joints a partial penetration joint (Fig. 5.5b), may be accept-able. Partial penetration can be achieved by the use of a close square buttjoint or a thick root face. There are cost benefits associated with the partialpenetration joint as little or no edge preparation is required, it is econom-ical on filler metal and it is easy to assemble since the root gap does notneed to be controlled. The limitations are that radiographic interpretationis difficult due to the lack of penetration, the fatigue life is compromisedand static mechanical strength is reduced. The effective size in the case ofthe partial penetration weld is the throat of the weld minus the cap height.
Where two sections of unequal thickness are to be welded the welder’stask will be eased and the best properties, particularly fatigue, will beachieved if the thicker of the two is bevelled or tapered to match thethinner. The taper on the thicker component to achieve this should be inthe region of 4 to 1 to reduce the stress-raising effects of an abrupt changein thickness (Fig. 5.9).
The weld preparation shape may be selected to achieve root penetrationand a sound root, to permit the required pass sequence or to control weldmetal dilution from the parent metal. The MIG process can, but with diffi-culty, be used to produce a sound, defect-free penetration bead – for asound joint either a backing bar or strip needs to be used or the weld mustbe cut-back and a second side weld made. These techniques are dealt within greater detail elsewhere. The TIG process can be used to make a sound,fully penetrated root bead without a cut back or backing strip. A ‘landed’bevel joint (Fig. 5.10) is designed to enable the highest quality root pene-tration bead to be made using the TIG process. This is of use in applica-tions such as pipe butt welding, where the welds need to be single sided andto have a smooth root bead that will not hinder flow in the pipe.
Welding design 77
taper of atleast 4 : 1
Single or double sided butt weld
5.9 Suggested design for the joining of dissimilar thickness plates.
The strength of a sound, defect-free butt weld generally matches that ofthe filler metal or the annealed strength of the parent metal, as discussedin Chapter 2. The butt joint is the best in a dynamic loading environment,particularly if the excess weld metal is dressed flush. To achieve the bestproperties the two component parts require accurate alignment, whichimplies adequate tacking, jigging and fixturing.
5.5.2 Backing bars and backing strips
Although it is possible to deposit a sealing run on the reverse side of a buttweld without a back-gouge, this cannot be relied upon to give a sound,defect-free weld. Single sided joints may be welded by TIG to produce asound root pass but the conventional (non-pulsed) MIG process oftenrequires either permanent or temporary backing on which to deposit theMIG root pass. The purpose of the backing bar or strip is to support theroot pass where conditions make the control of the bead difficult. Conven-tionally, a backing bar is temporary and can be lifted away as soon as theweld has been completed, and a backing strip is a permanent part of thejoint. A backing bar or strip can greatly simplify the task of setting up the joint – for example, root gap variations are easily coped with and jointscan be self-jigging, good root bead appearance can be achieved and costscan be reduced.
A grooved temporary backing bar will produce good penetration beadshape, the groove being used as a mould for the molten weld metal. Thiswill provide a better dynamic performance than a permanent backing strip.Backing bar material can be an inexpensive mild steel but a longer life canbe obtained from the bar with less risk of contamination if stainless steel isused. Ceramic backing, provided as a flexible strip of tiles or on adhesivetape, can also be used. Copper or copper alloys should be avoided because
78 The welding of aluminium and its alloys
Rootradius 1.5 to2mm
Parallel landzero gap
Bevel angle15 to 20°
For AC-TIG welding theland should be 4.5mmmin,for DC -ve TIG and MIGthe land should be 2mmmin
5.10 ‘Landed’ single-V butt weld.
of the risk of contamination. An ungrooved backing bar will need the rootpass to be back-ground and perhaps a sealing pass to be deposited toproduce a sound weld. If TIG welding using a backing bar the weld shouldbe made with no root gap. This is necessary to prevent the TIG arc actingdirectly on and perhaps melting the backing material.
The permanent backing strip is fused into the root pass and care must betaken to select an alloy that is compatible with the parent metal and thefiller. The strip should be in the region of 4–6mm thick and tacked in posi-tion. Many extrusions in aluminium, however, can be produced with thebacking strip incorporated and in this way joint set-up is simplified. It ispossible to design the extrusions with both the backing strip built in and ofsuch a shape that the joint is self-jigging, as illustrated in Fig. 5.11.
The crevices associated with permanent backing strips result in localstress concentrations. These may reduce both impact and fatigue resistanceif the root is in a highly stressed area. The crevice may also give rise tolocalised corrosion although even in marine environments this has not beenreported as a major problem when the correct alloy has been chosen.Despite these potential drawbacks, permanent backing strips are a commonfeature in many structures used in challenging applications.
Inert gas backing can be used for critical applications such as food pro-cessing or pharmaceutical process pipework or vessels and is very usefulwhen there is no access to the back of the weld to back-gouge and seal. Anargon purge will prevent oxidation of the root penetration bead and oxidefilms being fused into the joint, giving a smooth, even TIG root bead.Typicaldesigns of backing bars and strips are given in Fig. 5.12.
Welding design 79
5.11 Typical self-jigging extrusions. Courtesy of ALCAN.
5.5.3 The T-joint
As the name infers, the T-joint (Fig. 5.4b) is one where one member is posi-tioned at approximately right angles to its partner with the most usual appli-cations being plate to plate or branch connections.The upright of the T maybe joined by a butt weld, by a fillet weld or welds or by a combination of
Suggested design of atemporary backing bar forplate or pipe less than6mm thick
5.12 Backing bar and strip designs.
the two weld types (Fig. 5.5c). The T-joint is a simple, easily designed weld-ment which, except in the case of the T-butt, requires little or no edge prepa-ration. The accuracy of the fit-up depends to a great extent on the accuracywith which the edge of the upright of the T is prepared. An irregular cutwill give a variable gap, which may result in an inadequate throat thicknessas illustrated in Fig. 5.13.
A fillet weld can present difficulties in achieving full penetration into theroot, resulting in a void being formed in the corner.This is regarded as unde-sirable, particularly in critical applications, as this lack of fusion acts as astress raiser in the root and also reduces the throat thickness. The welderneeds to be made aware of this problem as the main cause is incorrectwelder technique.
If the T-butt is a flanged joint, sufficient metal must be left that the welddoes not melt away the corner of the flange and to allow for variations infit-up. As a rule of thumb, some 2.5 to 3 times the fillet weld leg length isregarded as being adequate (Fig. 5.14). This may not prevent the edge ofthe flange from buckling due to distortion from the heat of welding, par-ticularly where the fillet size is large in proportion to the flange thickness.
The strength of a fillet welded T-joint is determined by the shear strengthof the fillet weld or welds, the strength of a butt-welded T-joint by thestrength of the weld metal or the HAZ. If the joint is subjected to trans-verse shear loads the bending stresses in the joint can lead to prematurefailure, particularly if the joint is fillet welded on one side only. Fillet weldson both sides or a full penetration T-butt joint will permit substantiallyincreased loads before failure occurs (Fig. 5.15). Dynamic performance ofT-joints is not good: the change in section from the horizontal to vertical
Welding design 81
Expected throatReduction inthroat
5.13 Effect of an irregular cut edge on the fillet weld throat thickness.
member gives rise to high stresses at the weld toes, drastically shorteningthe fatigue life.
5.5.4 The corner joint
The corner joint may be regarded as a butt joint and is used to join twoplates at right angles to each other (Fig. 5.4f). It can be difficult to assem-ble and maintain correct alignment, particularly in thin flexible sheet. Theroot of a single-sided weld when loaded in tension is very weak and for the highest strength the corner joint needs to be welded from both sides.The single-sided weld may also have a crease containing oxides along thecentre line of the penetration bead, further reducing the strength of theweld. Pulsed AC-TIG has been found to be effective in reducing the occur-
82 The welding of aluminium and its alloys
Leg length Z
5.14 Recommended distance of weld toe from the flange edge.
Poor performance Better performance
5.15 Redesign of side loaded fillet welds for improved performance.
rence of this feature. The corner joint is most often found in low load-carrying applications and in sheet metal work.
5.5.5 The edge joint
The edge joint (Fig. 5.4e) is simple to assemble and to hold in positionduring welding. Like the corner weld, it is weak in loading situations thatput the root in tension and is rarely used in a structural application, beingconfined to non-load-carrying applications in thin sheet metal. Melting ofthe corners of the edges being joined can be a problem and may result ina shallow, low throat thickness weld.
5.5.6 The lap joint
The lap joint is perhaps the easiest joint of all to assemble. It comprises twooverlapping plates joined by a fillet weld (Fig. 5.4c). Variations in compo-nent sizes are easily accommodated and no edge preparation is required,although a bevel, as in Fig. 5.16, may be used to guarantee full root fusion.
The joint is uneconomical in terms of material as the overlapping mate-rial is waste. The overlap should be at least three times the thickness of thethinner plate. Care also needs to be taken to ensure that the weld does notmelt away the corner of the upper plate as this results in a reduction in theeffective throat thickness of the fillet.
The joint strength is set by the shear strength of the fillet weld.Weld sizesand lengths should be specified by the designer to guarantee adequate load-carrying capacity.
5.5.7 Spot, plug and slot welds
Arc welded plug and spot welds are illustrated in Fig. 5.17. Both the TIGand MIG processes are capable of fully penetrating 2–3mm through theupper sheet of a lap type joint to provide an acceptable weld. Laser and
Welding design 83
Bevelling the plate edge as above assists in achieving full penetration at the root
A square edge as shown above may lead to difficulty in penetrating completely into the root, resulting in a lack of fusion defect and a reduction in throat thickness
5.16 Bevelling the plate edge in a lap joint to improve penetration.
electron beam welding are capable of spot and ‘stake’ welding through asubstantial plate thickness, in the case of electron beam up to 200mm.
TIG welding tends to be confined to thin sheet, less than 2mm thick,and finds only a very limited application in production. The bulk of spotwelding is performed using MIG welding and is covered in greater detailin Chapter 7. The designer must be aware, however, of the variable qualityof the spot weld which results in low strength and poor fatigue performance.The high restraint inherent in this weld form almost always results in distortion, particularly when the welds are close pitched, and may pro-duce hot cracks in the HAZ. These features limit the applications of spot welding.
Plug welding is similar to spot welding except that the upper plate is cutto provide a hole which is either completely filled with weld metal or is filletwelded around its rim. This type of weld suffers from the same problems ofvariable quality and inadequate strength as do the spot welds. They bothtend to be avoided when structural integrity is required.
The slot weld is rather more useful in a structural application than thespot or plug weld since there is a reasonable length of weld to be deposited.This permits a stable weld pool to be established and a sound joint to bemade. The weld may be a single pass completely filling the slot or it may befillet welded both sides. For best quality the start and stop positions shouldbe on the upper plate, clear of the slot. Fillet welded slots are preferredwhen the plate thickness exceeds 5mm. The strength of a slot weld is deter-mined by the shear strength of the weld deposit.
Residual stress due to heating and cooling of the HAZs and the contrac-tion of the weld metal as it cools from a molten state to ambient tempera-ture is an unavoidable feature of welded joints.The stress deriving from thisshrinkage results in distortion. This distortion may be localised, evenly dis-tributed and acceptable or may render the entire structure unfit for itspurpose. In a ship’s hull, for instance, buckling of the hull plates can induceturbulence and increase drag; in piping it can restrict fluid flow; and in archi-tectural applications it can be aesthetically unacceptable.
84 The welding of aluminium and its alloys
5.17 Plug and spot welds using TIG or MIG welding.
Distortion can appear as longitudinal shrinkage, transverse shrinkage,angular distortion, bowing or buckling. The various forms are shown in Fig. 5.18. The amount of distortion is affected by the heat input from thewelding process, the welding sequence, joint design, the amount the joint isrestrained, stresses in the parent metal and its physical characteristics.
Although the coefficient of thermal expansion of aluminium is abouttwice that of steel, its high thermal conductivity means that temperaturegradients are less severe. However, the change that occurs when the weldmetal solidifies is around a 5% volume shrinkage, compared with a 3%reduction in steel. The net result is that distortion in aluminium is some-what greater than would be expected in a similar steel structure. If the metalis in a highly stressed state, such as being cold worked, this will also lead togreater distortion as these stresses are released by the heat of welding.
The measures that can be taken to minimise the problem are similar tothose that would be used for steel:
• Weld on or very close to the neutral axis.• Balance the welds about the neutral axis of the component (Fig. 5.19).
Welding design 85
Transverse andlongitudinalshrinkage in abutt weld
Angulardistortion fromfillet welds
Bowing in a platedue to longitudinalshrinkage
Result of angulardistortion caused by fillet weldedlongitudinalstiffeners
5.18 Longitudinal, transverse and angular distortion. Courtesy of TWI Ltd.
5.19 Welding around the neutral axis. Courtesy of TWI Ltd.
• Where appropriate use a double-V preparation and balance the weldingabout the plate centre line (Fig. 5.20).
• Use the lowest heat input process and welding parameters, consistentwith achieving the required quality. Of the fusion welding processes thepower beam processes – electron beam or laser welding – will give theleast distortion.
• Use the fewest number of weld passes to fill the joint. This implies thata high heat input process will result in less distortion than a low heatinput process. This may seem to be in conflict with the point above butit should be remembered that it is the total heat input to the joint thatis significant.The sum of heat inputs from a large number of small passeswill result in a higher total heat input than that from a small number of large beads for the same volume of weld metal. TIG welding, forinstance, will almost always give more distortion than MIG welding thesame component.
• On long welds, weld from the centre towards the ends. On items suchas beams this will approximately halve the amount of bowing that wouldbe expected if the beam was welded by starting at one end and weldingthrough to the opposite end.
• Use a ‘back-step’ sequence, i.e. weld from a cold section of joint towardsa hot section already welded (Fig. 5.21).
• Break the construction down into sub-assemblies, weld the individualsub-assemblies and assemble the complete item, balancing any distor-tion from the individual items to minimise the overall distortion.
• Preset the components (Fig. 5.22). If the amount of distortion is knownor can be predicted, the items can be assembled and offset by theamount of expected distortion. On completion of welding the distortion
86 The welding of aluminium and its alloys
5.20 Balanced welding in a butt weld. Courtesy of TWI Ltd.
has been used to pull the items to within tolerance. This technique ismost easily used to cope with angular distortion on plates.
• Use automatic welding. This may enable faster travel speeds to be usedand hence lower heat input to be achieved. Mechanised/automaticwelding will also give more consistent distortion which enables the tech-nique of pre-setting components to be used with greater confidence.
• Use a planned welding sequence. This is of use on fabrications such aslattice beams where a planned sequence can be of great benefit. Theprecise sequence to minimise distortion will vary from assembly toassembly and is best designed from experience. Staggered welds, backstep and skip welding can also be employed.
• Use adequate tack welds. In a butt joint the contraction of the solidify-ing weld metal tends to pull together the two edges (Fig. 5.22).With thin
Welding design 87
5.21 Backstep welding. Courtesy of TWI Ltd.
5.22 Presetting of components before welding. Courtesy of TWI Ltd.
sheets this can result in the edges riding up over each other, requiring thetack welds to be more closely pitched.The length of tack welds should bein the region of 8 times the component thickness and spaced at intervalsnot greater than 35 times the thickness.They must be made with the sameprocedure and with as much care as the main weld. Tacks are expectedto carry the assembly stresses and can therefore experience high loadsthat may well cause cracking problems. Incorporation of cracked tacksin the constructional weld will be an expensive problem to eliminate!
• Ensure that the joint fit-up is accurate. This is perhaps one aspect wherethe importance cannot be over-emphasised. Large root gaps, forinstance, will always result in large amounts of distortion as the rootweld metal contracts.
• Do not over-weld and avoid the use of wide bevel angles, large root gapsand large amounts of excess metal. Fillet welds should be as small aspermitted by design – for example, an 8mm leg length fillet weld con-tains over 80% more weld metal than a 6mm leg length fillet. It is worthremembering that not only does excess weld metal increase distortion,it also costs a lot of money to deposit it!
• Use jigs and fixtures (Fig. 5.23), to hold and retain the components inthe correct alignment. The use of rigid restraints will give increasedlevels of residual stress and may increase the risk of cracking. Jigs needto be designed to provide good access for welding, to be rigid and robust,to be foolproof in use and to be well maintained to ensure that wear istaken into account and tolerances are achieved.
5.7 Rectification of distortion
If the measures listed above are not effective, remedial measures to rectifythe distortion will be necessary. These may be based upon those used forsteel but great care needs to be exercised if such techniques are used. Themost effective methods are those that use some form of mechanical workingor stretching as these will not significantly affect the mechanical properties
88 The welding of aluminium and its alloys
5.23 Jigging of plate to maintain flatness. Courtesy of TWI Ltd.
Welding design 89
of the base materials. Longitudinal bow in welded beams should preferablybe done cold by pressing, and buckled plate may be pressed flat.
As a last resort, local spot or line heating may be used to heat-shrinkitems that have been distorted by the welding of, for instance, stiffeners.Some examples of how these techniques can be applied are illustrated inFig. 5.24. The high thermal conductivity of aluminium means that localheating with an oxy-gas torch is not very effective. If this technique is to beused then electric induction heating is the most effective method of intro-ducing sufficient heat into the component.
If heat must be used then this should not exceed 400°C for the non-heattreatable alloys. Remember, though, that temperatures over 250°C willproduce full softening in the alloy if it is in the work-hardened condition.The age-hardened heat-treated alloys should not be heated to more than150°C as this will cause softening due to overageing of the precipitates.
Whenever these techniques are used then reference must be made to thedesign engineer to ensure that the potential loss of strength is taken intoaccount.
5.8 Fatigue strength of welded joints
Fatigue, as the name suggests, is a failure mechanism where the componentfails after a period of time in service where it sees a repetitive cyclic stress.Failure may occur even if this stress is substantially below the yield strengthof the metal as the other factor in causing failure is the number of stresscycles that the component experiences. Failure always occurs normal to theprincipal applied stress and the fracture surface is characterised by so-called‘beach marking’ where changes in the stress level give different rates ofcrack propagation. This gives the surface a rippled appearance similar to abeach when the tide has ebbed away. The rate of crack propagation is pro-portional to the stress range and the crack length. Cracks in the early stagesof growth tend to be very small and to grow slowly, making it easy for themto be missed during in-service inspection.
To be able to predict the fatigue life of a structure the designer needsaccurate details of the full service loading conditions and accurate fatiguedata on the performance of the component parts of the structure. The mostcommon sites for initiation are weld toes, both root and face, drilled holes,machined corners and threaded holes. Of these sites the most significant arewelds. Since welding has such a significant effect on fatigue life it will benecessary to specify welding details and controls rather more closely thanfor a statically loaded structure. This will, inevitably, have an effect on thecost of fabrication.
90 The welding of aluminium and its alloys
5.24 Rectification of distortion by (a) line, (b) wedge and (c) spotheating. Courtesy of TWI Ltd.
Fatigue performance can be represented graphically on an S/N curvewhere ‘S’ is the stress and ‘N’ the number of cycles to failure. For unweldedcomponents a fatigue limit is reached where below a certain stress failurewill not occur, irrespective of the number of cycles of stress it sees.A weldedjoint, however, does not exhibit a fatigue limit – failure will always occur ifenough stress cycles are applied. These points are illustrated in the S/Ncurve in Fig. 5.25.
Welding results in a substantial reduction in the fatigue life and an elim-ination of the fatigue limit. This is such a dominant effect that there is littledifference in fatigue life between the various alloys and tensile strength inthis context is, to a great extent, irrelevant. The presence of welding defectswill have an additional adverse effect, particularly those defects that maybe classified as planar. Abrupt changes in section, notches and corners allreduce the fatigue life. Poorly shaped welds where there is a poor toe blendwith the excess weld metal meeting the parent metal at a sharp angle (seethe convex fillet in Fig. 5.7 as an example) are significant stress raisers. Forthe best fatigue performance the welds should be smoothly blended withno abrupt changes on section.
The corollary of this is that the form and shape of the weld will have amajor effect on fatigue performance. Many specifications categorise thevarious weld forms and the direction of loading with respect to the fatiguelife as shown in Table 5.1 parts a and b.
Apart from the need to ensure that the welds are smooth and wellblended the orientation of the welded item to the principal stress needs tobe taken into account. Fatigue improvement techniques comprise, firstly,eliminating the weld if possible or moving it to an area of lower stress.Redesign to a joint type with a higher category should be considered. If this
Welding design 91
105 106 107 108
Unwelded. This line becomes asymptotic
Welded joint,This line trendsdown to zero
‘N ’, number of cycles (log scale)
5.25 Stress/no. of cycles curve for alloy 5083.
Table 5.1a Fatigue classification of welded details
Fillet or butt Calculate peak stresses 24 (depends F or Wwelded nodal joint acting on the joint on loading
Fillet and partial Weld throat is used to 43 (automatic Wpenetration butt calculate stress welds)welds in 35 (multiplelongitudinal shear stop/starts)
Table 5.1b Fatigue life prediction for welded items from BS 8118
cannot be done then thickening the component will reduce the stress expe-rienced by the weld. The fatigue life of the weld can be improved by induc-ing compressive stresses at the toe of the weld. Overstressing the joint orhammer peening the weld toe will both do this, although great care needsto be taken that an over-enthusiastic application of either technique doesnot introduce defects. Dressing of the weld toes has been found to be aneffective method but, once again, over-enthusiastic grinding can reducerather than improve fatigue life. If the weld toes are ground this should becarried out by fully trained personnel. Grinding should be performed trans-verse to the weld toes in order that the grinding marks are parallel with theprincipal stress.
96 The welding of aluminium and its alloys
Tungsten arc inert gas shielded welding, EN process number 144 abbrevi-ated to TIG, TAGS or GTAW (USA), is an arc welding process that uses anon-consumable tungsten electrode and an inert gas shield to protect theelectrode, arc column and weld pool, as illustrated in Fig. 6.1. The weldingarc acts as a heat source only and the welding engineer has the choice ofwhether or not to add a filler wire. The weld pool is easily controlled suchthat unbacked root passes can be made, the arc is stable at very low weldingcurrents enabling thin components to be welded and the process producesvery good quality weld metal, although highly skilled welders are requiredfor the best results. It has a lower travel speed and lower filler metal deposi-tion rate than MIG welding, making it less cost effective in some situations.
TIG tends to be limited to the thinner gauges of aluminium, up toperhaps 6mm in thickness. It has a shallower penetration into the parentmetal than MIG and difficulty is sometimes encountered penetrating intocorners and into the root of fillet welds. Recommended weld preparationstaken from BS 3019 ‘TIG Welding of Aluminium’ are given in Table 6.1.
6.2 Process principles
The basic equipment for TIG welding comprises a power source, a weldingtorch, a supply of an inert shield gas, a supply of filler wire and perhaps a water cooling system. A typical assembly of equipment is illustrated inFig. 6.2.
For welding most materials the TIG process conventionally uses directcurrent with the electrode connected to the negative pole of the powersource, DCEN. As discussed in Chapter 3 welding on this polarity does notgive efficient oxide removal. A further feature of the gas shielded arcwelding processes is that the bulk of the heat is generated at the positivepole. TIG welding with the electrode connected to the positive pole, DCEP,
Filler wire –if required
Weld pool Solidifiedweld metal
Gas shieldCeramic gasshroud
6.1 Schematic of the TIG welding process.
Table 6.1 Suggested welding preparations for TIG welding from BS 3019
Thickness Edge preparation Remarks(mm)
20swg = Flanging should 0.9mm and be used only 16swg = where square 1.6mm edge close butt
welds are impracticable
3.8mm Where a backing bar cannot be used, welding from both sides is recommended
6.4mm If no backing bar is used, it is goodpractice to chip back to sound metal and add sealing run
9.5mm (a) If no backing bar is used, chip back to sound metal and add sealing run(b) Chip back firstrun to sound metal before welding underside
70° to 90° 70° to 90°
0.8 mm 2.4 mm
(a) 2 or 3 runs (b) 2 or more runs
70° to 90°
1.6 mm1 or 2 runs
70° to 90°
6.2 Manual DC-ve TIG welding repair of aluminium castings usinghelium shielding gas. Courtesy of TPS-Fronius Ltd.
Table 6.1 (cont.)
Thickness Edge preparation Remarks(mm)
12.7mm (a) Chip back firstrun to sound metal before welding underside. Preheating may be necessary(b) Chip back firstrun to sound metal and add sealing run.
Preheating may be necessary
(a) 4.8–6.4mm Preparation for(b) Over vertical butt welds
6.4–12.7mm using double operator technique. One pass only required
2.4 mm 2.4 mm
70° to 90°60°
2.4 mm 2.4 mm
(a) 2 or more runs (b) 4 or more runs
results in overheating and melting of the electrode. Manual TIG welding ofaluminium is therefore normally performed using alternating current, AC,where oxide film removal takes place on the electrode positive half cycleand electrode cooling and weld bead penetration on the electrode negativehalf cycle of the AC sine wave. The arc is extinguished and reignited everyhalf cycle as the arc current passes through zero, on a 50Hz power supplyrequiring this to occur 100 times per second, twice on each power cycle.To achieve instant arc reignition a high-frequency (HF), high-voltage (9–15000V) current is applied to the arc, bridging the arc gap with a continu-ous discharge. This ionises the gas in the arc gap, enabling the welding arcto reignite with a minimum delay (Fig. 6.3). This is particularly importanton the DCEP half cycle.
Aluminium is a poor emitter of electrons, meaning that it is more diffi-cult to reignite the arc on the electrode positive half-cycle. If there is anydelay in reignition then less current flows on the positive half cycle than onthe negative half cycle. This is termed partial rectification and can eventu-ally lead to full rectification where no current flows on the positive halfcycle. The arc becomes unstable, the cleaning action is lost and a directcurrent component may be produced in the secondary circuit of the powersource, leading to overheating of the transformer.This is prevented on olderpower sources by providing an opposing current from storage batteries andin more modern equipment by inserting blocking condensers in the powersource circuit.
The HF current is operating continuously when the arc is burning in theAC-TIG process. An important word of caution relates to this – the HFcurrent can track into other equipment in the vicinity of the arc and
100 The welding of aluminium and its alloys
HF sparks Arc voltage
Voltage across arc gapWelding currentOpen circuit voltage
+ ++ + ++– – – – – – – –
+ + + + +
6.3 HF current and its effect on voltage and current.
can seriously damage electronic circuits, can cause malfunctions and uncontrolled movements of robotic systems and NC machines and canaffect the functioning of telephones and computer networks. Where HFcurrent is used precautions must be taken to prevent damage by adequateshielding of equipment and electronic circuits, perhaps by the use of aFaraday cage.
6.2.1 Square wave power sources
The most modern equipment (Fig. 6.4) uses solid state circuitry and iscapable of providing a square wave AC current rather than the sinusoidalwave form of the older equipment. These power sources can be adjusted tovary the wave frequency and the balance of positive and negative current
TIG welding 101
6.4 Inventor-based multi-function MMA/TIG power source capable ofproviding square wave AC for the welding of aluminium. Courtesy ofKemppi (UK) Ltd.
by shortening or extending the length of time spent on the positive or negative half cycle. The latest inverter-based units provide a high degree ofcontrol with the electrode negative duration time capable of being adjustedfrom 50% to 90% of the cycle. Increasing the frequency results in a morefocused arc, increasing penetration, enabling faster travel speeds to be usedand reducing distortion. Increasing the electrode negative portion of thecycle will give similar results of increased penetration and faster travelspeed although the cathodic cleaning effect will be reduced. Biasing thesquare wave more towards the electrode positive half cycle will reduce pen-etration, useful when welding thin materials, and will widen the bead profile.
Another very important difference between older units and the inverter-based power sources is that the square wave cycle passes through the zerowelding current point many times faster than with a sinusoidal wave. It ispossible to dispense with continuous HF current for arc stabilisation,removing the risks of damaging sensitive electronic equipment. High frequency will still be needed to initiate the arc, however, so a small riskremains. The lack of continuous high frequency may also result in an un-stable arc on very clean, etched surfaces or on the weld metal. Inverterpower sources are also capable of overcoming a problem encountered whenusing two arcs close together. Welding current can track from one powersource to the other, damaging the circuitry. With the very latest equipmentthe two arcs are matched.
Square wave power sources have a further advantage in that tungsten‘spitting’, where the electrode tip spalls off and contaminates the weld pool,can be reduced. Reducing the electrode positive portion will reduce theoverheating that causes tungsten spitting.
6.2.2 Shielding gas
The preferred gas for the AC-TIG welding of aluminium is argon, althoughhelium and argon–helium mixtures may be used. Argon gives a wide,shallow penetration weld bead but will leave the weld bright and silvery in appearance. The easiest arc ignition and most stable arc will also beachieved with argon. Typical butt welds in 3mm and 6mm plate are illus-trated in Fig. 6.5 and a fillet weld in 6mm thick plate is shown in Fig. 6.6.A table of suggested welding parameters for use with argon as a shield gasis included as Table 6.2. Typical current ranges for a range of plate thick-nesses are illustrated graphically for butt welds in Fig. 6.7 and for fillet weldsin Fig. 6.8.
Helium increases arc voltage with the effect of constricting the arc,increasing penetration but making arc ignition more difficult, and adverselyaffecting arc stability. Some of the modern welding power sources areequipped with a facility to start the weld with argon and, once a stable arc
102 The welding of aluminium and its alloys
6.5 AC-TIG argon shielded (a) unbacked 3mm sheet, single pass, flatposition; (b) unbacked 6mm thick plate, two pass, flat position.
6.6 AC-TIG argon shielded, 6mm thick plate, single pass,horizontal–vertical.
0 50 100 150 200 250 300 350 400
WELDING CURRENT (A)
6.7 Typical TIG current ranges for various material thicknesses.
104 The welding of aluminium and its alloys
0 50 100 150 200 250 300 350 400
TIG WELDED FILLET JOINTS
6.8 Typical TIG welding parameters for fillet welding.
Table 6.2 Suggested welding parameters – argon gas shielding
Thickness Joint Root Current No. of Filler Travel Nozzle(mm) type gap (A) passes diam. speed diam.
1. The conditions shown are for the PA (flat) position. A reduction in current ofaround 10% should give acceptable parameters for other positions.2. The thickness is limited to 10mm. Above this the TIG process is rarely usedbecause of economic considerations.
is established, for an automatic change-over to helium to be made. For com-parison purposes with the argon shielded welds typical cross-sections ofbutt welds in 3mm and 6mm thick plate and a fillet weld in 6mm thick plateare shown in Fig. 6.9 and Fig. 6.10. In the UK helium is a more expensivegas than argon – some five to six times more – and provides little or no arccleaning action. Indeed, in some circumstances, the use of helium can resultin ‘soot’ being deposited in the HAZ and although this may normally beremoved by wire brushing, it can be difficult to remove. For these reasons100% pure helium is rarely used in manual AC-TIG welding.
The addition of argon to helium improves arc striking and arc stability.Travel speeds and penetration will be less than with pure helium but greaterthan with argon. It is possible to control bead width and penetration byvarying the amount of argon in the mixture. The most popular mixture inthe UK is 25% helium in argon.
The power source controls should provide for both pre-flow and post-flowof the shield gas. A pre-flow is used to purge the hoses and the torch and toprotect the electrode when the arc is established. Maintaining the flow of gaswhen the weld is terminated is also necessary to protect both the weld pooland the electrode from oxidation as they cool from welding temperature.Gas flow rates are important in ensuring adequate gas coverage. ‘Bobbin’type flow meters are often used attached to the regulator to control flow.Anyrestriction between the bobbin meter and the torch means that the flow ratewill not be set accurately. It is a good idea to validate meter readings by attaching a flow meter to the torch gas shroud and monitoring the flow.Flow meters are also calibrated for a specific gas and will give inaccuratereadings if they are used to control the flow of other gases or gas mixtures.This is particularly important when using helium or argon–helium mixtures.
6.2.3 Welding torches and cables
There is a wide variety of welding torches available with torch ratingsranging from some tens of A to 450 A, the appropriate rating dependingessentially on the thickness of the metal to be welded. Most of the moderntorches (Fig. 6.11), are provided with current controls built into the torchhandle. All but the lightest torches, i.e those rated to operate below around200 A, are water cooled and the same water may be used to cool the powercables, enabling them to be lighter and more flexible.
Overheating of the torch can melt the brazed joints within the torch orthe plastic tube that sheaths the power cable and it is important that
106 The welding of aluminium and its alloys
6.10 DC-TIG helium shielded, unbacked 6mm thick plate, single pass,horizontal–vertical.
the correctly rated torch is selected for the current to be used in produc-tion. The manufacturer’s rating for a torch may be based on DC-positivecurrent and a torch rated in this way will need to be de-rated when usedwith AC.
Most of the torches can be fitted with either metal or ceramic gas shroudsalthough the ceramic shrouds are the most popular. They are, however,rather more easily damaged than the metal shrouds. Nozzle sizes for a rangeof thicknesses and gas flow rates are given in Table 6.3. It is recommendedthat a device known as a gas lens is fitted to welding torches. This is a meshdisc inserted into the torch which assists in providing a more efficient,laminar flow gas shield with better coverage. The beneficial effect of a gaslens is illustrated in Fig. 6.12.
TIG welding 107
6.11 Modern TIG torch. Courtesy of TPS-Fronius.
Table 6.3 Suggested nozzle sizes and gas flow rates
Material thickness Gas nozzle diameter Shield gas flow rates(mm) (mm)
Argon Helium(l/min) (l/min)
up to 1 9.5 3.4 7.51 to 3 9.5 4.5 9.53 to 5 12.5 5.6 11.85 to 9 12.5 7.0 14.29 to 12 16.0 8.0 16.512 and above 25.0 12.0 21.0
6.2.4 Tungsten electrodes
There are several types of electrodes available for TIG welding. Theseinclude pure tungsten and tungsten alloyed with thoria (ThO2) or zirconia(ZrO2). These compounds are added to improve the arc starting charac-teristics, to stabilise the arc and to extend the electrode life. Recently therehas been a move towards the use of other rare earth elements such ascaesium, cerium or lanthanum, which are claimed to extend the electrodelife further and will reduce the radiation risk arising during the grinding ofthoria containing electrodes. Zirconiated electrodes are preferred for AC-TIG welding since these have a higher melting point than either pure tung-sten or thoriated tungsten electrodes and can therefore carry higher weldingcurrents, are more resistant to contamination and are less likely to spall.
The electrode tip assumes a hemispherical shape during welding. It isimportant that this shape is maintained if a stable arc is to be achieved. The
108 The welding of aluminium and its alloys
6.12 Demonstration of laminar flow by use of gas lens. Courtesy ofTWI Ltd.
electrode tip should be lightly tapered to assist in the formation of therounded tip as illustrated in Fig. 6.13.
Too small an electrode for the current will lead to overheating and possibly melting, resulting in tungsten contamination of the weld pool. Toolarge an electrode for the current will result in arc stability problems and a very wide weld pool. Electrodes are available in diameters ranging from0.3mm to 6.4mm. Recommended electrode diameters and welding currentsare given in Table 6.4. The electrode should not protrude from the nozzleby more than about 6mm, although this may be extended by up to 10mmif a gas lens is fitted to the torch. This extension can be useful if access isrestricted because of the ceramic nozzle fouling on the component.
Before production welding is started it is recommended that the elec-trode is preheated by forming an arc on a piece of aluminium scrap. Thisenables the rounded tip to be formed, allows the welder to check that theelectrode is performing correctly and enables the arc to be reignited on theproduction component with ease. If the tip becomes contaminated or isdamaged in any way it should be reground and reformed as above.
Table 6.4 is for square wave AC-TIG with a balanced wave form. If the current is biased to give a greater proportion of positive current thevalue will need to be reduced by an amount appropriate to the amount ofimbalance in the wave form. If using a conventional balanced sine wavecurrent then these values should be reduced by around 25%.
TIG welding 109
D 0.4D radius
6.13 Recommended tungsten electrode shape.
Table 6.4 Recommended electrode diameters –zirconiated tungsten electrodes and argon shield gas
The welder should attempt to maintain the shortest practicable arc length.In practice this is approximately equal to the electrode diameter. If the arcis too long penetration is decreased and the risk of lack of fusion defects isincreased. Undercutting, poor bead shape and excessive bead widths mayalso be produced. Gas shielding may also be affected with entrainment ofair into the shield gas giving oxide inclusions in the weld.
The torch should be held normal to the weld but pointing forwardstowards the direction of travel, at an angle of around 80°. When weldingjoints of unequal thickness the arc should be directed more towards thethicker side of the joint. For fillet welds the torch should bisect the anglebetween the two plates. Weaving of the torch may be carried out but theweave width should be restricted to the diameter of the nozzle.
188.8.131.52 Filler rods
The filler rod, if used, should be fed into the leading edge of the weld poolwith a slow, ‘dabbing’ action at an angle of 10–20° (Fig. 6.14). It should notbe fed directly into the arc column as this tends to cause spatter and mayaccidentally contaminate the electrode. A steeper angle than 10–20°restricts the welder’s view of the weld pool. The tip of the filler rod shouldbe held inside the gas shield while it is hot to prevent oxidation.As the com-ponent thickness increases the filler rod diameter increases, necessitatingan increase in arc length. Bear in mind that too long an arc can cause oxideentrapment problems. A large diameter rod can also shield the materialahead of the weld pool from the cleaning action of the arc and this mayalso lead to oxide entrapment.
110 The welding of aluminium and its alloys
10 to 20°
6.14 Angle of torch and wire workpiece.
184.108.40.206 Root bead penetration
It is possible to produce fully fused root beads without backing using AC-TIG. Up to 3mm thickness the weld can be made without a weld prepara-tion but above this a V- or U-preparation will be necessary to achieve fullfusion. Root gaps should be avoided. A skilled welder will use the appear-ance of the weld pool to judge when a fully penetrating root bead has beenproduced. When full penetration has been achieved the weld pool will sinkand will have a bright shiny surface. A U-preparation will make it easierfor the welder to judge when this happens. In thicker material when usinga V-preparation the arc tends to favour the side walls instead of actingdirectly on the root, sometimes leading to lack of fusion type defects.An alternative to a U-preparation that avoids this problem is to use a V-preparation with an included angle of at least 90°.When welding root passesin position, particularly overhead, root concavity or ‘suck-back’ is aproblem. This requires the filler rod to be pushed into the weld pool todisrupt the oxide film and to form a convex bead.
The oxide film that causes suck-back is also responsible for a featureknown colloquially as a ‘baby’s bottom’, a very accurate description of the appearance of this root defect (Fig. 6.15). Oxides tend to migrate to the centre of the root penetration bead. When these become excessive thecentre of the bead sinks to produce a deep groove along the centre line thatmay also be associated with hot cracking. In butt welds a very wide weld
TIG welding 111
6.15 Oxide intrusion and cracking associated with suck-back.
bead caused by a large root gap or a high welding current will also con-tribute. This defect is particularly prevalent in corner joints in thin sheetassemblies and is caused by a failure to clean the weld preparations and thefiller wire adequately. It has been found helpful to use unbalanced squarewave AC to increase the arc cleaning action and pulsed square wave AC,with a heavy bias towards DC positive, has been successfully used in particularly troublesome applications.
Permanent backing strips may be used to simplify root bead control.These require a very good fit-up between the underside of the plates andthe backing strip to prevent lack of fusion or suck-back type defects. Toachieve good penetration into the backing strip there must be a root gapof at least 1.5 times the electrode diameter and this gap must be maintainedalong the full length of the component. This means that the joints must beadequately tack welded together.
220.127.116.11 Weld termination
Controlled finishing of a weld pass is important if defects are to be avoided.Abruptly switching off the welding current can cause craters, piping (elon-gated pores) and cracks in the finished weld pool. When finishing the weldit is necessary to reduce the welding current gradually and to decrease thearc length as the arc fades away, adding filler rod until such times as the arcis extinguished. If a crater begins to form the arc should be briefly re-established, additional filler metal added and the arc decayed as before. Onthin material the travel speed may be increased to a point at which it canbe seen that the metal has ceased to melt.
6.2.6 DCEN helium TIG welding
Welding aluminium with the electrode connected to the negative pole canbe carried out using helium as the shield gas. This gives a higher tempera-ture arc and increased penetration compared with AC-TIG but the oxideremoval action of the positive arc is absent. This means that cleaning of theitem to be welded assumes even more importance than when using AC.Thehigher heat input and the deeper penetration means that higher travelspeeds can be used and a wider range of thicknesses may be welded thanwith AC-TIG, although the high travel speeds do mean that the process israrely used in a manual context but is almost entirely mechanised. Typicalsingle pass welds using helium as the shield gas are illustrated in Fig. 6.9(butt welds) and Fig. 6.10 (fillet weld). Note in particular the wider andmore deeply penetrating fillet weld bead compared with argon shielding.Suggested welding parameters for butt and fillet welding using helium aregiven in Table 6.5.
112 The welding of aluminium and its alloys
Unlike AC-TIG where zirconiated electrodes are preferred, the best elec-trodes for DCEN welding are thoriated tungstens, which permit easier arcstarting, maintain their tip shape longer and result in less tungsten spitting.The tip of the electrode should be tapered at an angle of 45° and the endblunted by grinding on a flat of about half the electrode diameter. A longtapered tip can result in shield gas turbulence, poor weld profiles and undercutting.
Wire feeding differs from that used in AC-TIG welding in that the wiretip should be fed into the weld pool by pushing the still solid wire into thepool and then withdrawing it when a sufficient amount of filler wire hasbeen added, keeping the wire tip within the gas shield. The torch is thenmoved forward and a fresh weld pool established. This discontinuousmethod of welding assists in piercing the oxide skin on the weld pool surfaceand in increasing penetration. With temporary backing bars this techniqueenables square edge butt joints to be welded at thicknesses of up to 9mm,provided that the welder has sufficient skill. Double sided square edge buttwelds can be made successfully at up to 12.5mm thickness.Above this thick-ness then a ‘V’ or preferably a ‘U’ preparation needs to be used to enable
TIG welding 113
Table 6.5 Suggested parameters – DC-ve helium shielded gas welding
Thickness Joint Root gap Current Voltage No. of Filler Travel(mm) type /face (mm) (A) (V) passes diam. speed
1. Ceramic nozzle size should be 12.7 mm.2. The parameters shown are for welding in the PA (flat) position for the butt welds and the PB (horizontal) position for the fillets.
single sided unbacked butt joints to be made. It is recommended that anelectrode with a fully tapered tip is used to concentrate the arc into the rootof the joint when a weld preparation is to be welded.
One feature seen with helium shielded arc welding, which often givescause for concern, is the formation of a black ‘soot’ along the heat affectedzones of the weld. This ‘soot’ is not detrimental to the weld quality and caneasily be removed by stainless steel wire brushing. If left in place betweenpasses it can affect arc stability and is unsightly on a completed weld.
6.3 Mechanised/automatic welding
Automation or mechanisation of the TIG process can have a number of benefits.These include the ability to use faster travel speeds, resulting in lessdistortion and narrower heat affected zones; the better and more consistentcontrol of the welding parameters enables very thin sheet material to bewelded; there is a greater consistency in the weld quality; and it is possibleto employ operatives with a lesser degree of skill and dexterity than isrequired for manual welding. There are, as ever, some drawbacks to the useof mechanisation,not least of which is the need to provide the welding fixturewith far more accurate and consistent weld preparations than are requiredby the manual welder.Accurate joint fit-up and alignment is crucial to achiev-ing consistently high weld quality. Jigs and fixtures also need to be capableof holding the components within tight tolerances and of maintaining thesetolerances as welding proceeds. As an example, autogenous welding of thin(say 3mm) plate requires root gaps to be maintained at 0–0.025mm and plateedges to be aligned to better than 0.05mm if root penetration problems areto be avoided. Adding filler wire will assist in increasing the permissible tolerances but at the expense of welding speed. It is possible to developwelding procedures that will provide an acceptable unbacked root pass, butin many welding fixtures a removable backing bar is part of the clampingsystem.This greatly simplifies the task of setting up the joints accurately andin achieving a sound root and is to be recommended.
Although the parameters of welding current and voltage require con-trolling within small tolerance bands, the parameters of wire feed speed andtravel speed are far more significant.Variations in wire feed speed may leadto either underfill if the feed speed slows or overfill and lack of fusion orpenetration defects if the wire feed speed increases. Too slow a wire feedspeed can also result in the wire ‘balling back’ and prevent a smooth meltingof wire into the pool.
Automation or mechanisation of both AC-TIG and DCEN helium TIGwelding may be achieved by adapting the manual techniques using con-ventional manual equipment attached to manipulating equipment such ascrawler tractors. The task of mechanisation is simplified if the weld is
114 The welding of aluminium and its alloys
autogenous and a wire feed is not required, although this can be easily pro-vided from a spool of wire fed from a cold wire feed unit. The wire shouldbe fed into the leading edge of the weld pool at a similar angle to that usedin manual welding. Both the start of the wire feeding and carriage travelshould be delayed until the weld pool is well established. When ending theweld the current should be tapered down and the wire feed speed adjustedto provide crater filling.
DCEN helium TIG is ideally suited to mechanisation since full advan-tage can be taken of the increase in travel speed, which may be up to 10times that of an argon shielded AC-TIG weld. It is also possible to weldthick plates, up to 18mm thick, in a single pass, square edge preparationwith no filler metal, making this a very cost-effective method. The hightravel speeds possible with the technique may lead to undercutting, partic-ularly if the welding current is increased in the expectation that this willpermit even higher travel speeds to be achieved. Short arc lengths are nec-essary when autogenous welding, typically 0.8–1.5mm, and in some cir-cumstances the electrode tip may be below the surface of the plate with thearc force depressing the weld pool surface. Contraction during cooling willcause upsetting to occur, resulting in a local thickening of the joint and providing sufficient excess weld metal that the joint is not underfilled.
6.4 TIG spot and plug welding
By overlapping two plates a spot weld can be achieved by using the DCENTIG process to fuse through the top plate and melt into the lower plate.Initial use of the process was carried out without a filler wire but hot crack-ing problems with the alloys meant that it was confined to pure aluminiumup to 2mm thick. The development of automatic wire feeding systemscapable of feeding wire into the weld pool as the weld is terminated hashelped in extending the range of alloys that could be welded. Even withthis improvement, however, it has been found that the critical nature of thesurface condition causes welding defects such as oxide films.This means thatthe process does not find general use because of low strength and poorquality.
Further work has taken place using fully automated equipment andhelium shield gas and with low-frequency AC. These improvements haveresulted in a wider use of the process but MIG spot welding tends to bepreferred as providing better and more consistent quality.
TIG welding 115
The metal arc inert gas shielded process,EN process number 131,also knownas MIG, MAGS or GMAW, was first used in the USA in the mid 1940s. Sincethose early days the process has found extensive use in a wide range of indus-tries from automotive manufacture to cross-country pipelines. It is an arcwelding process that uses a continuously fed wire both as electrode and asfiller metal, the arc and the weld pool being protected by an inert gas shield.It offers the advantages of high welding speeds, smaller heat affected zonesthan TIG welding, excellent oxide film removal during welding and an all-positional welding capability. For these reasons MIG welding is the mostwidely used manual arc welding process for the joining of aluminium.
7.2 Process principles
The MIG welding process, illustrated in Figs. 7.1 and 7.2, as a rule uses directcurrent with the electrode connected to the positive pole of the powersource, DC positive, or reverse polarity in the USA. As explained inChapter 3 this results in very good oxide film removal. Recent power sourcedevelopments have been successful in enabling the MIG process to be alsoused with AC. Most of the heat developed in the arc is generated at thepositive pole, in the case of MIG welding the electrode, resulting in highwire burn-off rates and an efficient transfer of this heat into the weld poolby means of the filler wire. When welding at low welding currents the tipof the continuously fed wire may not melt sufficiently fast to maintain thearc but may dip into the weld pool and short circuit.This short circuit causesthe wire to melt somewhat like an electrical fuse and the molten metal isdrawn into the weld pool by surface tension effects. The arc re-establishesitself and the cycle is repeated. This is known as the dip transfer mode ofmetal transfer. Excessive spatter will be produced if the welding parame-ters are not correctly adjusted and the low heat input may give rise to lack-
of-fusion defects. At higher currents the filler metal is melted from the wiretip and transferred across the arc as a spray of molten droplets, spray trans-fer.This condition gives far lower spatter levels and deeper penetration intothe parent metal than dip transfer. When MIG welding aluminium the lowmelting point of the aluminium results in spray transfer down to relativelylow welding currents, giving a spatter-free joint.
The low-current, low-heat input dip transfer process is useful for thewelding of thin plate or when welding in positions other than the flat (PA)
MIG welding 117
7.1 Fundamental features of the MIG process. Courtesy of TWI Ltd.
7.2 Illustrating the general arrangement of the power source, wirefeeder gas cylinder and work area. Courtesy of TWI Ltd.
position (see Fig. 10.3 for a definition of welding positions). It has, however,been supplanted in many applications by a pulsed current process, where ahigh current pulse is superimposed on a low background current at regularintervals. The background current is insufficient to melt the filler wire butthe pulse of high current melts the filler metal and projects this as a sprayof droplets of a controlled size across the arc, giving excellent metal trans-fer at low average welding currents.
Table 7.1 lists the likely and/or commonest methods of metal transferwith respect to wire diameter. Figure 7.3 illustrates the typical currentranges for a range of wire diameters.
118 The welding of aluminium and its alloys
Table 7.1 Metal transfer modes and wire diameter
Metal transfer mode Wire diameter
Dip 0.8mmPulsed 1.2 and 1.6mmConventional spray 1.2 and 1.6mmHigh-current spray 1.6mmHigh-current mixed 2.4mmspray/globular
7.3 Typical welding current ranges for wire diameter and weldingcurrent.
7.2.1 Power sources
The MIG arc requires a power source that will provide direct current andwith a suitable relationship established between welding current andvoltage, this relationship being known as the power source dynamic char-acteristic.As mentioned above the MIG process uses a continuous wire feedand for the majority of welding operations it is important that the rate atwhich the wire burns off in the arc is matched by the wire feed speed. Failureto do this can result in an unstable arc and variable weld quality. To achievethis control many MIG/MAG welding power sources are designed with aflat or constant voltage characteristic. The importance of this characteristicbecomes apparent when we consider what happens during manual welding.The manual welder cannot maintain a fixed invariable arc length whilewelding – an unsteady hand or repositioning himself during welding meansthat the arc length varies and this in its turn causes variations in arc voltage.When this happens with a flat characteristic power source a small increasein the arc length results in an increase in arc voltage, giving a large drop inarc current, as illustrated in Fig. 7.4. Since the wire burn-off rate is deter-mined by the current this also decreases, the tip of the wire moves closerto the weld pool, decreasing the voltage and raising the current as it doesso. The burn-off rate therefore rises, the arc length increases and we havewhat is termed a self-adjusting arc where a constant arc length and fillermetal deposition rate are maintained almost irrespective of the torch movement.
During both dip and spray transfer the speed at which the power sourceresponds to the changes in the arc length is determined by the inductance
MIG welding 119
Small change in voltage
Large change in current
7.4 Schematic of the effect of arc voltage vs arc current. Flatcharacteristic power source.
in the welding circuit. This controls the rate of current rise or fall and canhave a significant effect on weld quality. Insufficient inductance permits thewelding current to rise extremely rapidly, giving rise to excessive spatterand burning back of the wire to the contact tip. Too high an inductancemeans that the wire does not melt sufficiently rapidly and the wire tip maystub into the weld pool or be pushed through the root pass to protrude fromthe root. It is essential therefore that the power source is adjusted for thecorrect amount of inductance when, for example, the wire diameter or wirefeed speed is changed.
The converse of the flat characteristic power source is the drooping char-acteristic or constant current power source, illustrated in Fig. 7.5. This designof power source is generally used in MMA and TIG welding but it also hassome advantages when MIG welding aluminium. With a drooping charac-teristic a large change in arc voltage results in only a small change in arccurrent. Heat input is therefore reasonably constant, unlike that from a flatcharacteristic power source arc, giving more consistent penetration.
The problem with the drooping characteristic power source when usedfor MIG welding is that it requires more skill on the part of the welder.With push wire feeders the soft aluminium wire can buckle within the wirefeed conduit, particularly with long and flexible conduits. This results in thewire feed speed at the contact tip fluctuating and, if no action is taken, vari-ations in the heat input to the weld. When using a flat characteristic power
120 The welding of aluminium and its alloys
Small change in current
Large change in voltage
7.5 Schematic of effect of arc voltage vs arc current. Droopingcharacteristic power source.
source these fluctuations are compensated for by the power source and thewelder may not appreciate that this is occurring – with the drooping char-acteristic the arc length changes and the welder may experience what areperceived as arc stability problems. If the welder is sufficiently skilled, cor-rective action can be taken before this results in welding defects, whereaswith the flat characteristic power source the welder can produce lack offusion or excess penetration defects unknowingly. An advantage of thedrooping characteristic power source is that as the welding current and thewire feed speed are fixed the welder can employ these features to enablethe wire tip to be pushed into the joint, a useful feature when making theroot pass.
The drooping characteristic unit is also useful in deep weld preparations.In such joints the constant voltage power source may measure the arcvoltage from the side wall, rather than from the bottom of the weld prepa-ration, resulting in an unstable arc condition, poor bead shape and variablepenetration.The same restrictions apply when welding the root pass in filletwelds where a drooping or constant current unit may give better resultsthan the constant voltage power source. Weaving of the torch may alsocause problems where the torch is moved simply by pivoting the wrist. Thisgives a regular increase and decrease in arc length, causing a loss of pene-tration at the limits of the weave with the flat characteristic power source.However, despite the apparent advantages of a drooping characteristicpower source the bulk of MIG welding units in production today use a flatcharacteristic with consistent and acceptable results.
18.104.22.168 Pulsed MIG welding
Pulsed MIG welding was developed in the early 1960s but it was not untilthe late 1970s that the process began to be widely adopted on the shop floor.Prior to this date the equipment had been expensive, complicated and difficult to set up for optimum welding parameters, making it welder-unfriendly and impeding its acceptance by the most important individualin the welding workshop. Solid state electronics started to be used inwelding power sources in the 1970s and ‘single knob’ control became pos-sible with the advent of synergic logic circuits. The synergic capabilityenabled all of the welding parameters to be controlled from a single dialcontrol which optimised the current peak pulse and background values, thevoltage and the wire feed speed. It has also became possible to repro-gramme the power source instantly when wire size, shield gas, filler metalcomposition, etc. are changed, simply by dialling in a programme number(Fig. 7.6). These programmes have been established by the equipment man-ufacturer with the optimum parameters for the application. Initially theseunits were expensive but the price has been steadily reduced such that they
MIG welding 121
are now only marginally more costly than a conventional power source,leading to a far wider usage. The modern inverter-based units (Fig. 7.7), arealso far lighter, far more energy efficient and more robust than the olderunits that they are replacing.
The pulsed MIG process uses a low ‘background’ current, sufficient tomaintain the arc but not high enough to cause the wire to melt off. On thisbackground current a high-current, ‘peak’ pulse is superimposed. Underoptimum conditions this causes a single droplet of molten filler wire to beprojected across the arc into the weld pool by spray transfer. It is thus pos-sible to achieve spray transfer and a stable arc at low average welding cur-rents. This enables very thin metals to be welded with large diameter wireswhere previously very thin wires, difficult to feed in soft aluminium, neededto be used.The lower currents also reduce penetration, useful when weldingthin materials and also enable slower welding speeds to be used, making iteasier for the welder to manipulate the torch in difficult access conditionsor when welding positionally.
The use of electronic control circuitry enables arc starting to be achievedwithout spatter or lack of fusion defects. Some units now available willslowly advance the wire until the tip touches the workpiece, sense the shortcircuit, retract the wire to the correct arc length and initiate the full weldingcurrent (Fig. 7.8). Similarly, in most of these modern units a crater fillingfacility is built in, which automatically fades out the current when the triggeron the gun is released.
122 The welding of aluminium and its alloys
7.6 Typical modern pre-programmable control panel for synergicpulsed MIG power source. Courtesy of TPS-Fronius Ltd.
7.7 Modern 500 amp inventor-based programmable synergic pulsedMIG power source. Courtesy of TPS-Fronius Ltd.
7.8 Programmed arc start – reducing the risk of lack of fusion defects.Courtesy of TPS-Fronius Ltd.
If you are contemplating purchasing new or replacement MIG equip-ment it is recommended that pulsed MIG power sources are purchased,even though they are more expensive than conventional equipment. Thiswill give the fabrication shop a more flexible facility with a wider range ofoptions than with the straight DC units.
22.214.171.124 Fine wire MIG
As the name suggests the fine wire MIG process uses a fine, small diameter wire, less than 1.2mm and as small as 0.4mm in diameter, althoughwires of 0.4 and 0.6mm in diameter need to be specially ordered from thewire drawer. Small diameter wires are notoriously difficult to feed and toeliminate feeding problems a small wire reel and a set of drive rolls aremounted directly on the welding torch. Welding parameters are in theranges 50–140 A and 17–22 V, resulting in a short-circuiting mode of metaltransfer. Travel speeds are generally around 320mm/min, giving low heatinput and enabling thin sheets, around 1mm in thickness, to be weldedwithout burn-through, excessive penetration or excessive cap height. Thefine wire process, although successful, has now largely been replaced bypulsed MIG welding.
126.96.36.199 Twin wire MIG
A relatively recent development has been the twin-wire process. Thecurrent that can be used is limited in the single wire process by the forma-tion of a strong plasma jet at high welding currents. This jet may cause anirregular bead shape, porosity or excess penetration. The twin wire processovercomes these difficulties with two independent arcs operating in thesame weld pool, enabling major improvements in productivity to beachieved. The basis of this is the use of two inverter-based pulsed MIGpower sources coupled in series, each complete with its own microproces-sor control unit and wire feeder (Fig. 7.9). The two units are linked by acontroller that synchronises the pulses from each unit such that when oneunit is welding on the peak of a current pulse the other unit is on back-ground current. By this means a stable welding condition is created withthe two arcs operating independently of each other. The wires are fed to asingle torch carrying two contact tips insulated from each other. The wiresmay be positioned in tandem, side by side or at any angle in betweenenabling the bead width and joint filling to be precisely controlled.
The limitation of twin wire MIG is that the process can only be used ina mechanised or robotic application. With suitable manipulators, however,it is capable of very high welding speeds, a 3 mm leg length fillet weld, for
124 The welding of aluminium and its alloys
instance, being capable of being made at travel speeds of over 2 metres perminute.The welding torch is large, making access a problem, and the capitalcost of the equipment is high.
7.2.2 Wire feeders and welding torches
188.8.131.52 Welding torches
The MIG process requires the filler wire to be delivered to the weldingtorch (Fig. 7.10) at a fixed speed and for the welding current to be trans-ferred to the wire via a contact tip within the torch. The torch must also beequipped with a means of providing the shield gas and of enabling thewelder to commence and end the welding sequence. This is generallyachieved by means of a trigger on the handle of the torch. Operatingthe trigger initiates the shielding gas flow and the welding current when the wire tip is scratched on the workpiece surface. This, in its turn, starts thewire feed. Releasing the trigger stops the wire feed and shuts off the currentand shielding gas. The heat generated in the torch during welding may alsorequire the torch to be water-cooled. All of these services must be deliv-ered to the torch via an umbilical cable containing a wire feed conduit,
welding current cable, shield gas hose, cooling water delivery and returnhoses and the electrical control cables. At the same time the torch must not be made so heavy and cumbersome that the welder cannot easilymanipulate the torch with a minimum of effort. A well-designed torchtherefore needs to be lightweight, robust and easily maintained and theumbilical cable needs to be light and flexible. It is most important if con-sistent quality is to be achieved that the welder is provided with the besttorch available.
126 The welding of aluminium and its alloys
7.10 Exploded view of a typical MIG torch: A ergonomically shapedhandle; B contact tip, C gas shroud, D gas diffuser, E power cableconnector, F umbilical containing gas hose, power cable and controlcable, G power switch, H replaceable liner, I adjustable nozzle.Courtesy of Bernard Welding Equipment Company.
184.108.40.206 Wire feed systems
There are three basic forms of wire feeders: the ‘push’ system, the ‘pull’system and the ‘push–pull’ system.As the name suggests, in the push system,the wire is pushed by the wire feed drive rolls along the conduit to thewelding torch. The flexibility of aluminium wire means that the wire canbuckle and jam inside the conduit, resulting in irregular wire feeding at thewelding torch and, in extreme cases, a ‘bird’s nest’ of tangled wire at thewire feed unit. Such wire feeders are generally restricted to a minimum wirediameter of 1.6mm and the wire feed conduit to a length of 3.5m.
The pull system utilises a set of wire rolls in the torch handle which pullthe wire from the wire reel (Fig. 7.11).This arrangement increases the weightof the torch and does not increase the distance over which the wire can befed, this still being limited to around 3.5m, although the consistency of thewire feed is improved and wire diameters down to 0.8mm can be used.
The push–pull system is a combination of the above two systems with aset of drive rolls at both the wire reel feeder and in the torches illustratedin Fig. 7.11. This enables small diameter wires to be fed up to 15m from thewire reel. The final variation on this theme is the spool on gun torch whichutilises a small 100mm diameter wire reel mounted on the welding torchand a set of drive rolls in the torch body. These rolls push the wire the short
distance from the reel to the contact tip, enabling wires as small as 0.4mmin diameter to be used. The length of the umbilical cable is limited only bythe voltage drop in the power delivery and return leads and perhaps theneed to provide water cooling to the torch.
All of these systems require that the wire is driven at a constant, con-trolled rate unaffected by continuous operation, variations in supply voltageor fluctuations in temperature. They must also be able to reach the desiredwire feed speed as rapidly as possible in order to give good and stable arcstarting. The control for feed speed may be mounted on the torch or on thewire feeder.
While manual welding may use any of the systems mentioned, push–pullsystems are becoming the standard method of wire feeding in robotic appli-cations because of the need for highly consistent feed speeds and defect-free arc starting.
220.127.116.11 Wire drive rolls
Aluminium wire is very much softer than steel and this can result in feedingdifficulties, the wire being easy to deform by excessive roll pressure, causingthe wire to jam in the feed conduit or in the contact tip. With push wirefeeders any impediment to the wire feed, such as metal shavings or wiredrawing soap compacted in the contact tip, kinks in the wire feed liner orspatter on the contact tip, may cause the wire to buckle within the wire feedconduit.Wire feed rolls must not be knurled but should be smooth, groovedrolls or, better still, one flat roll and one with a 60° V-groove. Wire feedingsystems for aluminium also employ four drive rolls (Fig. 7.12) rather thanthe two rolls that conventionally are used to feed steel wires. It is impor-tant that the roll pressure is adjusted such that the wire is not grooved orflattened by the rolls since this will also lead to wire feeding problems. Thewire should be kept as clean as possible. Covers to protect the reel fromdust and heated cabinets are available and it is recommended that theseare used where the highest quality is required.Also available are wire clean-ing devices comprising a cloth or felt pad clamped around the wire andsoaked in a cleaning fluid such as alcohol or acetone. This can be used toremove grease, drawing soap and loose particles of swarf or oxide at thepoint at which the wire enters the conduit.
A relatively recent innovation in wire drive rolls is finding increasing use.This is the orbital welding system in which the wire passes through thehollow centre of the drive motor and is driven by a set of rolls set at anangle to and orbiting around the wire. This method of driving the wire hasthe advantages of both straightening and vibrating the wire, aiding infeeding the wire through the conduit.
128 The welding of aluminium and its alloys
18.104.22.168 Contact tip (tube)
The contact tip is a small but vital component in the welding power circuit.The tip is formed from a tube made to be a sliding fit for the wire. It isscrewed into the torch head, ‘B’ in Fig. 7.10, and is the point at which thewelding current is picked up by the filler wire. The contact tip is made fromcopper or brass and wears in use. It is therefore made to be replaceable.The tip for aluminium welding may vary in length from 25mm to 100mm.The longer contact tips provide the best current transfer conditions andtherefore the most stable welding conditions. Tips have been designed thatcarry either a spring-loaded shoe to maintain a constant pressure on thewire or with the hole offset in order to force the wire against one wall,thereby improving and maintaining contact.
A worn contact tip may cause the wire to jam, resulting in a tangle at thewire drive rolls. A perhaps more serious weld quality problem may alsoarise from arc instability caused by the point at which the wire picks up thecurrent moving up and down the contact tip. This effectively changes thewire stick-out length which in its turn affects the voltage, leading to arcinstability and lack of penetration defects. Poor contact between the tip andthe wire may cause arcing within the tip, giving rise to arc instability andperhaps wire feed problems. Damage to the tip from spatter, accidentaltouch-down or mechanical damage may cause similar problems.
MIG welding 129
7.12 Four roll MIG wire drive unit. Courtesy of TPS-Fronius Ltd.
The tip should be recessed in the gas shroud by at least 5mm whenwelding in spray transfer. If the tip is too close to the end of the gas shroudthere is an increased risk of spatter damaging the tip. If the tip protrudesfrom the shroud then there is a risk of the tip touching and melting into theweld pool. This will cause weld pool cracking, may give rise to ‘bird’snesting’ and will require the tip to be replaced.
7.3 Welding consumables
7.3.1 Shielding gases
The shielding gases, as with TIG welding, are the inert gases argon andhelium or combinations of these two. Other, active, gases such as oxygen ornitrogen even in small amounts will give porosity and smutting problems.The most commonly used gas is argon which is used for both manual andsome automatic welding. It is substantially cheaper than helium and pro-duces a smooth, quiet and stable arc, giving a wide, smooth weld bead witha finger-like penetration to give a mushroom-shaped weld cross-section.Argon, however, gives the lowest heat input and therefore the slowestwelding speeds.There is therefore a risk of lack of fusion defects and poros-ity on thick sections. Argon may also give a black sooty deposit on thesurface of the weld. This can be easily removed by wire brushing. Sectionsof 3mm thick butt welds using conventional and pulsed current are illus-trated in Fig. 7.13. Thicker section butt and fillet welds are illustrated in Fig.7.14. In these thicker section welds the characteristic finger penetration ofan argon gas shield can be seen.
Helium increases the arc voltage by as much as 20% compared withargon, resulting in a far hotter arc, increased penetration and wider weld
bead. The wider bead requires less critical positioning of the arc and assistsin avoiding missed edge and lack of penetration-type defects. The hotter,slower cooling weld pool also allows hydrogen to diffuse from the moltenweld metal, making this a method that may be used to reduce the amountof porosity. The increased heat also enables faster welding speeds to be
achieved, as much as three times that of a similar joint made using argonas a shielding gas.
Helium, however, is expensive and gives a less stable arc than argon. Purehelium therefore finds its greatest use in mechanised or automatic weldingapplications. Helium shielded manual welds are illustrated in Fig. 7.15.
For manual welding and some mechanised applications mixtures of argonand helium give good results with characteristics intermediate between thetwo gases. These mixtures are useful on thicker materials because theyincrease the heat input and provide a wider tolerance box of acceptablewelding parameters than pure argon. They will also improve productivityby enabling faster travel speeds to be used. The most popular combinationsare 50% and 75% of helium in argon. Typical welds using 50% helium/50%argon are illustrated in Fig. 7.16. These show weld bead shapes intermedi-ate between the pure argon and pure helium welds in Figs. 7.14 and 7.15.
The last point to be made concerning gases is purity, already covered inChapter 3, but worth re-emphasising because of the major effect that thishas on weld quality. Shielding gases must have a minimum purity of99.998% and low moisture levels, ideally with a dew point less than -50°C(less than 39ppm H2O) – do not forget that this is at the torch, not at theoutlet of the cylinder regulator!
7.3.2 Welding filler wire
The wire acts as both the filler metal and the anode in the welding arc.In order to do this the wire picks up the welding current by a rubbingcontact between the wire and the bore of the contact tip. Filler wire diam-eters vary from 0.8mm to 3.2mm which results in a high surface area tovolume ratio. This relatively large surface area requires the wire to be keptscrupulously clean since surface contamination will give rise to porosity.Wires should be stored in clean, dry conditions in their unopened packag-ing where possible. Wires that have been in store for a substantial periodof time, e.g. 6 months or more, even when stored in their original packag-ing can deteriorate and give rise to porosity. If left on the welding machineovernight or over weekends they should be protected from contaminationby covering the reel with a plastic bag. In critical applications it may be nec-essary to remove the reel from the machine and store it in a steel canbetween periods of use.
Condensation can form on the wire if it is brought into a warm fabrica-tion shop from a cold store, and in conditions of high humidity moisturemay once again form on the wire. Some power sources incorporate heatersin the wire feeder to prevent this from happening. If condensation is trou-blesome and this facility is not available, a 40 watt light bulb installed in thewire feeder cabinet provides sufficient heat to maintain the wire in a drystate.
It is possible to obtain wire cleaning devices that clip on the wire at thepoint where it enters the wire feed cable. These devices consist of a felt padcarrying a cleaning fluid which removes contaminants as the wire passes
into the cable. They can be very effective at removing traces of grease andoils, dust, etc. on the surface of the wire. Better still is shaving the wire. Thisnot only removes surface contaminants and oxides but hardens the wire,making it easier to feed and less likely to tangle.
7.4 Welding procedures and techniques
A set of outline welding procedures are given in Tables 7.2 and 7.3 for buttwelding using either argon or helium as the shielding gas, and guidance onparameters for fillet welding is illustrated in Fig. 7.17. The parametersquoted form a starting point from which to develop a procedure specificallydesigned for the application. They are not to be regarded as hard and fastrules. Also included as Table 7.4 are suggested weld preparations for MIGwelding of a range of plate thicknesses.
7.4.1 Arc starting
Because the wire is fed into the arc immediately that the arc is started there can be no preheating of the joint as possible with TIG. This results in shallow penetration and a humped weld bead on starting. Lack offusion defects are often encountered – a ‘cold start’ – and weld bead shape may not be acceptable. To avoid these defects the welder shouldstrike the arc some 25mm ahead of the desired start point and thenmove back to the weld start before beginning to weld forward at a normalspeed.
Arc starting may be achieved using a scratch start where the wire isallowed to protrude from the contact tip by 10mm and brought to within20mm of the surface. The trigger is operated and at the same time thewelding torch is moved to scrape the wire tip over the work surface. Assoon as the arc is established the power source senses the change in voltageand starts the wire feed, the weld pool forms and welding can commence.A ‘running’ start is one where the wire begins to feed as soon as the triggeris operated and is short-circuited when it touches the workpiece, establish-ing the arc. The current surge on short-circuiting may cause arcing withinthe contact tip and spatter to adhere to the shroud and contact tip. Thesecan lead to wire feeding problems.
As mentioned earlier, the new inverter power sources have a facility fora highly controlled arc start sequence.When the trigger is operated the wireis fed at a slow and controlled rate until the wire tip touches the workpiece.It is then retracted slightly and a pilot arc is ignited. Once this is stable thecurrent is increased at a controlled rate, the wire speed increased to thedesired feed rate and welding commences (Fig. 7.8). This gives a spatter-free start and a low risk of lack of fusion defects, a major improvement overthe capabilities of older equipment.
1. Where two welding parameters are specified in one entry the first refers to the requirements for the first pass.2. Where a reverse side weld is specified it is necessary to grind the reverse of the root pass to ensure a sound joint.3. When making a double sided joint it is recommended that the weld passes are balanced to reduce distortion.
7.4.2 Torch positioning
The angle at which the torch is presented to the joint is important in thatan incorrect angle can result in air entrainment in the shielding gas and willalso affect the degree of penetration. Ideally the torch should be normal tothe surface and pointed forwards towards the direction of travel at an angleof between 10° and 15° from the vertical, the forehand angle (Fig. 7.18). Asthis angle increases penetration decreases and the amount of air entrainedin the shielding gas gradually increases.
Arc length cannot be set by adjusting the voltage since this is a functionof the resistance of the circuit as a whole.The arc length is set by the welderusing both sight and sound, a correct arc length being characterised by a
Thickness Root Included Current Voltage No. of Filler Travel(mm) gap/ angle (A) (V) passes diam. speed
face (degrees) (mm) (mm/min)(mm)
50 0/5 70/2 550 32 2 each 4.8 250sided side
75 0/10 30 650 30 3 each 5.6 2506mm sideroot R
0 100 150 200
250 300 3500
MIG welded fillet joints Weldruns
3–4 1.6 300–400
7.17 Suggested parameters for fillet welding – argon shielding.
Table 7.4 Suggested weld preparations for MIG welding
Material Edge preparation Remarksthickness(mm)
1.6–4.8mm A backing bar givesgreater control ofpenetration
6.4–9.5mm Weld from bothsides, sighting Vsrecommended
4.8–12.7mm Suitable also forpositional welding,when welded fromboth sides
6.4–12.7mm Flat aluminium backingbar optional. Oneor more runs fromeach side. Back chippingrecommendedafter first run
6.4–19.1mm One or more runsfrom one side,depending on thickness.Suitable alsofor positionalwelding
12.7–25.4mm Up to 1.6mm rootgap. One or moreruns from each side.Back-chippingrecommended afterfirst run
70° to 90°
70° to 90°
70° to 90°
soft crackling sound similar to the sound of frying bacon. Too short an arcsounds harsh and gives excessive spatter while a long arc has a hummingsound. The effect of changing the arc length is summarised in Table 7.5.
7.4.3 Ending the weld
If, when the weld is ended, the wire feed is abruptly stopped the weld poolwill freeze and a shrinkage crater will form. If the weld pool is small thiscrater may be simply a shallow depression in the weld surface. In large weld
140 The welding of aluminium and its alloys
Angle for fillet welding Angle for butt welding
Angle of torch related to travel direction. Ideally thisshould be between 10° and 15°
Direction of torch travel
7.18 Torch position for MIG welding.
Table 7.5 Effect of arc length
Weld Bead Short Arc Long Arc
Excess metal High FlatPenetration Deep ShallowWidth Narrow WidePorosity Higher LowerSpatter Higher Lower
pools the crater may extend down into the weld to form an elongated pore– piping porosity. As the weld continues to cool and contract then the asso-ciated shrinkage stresses may cause hot short or crater cracks to form. Anyform of cracking is unacceptable and is to be avoided. Methods of elimi-nating this defect include the following:
• The use of run-off tabs on which the weld can be terminated, the tabbeing subsequently removed.
• Increasing the travel speed just before releasing the trigger. This causesthe weld pool to tail out over a distance. It requires a high measure ofskill on the part of the welder to produce acceptable results.
• Making a small number of brief stops and starts into the crater as theweld cools. This adds filler metal to the crater.
• As the trigger on the torch is released the wire feed speed and thewelding current are ramped down over a period of time. The crater isfed with progressively smaller amounts of molten filler metal as it forms,resulting in the filling and elimination of the crater. This crater fillingfacility is standard on modern equipment and is the preferred methodfor avoiding piping porosity and crater cracks.
7.5 Mechanised and robotic welding
As MIG welding is a continuously fed wire process it is very easily mech-anised. The torch, having been taken out of the welder’s hand, can be usedat welding currents limited only by the torch or power source and at highertravel speeds than can be achieved with manual welding. A typical robotMIG welding cell where the robot is interfaced with a manipulatorfor increased flexibility and a pulsed MIG power source is illustrated in Fig. 7.19. Greater consistency in operation means that more consistent weldquality can be achieved with fewer defects. The advantages may be sum-marised as follows:
• More consistent quality.• More consistent and aesthetically acceptable bead shape.• More consistent torch height and angle mean that gas coverage can be
better and the number of defects reduced.• Fewer stops and starts, hence fewer defects.• Higher welding speeds means less heat input, narrower heat affected
zones and less distortion.• Higher welding current means deeper penetration and less need for
large weld preparations with fewer weld passes and therefore fewerdefects.
• Higher weld currents mean a hotter weld and reduced porosity.
MIG welding 141
• The above advantages mean that less welding time is required andrework rates will be reduced, giving major improvements in productiv-ity and reductions in cost.
• There is no need for the skilled welder required for manual welding, amajor advantage in view of the current shortage of highly skilledwelders.The loading and unloading of the welding cell can be performedby unskilled workers, although knowledgeable and experienced engi-neers will be needed to programme and maintain the equipment.
There are some disadvantages to mechanised and robotic welding. Weldpreparations need to be more accurate and consistent; more planning isneeded to realise fully the benefits; capital expenditure will be required topurchase manipulators and handling equipment; maintenance costs maywell be higher than with manual equipment and the full benefits of highdeposition rates may only be achieved in the flat or horizontal–vertical posi-tion. Despite these problems there is an increased usage of mechanised andautomated MIG equipment because of the financial benefits that may beachieved.
142 The welding of aluminium and its alloys
7.19 Pulsed MIG power source interfaced with a robot andmanipulator. Courtesy TPS-Fronius Ltd.
To illustrate the cost benefits of mechanisation take as an example a 12mm thick butt weld. Made using manual MIG this would require fourpasses to fill at a travel speed of around 175mm/min, a total weld time of over 20 minutes per metre. A machine weld using argon as the shieldgas could be made in a single pass at around 480mm/min travel speed, atotal weld time of just over 2 minutes. Using helium as the shielding gaswould reduce this time even further. A set of typical parameters is given inTable 7.6.
Because of the higher duty cycle achievable with mechanised or auto-mated welding the power source, wire feeder and torch must be more robustand rated higher than those required for manual welding. Welding currentsof 600 A or more may be used and this must also be borne in mind whenpurchasing a power source. The torch manipulator, whether this is a robot,a dedicated machine or simply a tractor carriage, must have sufficient powerto give steady and accurate motion at a uniform speed with repeatable,precise positioning of the filler wire. Although at low welding currents con-ventional manual equipment may be adapted for mechanisation by attach-ing the torch to a manipulator, it is advisable to use water-cooled guns andshielding gas shrouds designed to provide improved gas coverage.
7.6 Mechanised electro-gas welding
A technique described as electro-gas welding was developed by the AlcanCompany in the late 1960s but seemed to drop out of favour in the late1990s, which is surprising when the advantages of the process are consid-ered. The weld may only be carried out in the vertical-up (PF) position butis capable of welding both square edge butt joints and fillet welds withthroats of up to 20mm in a single pass.
To operate successfully the process uses a long arc directed to the backof the penetration cavity. This provides a deeply penetrating arc that
MIG welding 143
Table 7.6 High current mechanised MIG parameters
Thickness Joint type Backing Current Voltage Travel speed(mm) (A) (V) (mm/min)
operates in the space above the weld pool. The pool fills the cavity belowthe arc, solidifying as the torch is traversed vertically up the joint line. Themolten pool is retained in position and moulded to shape by a graphite shoeattached to and following immediately behind the welding torch.
The process utilises a drooping characteristic power source capable ofproviding 600 A at 100% duty cycle coupled to a water-cooled machinetorch. The torch is mounted on a vertical travelling carriage at an angle of15° from the horizontal. The gas shroud should be at least 25mm in diam-eter and the tip of the contact tube should be flush with the shroud.
For butt welding the graphite shoe is made from a flat plate shaped witha groove to mould the cap, flared out towards the top of the shoe where theweld pool is formed. The fillet weld mould is provided with a pair of ‘wings’set back to press against the plates to form the fillet. In both cases the shoeis held against the plates by spring pressure. The shoe must be long enoughto hold the molten metal in place until it has solidified – in the region of100mm may be regarded as sufficient. It has been found that heating theshoe to 350°C before commencing welding assists in preventing fouling ofthe shoe with parent metal.
During welding the arc must be prevented from arcing onto the weld poolor the graphite shoe. This requires careful control of the wire position andthe wire feed speed, as a balance must be achieved between the volume ofmetal being fed into the pool, the volume of the mould and the traversespeed.
7.7 MIG spot welding
MIG spot welding may be used to lap weld sheets together by meltingthrough the top sheet and fusing into the bottom sheet without moving thetorch. The equipment used for spot welding is essentially the same as thatused for conventional MIG, using the same power source, wire feeder andwelding torch. The torch, however, is equipped with a modified gas shroudthat enables the shroud to be positioned directly on the surface to bewelded (Fig. 7.20). The shroud is designed to hold the torch at the correctarc length and is castellated such that the shield gas may escape. The powersource is provided with a timer so that when the torch trigger is pulled apre-weld purge gas flow is established, the arc burns for a pre-set time andthere is a timed and controlled weld termination. The pressure applied bypositioning the torch assists in bringing the two plate surfaces together.Because of this degree of control the process may be used by semi-skilledpersonnel with an appropriate amount of training.
The process may be operated in two modes: (a) by spot welding with theweld pool penetrating through the top plate and fusing into the lower oneor (b) by plug welding where a hole is drilled in the upper plate to enable
144 The welding of aluminium and its alloys
the arc to operate directly on the lower plate so that full fusion can beachieved. Plug welding is generally required when the top sheet thicknessexceeds 3mm. The size of the drilled hole is important in that this deter-mines the size of the weld nugget and the diameter should be typicallybetween 1.5 and 2 times the top sheet thickness. Typical welding parame-ters are given in Table 7.7.
Of the shield gases argon is the preferred choice as it produces a deep,narrow penetration. Argon also provides better arc cleaning than helium,important in maintaining low levels of oxide entrapment. Arc stability isalso superior. Surface preparation is important, cleanliness being crucial todefect-free welds. As with butt welds, degreasing and stainless steel wirebrushing, supplemented by scraping if a hole is drilled, are most important.
MIG welding 145
7.20 Schematic of the MIG spot welding process.
Table 7.7 Spot and plug welding parameters
Top plate Bottom plate Preparation Current Voltage Weld time(mm) (mm) (A) (V) (s)
Welding can be carried out with equal ease with the plate in thehorizontal, vertical or overhead position although in other than the flat position the welding time needs to be reduced from that listed in Table 7.7.This may result, however, in an increased level of porosity. Other defectsinclude cracking, lack of fusion and burn-through. To prevent and controlburn-through a temporary backing bar may be used. Fit up is important andfor the highest strength the gap between the plates should be as small aspossible.
146 The welding of aluminium and its alloys
While MIG and TIG welding may be regarded as the most frequently usedprocesses for the joining of aluminium and its alloys there are a largenumber of other processes that are equally useful and are regularlyemployed although perhaps in rather more specialised applications than the conventional fusion welding processes. Some of these processes are discussed here.
8.2 Plasma-arc welding
As described in Section 4.3 a modification to the TIG welding torch enablesa strong plasma jet to be produced that has some very desirable featuresfor both welding and cutting. Despite these advantages the process foundlittle application for the welding of aluminium when DC electrode nega-tive or electrode positive were used because of extensive lack of fusiondefects. Alternating current gave no better results as high currents wererequired, resulting in rapid electrode deterioration. The pulsing of thecurrent also caused weld pool instability, poor bead shape and lack of fusiondefects. These limitations were overcome with the development of squarewave power sources, already mentioned in Chapter 6, since which timeplasma-TIG has become accepted as a viable production process.
8.2.1 Plasma-TIG welding
22.214.171.124 Main characteristics
As mentioned above, the basic principles of the plasma-TIG process (ENprocess number 15) have been covered in Section 4.3 which describes theuse of the heat from the plasma-arc for cutting purposes. For welding thetransferred arc plasma-jet is used as the heat source, the major difference
8Other welding processes
from cutting being that no cutting gas is introduced to blow away the moltenmetal (Fig. 8.1).
There are a number of advantages that plasma-TIG has compared withconventional TIG mainly because of the cylindrical and constricted plasmacolumn.This provides less sensitivity to process variables than with the TIGprocess. The constricted plasma column means that the heat is confined toa smaller area than with TIG, enabling a very stable controllable arc to beproduced at currents as low as 0.1A. It is possible to weld without keyhol-ing at thicknesses less than 2.5mm but there is little advantage to be gainedin terms of productivity over TIG. The keyholing technique may be used inmanual welding but it is more common to find it in mechanised or auto-mated applications.
The plasma is strongly directional and can be pointed in any given direc-tion even at very low currents. The cylindrical plasma column means thatheat input is constant irrespective of torch to workpiece distance, unlikeTIG with its conical arc. The tungsten electrode is recessed inside the torchnozzle, making tungsten contamination an impossibility. There is also anincrease in weld quality with a reduced risk of porosity and distortion.Higher welding currents enable material as thick as 15mm to be weldedpositionally in a single pass with a square edge weld preparation using thekeyhole technique although in the flat position the maximum thickness islimited to around 8mm without filler metal.
The process may be used in a melt-in mode using techniques similar tothose that would be used for TIG. The weld may be made autogenously inthose alloys that are crack-resistant; filler wire may be added to those thatare crack-sensitive. This wire can be added manually but torches are avail-
148 The welding of aluminium and its alloys
8.1 Principles of the plasma-TIG transferred arc torch. Courtesy of TWILtd.
able equipped with automatic wire feed.This latter feature, however, makesthe process sensitive to stand-off distance. A change in the stand-off willaffect the position in which the wire enters the weld pool and this may givevariable weld quality.
The problem with conventional plasma-TIG is that the process normallyoperates on DC negative polarity so that no cathodic cleaning takes place,an obvious disadvantage when welding aluminium. Welding without thefacility to remove the oxide layer causes porosity. To overcome this a devel-opment of the DC positive plasma-TIG process, the variable polarityplasma process was developed. This utilises a square wave form with a suit-able balance of the DC negative and positive components to provide bothmelting and adequate oxide removal.
126.96.36.199 Variable polarity plasma-arc process principles
For the plasma to form, a pilot arc is first established within the torchannulus by means of a high-frequency discharge. As the plasma gas passesthrough this HF discharge it is ionised, allowing the welding current to flowand the plasma flame to be established. The plasma gas flow is very small,typically 1–5 litres/min. This is insufficient to provide adequate shieldingand therefore needs to be supplemented with a secondary shield gas. Thegases are generally high-purity argon similar in quality to that used for TIGwelding, but helium or argon–helium mixtures may also be used.
Arc stability and oxide removal are better than with TIG or MIG pro-vided that the appropriate wave form is used. It is necessary to tailor eachwave form and the balance between DC electrode positive and DC electrode negative to the individual alloy composition. Typical wave formcharacteristics for the keyhole welding of a number of alloys are given in Table 8.1. It is worth remembering that if the keyhole technique is used autogenously the alloys must be capable of providing crack-free weldmetal.
Other welding processes 149
Table 8.1 Typical parameters for keyhole welding of 6.5mm thick Al alloys
Over 8mm thick it is necessary to weld with a prepared edge and fillerwire although in the vertical-up (PF) position material as much as 16mmthick can be welded. The diameter of the filler wire is the same as would beused for TIG welding, generally 1.6 or 2.4mm diameter.
8.2.2 Plasma-MIG welding
Plasma-MIG welding utilises a MIG wire, generally 1.6mm in diameter, fedthrough a plasma-arc torch. This allows a higher combined welding currentto be used than for the MIG wire alone with a high current density and ahigher deposition rate than MIG being achieved. This enables weldingspeeds to be increased giving lower heat input and narrower heat affectedzones with better mechanical properties.
The process is generally used in a mechanised or automated applicationalthough it is possible to use it in a semi-automatic manual mode.The thick-ness that has been welded ranges from 6mm to 60mm.
8.3 Laser welding
Laser welding is being used increasingly in both the automotive and aero-space industries for the welding of a range of materials (Fig. 8.2). The laserwelding of aluminium and its alloys has, however, presented problems tothe welding engineer. Poor coupling of the beam with the parent metal,high thermal conductivity, high reflectivity and low boiling point alloyingelements have, until relatively recently, prevented the achievement of con-sistent weld quality.
150 The welding of aluminium and its alloys
8.2 Laser weld of thin plate. Courtesy of TWI Ltd.
The wavelength of the laser light affects the coupling – the absorption ofthe beam energy by the metal being cut or welded. As the wavelengthincreases the coupling becomes poorer and this is a particular problem withaluminium and its alloys. The wavelength of light from a CO2 laser is 10.6mm, that of a Nd-YAG laser 1.06 mm – the solid state laser is thereforebetter suited to the welding of aluminium. Development work, carried outmostly for the automotive industry on sheet metal, has also been of assis-tance in minimising these problems by improved focusing of the beam withboth types of laser. One of the earliest applications for this development isthe Audi A2 which has some 30 metres of laser welds in its bodywork. Themain reason for the improvement in laser weldability has been the abilityto achieve high-power densities, typically above 40kW/mm2, with both theNd-YAG solid state and CO2 gas lasers. As a process, laser welding offersthe advantages of a concentrated, high-energy density heat source. Thispower density enables the weld to be made in the keyhole mode (Fig. 8.3),improving the absorption of the laser beam due to reflections within thecavity. The deeply penetrating keyhole weld produces very narrow heataffected zones, minimising both distortion and the loss of strength in theHAZ of the work or precipitation-hardened alloys and reducing the loss oflow boiling point alloying elements such as magnesium.
The low boiling point elements, however, assist in establishing a stablekeyhole. The high-energy beam also enables very fast welding speeds to beachieved, speeds of 2 metres per minute with a 2kW Nd-YAG and 5–6metres per minute with a 5kW CO2 laser in 2mm thick sheet being easily
Other welding processes 151
Molten metal flowsround keyhole andrecombines to formweld
'Chevron' weldbead pattern
8.3 Principle of laser welding. Courtesy of TWI Ltd.
attainable.The main welding parameter is the laser power which determinesboth the depth of penetration and the travel speed. Other variables are theposition of the focal point, generally at the upper surface, wire diameterand feed speed and weld gap.
Defects in laser welded joints are similar to those encountered in weldsmade by other fusion welding processes. Porosity is caused by hydrogenfrom the environment, dissolved in the parent metal, contained in the oxidefilm or from an unstable keyhole condition. The solution to this problem iscareful surface preparation including pickling and scraping, gas shieldingand the use of adequate power to ensure the creation of a stable keyhole.Although most of the non-heat-treatable alloys are capable of being weldedsuccessfully, hot cracking may be encountered, particularly in those alloysthat are sensitive. This can be reduced or eliminated by the addition of asuitable filler wire. The last difficulty is caused by the low viscosity of themolten weld metal. This causes the problem of ‘drop-through’, where theweld metal falls out of the joint when welds are made in the flat position.This problem can be overcome by welding in the horizontal–vertical (PC)position.
8.3.1 CO2 laser welding
As mentioned above improved focusing has enabled very concentratedbeams with energy densities above 40kJ/mm2 to be produced.This has beenachieved by using parabolic reflectors or transmissive systems with a focallength of around 150mm. The alloy content affects the energy required toachieve a keyhole with increasing levels of zinc or magnesium requiring lessenergy.This is attributed to the low vaporisation temperature of these alloy-ing elements assisting in the formation of the keyhole. One corollary of thisis that higher welding speeds are possible in those alloys with the highermagnesium contents.
Helium gas shielding of both the root and face of the weld is re-commended for the higher magnesium-containing alloys such as 5083(Al4.5Mg). Over some 3mm in thickness a jet of helium, supplementing the shielding gas, directed at the weld pool also gives improved weld appearance. Helium–argon mixture and pure argon gas have also been used with acceptable results although with a reduced parameter tolerancebox.
Wire additions may be used to increase the resistance to hot cracking inthose alloys that cannot be autogenously welded such as the 6XXX and7XXX series of alloys.Wire additions are also beneficial in coping with gaps,a 1.2mm wire can be used to fill gaps of up to 1.2mm. Wire diameters maybe between 0.8 and 1.2mm. Feeding the wire into the leading edge of the
152 The welding of aluminium and its alloys
weld pool at an angle of around 45° will improve the bead shape on bothroot and cap.
The majority of welding has been carried out on butt welded sheets (Fig.8.4). The joint between the sheets results in an increase in beam absorptionand improved keyhole stability compared with bead-on-plate welds. Goodfit-up is necessary for autogenous welding if undercut is to be avoided. Thisrequires either square machined or high-quality guillotined edges. Wherelower-quality edges are produced, wire additions can be used to cope withany gaps. Where extrusions are welded, a small ‘V’ on the weld face aids inpenetration by reflecting laser light within the preparation.
8.3.2 Nd-YAG solid state welding
The wavelength of the light from solid state lasers is only a tenth of thewavelength of light from a gas laser. It is believed that this permits bettercoupling of the beam with the parent metal. The short wavelength alsoenables the laser light to be transmitted via fibre optics, rather than by theuse of the copper mirrors that are used to manipulate the light from theCO2 laser (Fig. 8.5). This gives greatly improved flexibility, allowing the useof a robot to move and position the beam. Most of the techniques used forCO2 welding apply to the solid state laser and, as with the CO2 laser, thereis a critical power density required to achieve keyhole penetration. Anaverage laser power less than 1kW is regarded as being the lower accept-able limit for the avoidance of lack of penetration or porosity.
Other welding processes 153
8.4 Laser weld of dissimilar thickness of automotive panelling.Courtesy of TWI Ltd.
Since the early 1990s the power available from the solid state lasers hasincreased so that a pulsed 3kW laser is capable of welding speeds of up to2.3 metres per minute in 1.5mm thick 5XXX alloys. Gas shielding, similarto that for CO2, can be achieved using either argon, helium or nitrogen fedco-axially with the beam or from a simple side port. Gas shielding of theunderbead will also give an improvement in the surface finish.
High-power diode lasers (HPDLs) are also being investigated and it islikely that they will become commercially available in the near future.Thereare several advantages with this type of laser, price and low maintenancebeing two. With the recent improvements in optics, HDPLs are capable ofachieving power densities of 5 ¥ 104 W/cm2 and, with wavelengths of around800nm, are producing good results when used to weld aluminium.
8.3.3 Welding defects
CEN standards are being developed to cover the quality assurance andquality control of laser welds in a range of metals, for example EN ISO13919-1 and EN 288 part 15. ASME IX already has requirements regard-ing procedure approval testing of laser welds. A brief summary of laserwelding defects is included in Table 8.2.
8.3.4 Arc augmented laser welding
There have been a number of relatively new developments where the laserhas been combined with the arc from a conventional welding power source.
154 The welding of aluminium and its alloys
8.5 Nd-YAG laser interfaced with a robot. Courtesy of TWI Ltd.
The MIG, TIG and plasma-arc processes have been used, enabling higherwelding speeds to be achieved, particularly in thin sheet for the automotiveindustry. Of these options MIG welding is the preferred fusion weldingprocess, although the plasma/laser process is also being actively developedand is producing good results. Figure 8.6 illustrates a commercially avail-able laser/MIG welding head and Fig. 8.7 the principles of operation.
In addition to higher speeds the enhancement of the laser beam enablesgreater variations in fit-up to be tolerated. Penetration, it is claimed, isincreased and the change in shape of the weld pool assists in allowinghydrogen to diffuse out of the joint, reducing the porosity often encoun-tered in laser welds. At present (2002) these augmented laser processes are in the early stages of development but show great promise in wideningthe field of applications of the process.
8.4 Electron beam welding
Electron beam welding is, like laser welding, a power beam process ideallysuited to the welding of close square joints in a single pass. Unlike the laserbeam, however, the electron beam process utilises a vacuum chamber in
Other welding processes 155
Table 8.2 Summary of laser welding defects and corrective actions
Unacceptable defect Corrective action
Cracks Check material specificationCheck filler metal composition if usedCheck welding speedCheck weld shape
Lack of penetration Increase laser powerReduce welding speedImprove beam focusImprove gas shielding
Lack of fusion Improve beam alignment with respect to the joint
Porosity Check for and remove surface contaminationCheck gas for moisture and contaminationImprove gas shielding
Sheet misalignment Improve fit-up and accuracy of weld prepared components
Discoloration/oxidation Improve gas shieldingImprove gas quality
156 The welding of aluminium and its alloys
8.6 Combined laser and MIG welding head. Courtesy of TPS-Fronius Ltd.
8.7 Principles of operation of the laser/MIG process. Courtesy of TPS-Fronius Ltd.
which is generated a high-energy density beam of electrons of the order of0.25–2.5mm in diameter (Fig. 8.8).
The beam is generated by heating a tungsten filament to a high temper-ature, causing a stream of electrons that are accelerated and focused mag-netically to give a beam that gives up its energy when it impacts the target– the weld line. This enables very deep penetration to be achieved with a keyhole penetration mode at fast travel speeds (Fig. 8.9), providing low overall heat input.
The process may be used for the welding of material as thin as foil andup to 400mm thick in a single pass. The keyhole penetration mode givesalmost uniform shrinkage about the neutral axis of the component, leadingto low levels of distortion. This enables finish machined components to bewelded and maintained within tolerance. The transverse shrinkage alsoresults in the solidifying weld metal being extruded from the joint to givesome excess metal outside the joint (Fig. 8.10).
The major welding parameters are (a) the accelerating voltage, a 150kVunit being capable of penetrating 400mm of aluminium; (b) the currentapplied to the electron gun filament, generally measured in milliamperes;and (c) the travel speed. The item to be welded is generally mounted on anNC manipulator, the gun being held stationary. The unwelded joint com-ponents are required to be closely fitting and are usually machined. Filler
Other welding processes 157
8.8 A 2m3 chamber, 100kW, electron beam welding machine, showing the open vacuum chamber. It is capable or welding up to 200mm thick aluminium. Courtesy of TWI Ltd.
metal is not normally added but if gaps are present this leads to concavityof the weld face.
The major drawback with this process is the need to carry out the weldingin a vacuum chamber evacuated to around 10-3 to 10-2 Pa. This requiresexpensive diffusion pumps and a hermetically sealed chamber large enough to accommodate the item to be welded. The cost of equipment, theaccuracy with which components have to be machined to provide an accu-rate fit-up and the time taken to pump the chamber down can make theprocess non-competitive with more conventional fusion welding processes.For high-precision welding, perhaps of finished machined items whereminimal distortion is required and for batch type applications where anumber of items can be loaded into the chamber the process is capable ofproviding excellent results in a cost-effective manner.
Welding the aluminium alloys with the electron beam process presentsone problem specific to the process, that of metal vapour from the weldpool causing arcing inside the electron beam gun. This is a particularproblem with those alloys that contain low boiling point alloys such as mag-nesium and zinc. Arcing inside the gun interrupts the beam and causes cav-ities to be formed in the weld. This problem may be avoided by trappingthe vapour by changing the beam path with a magnetic field or by shuttingoff the beam as soon as arcing is detected and re-establishing the beam
158 The welding of aluminium and its alloys
KeyholeWeldpool Motion of
8.9 Principles of electron beam welding, illustrating keyhole weldingmode. Courtesy of TWI Ltd.
Other welding processes 159
8.10 Single pass electron beam weld in 450mm thick A5083 alloy. Note the excess weld metal extruded on the weld face due to thermal contraction. Courtesy of TWI Ltd.
immediately the vapour has dispersed. This can be done extremely rapidly,the weld pool remains molten and cavity formation is avoided. Althoughsome of the alloying elements, i.e. magnesium and zinc, are lost, this is gen-erally insufficient to cause a loss of strength. Elongated cavities in the fade-out region may be produced, particularly in circular components where arun-off tab cannot be used. These may be avoided by careful control of thetravel speed and beam fade-out.
The non-heat-treatable alloys can be welded fairly readily without theaddition of filler wire but hot cracking problems may be encountered in themore sensitive grades and in the heat-treatable alloys.As with laser welding,wire additions may help. Heat affected zones are small and strength lossesare less than would be experienced in a similar thickness arc welded joint.
8.5 Friction welding
Unlike the other processes covered in this book friction welding is a solidphase pressure welding process where no actual melting of the parent metaltakes place. The earliest version of the process utilised equipment similarto a lathe where one component was held stationary and the other held ina rotating chuck (Fig. 8.11). Rubbing the two faces together produces suf-ficient heat that local plastic zones are formed and an end load applied tothe components causes this plasticised metal to be extruded from the joint,
160 The welding of aluminium and its alloys
8.11 Conventional rotary motion friction welding. Courtesy of TWI Ltd.
carrying with it any contaminants, oxides, etc. Thus two atomically cleanmetal surfaces are brought together under pressure and an intermetallicbond is formed. The heat generated is confined to the interface, heat inputis low and the hot work applied to the weld area results in grain refinement.This rapid, easily controlled and easily mechanised process has been usedextensively in the automotive industry for items such as differential casings,half shafts and bi-metallic valves. Since the introduction of this conventionalrotating method of friction welding many developments have taken placesuch as stud welding, friction surfacing, linear and radial friction welding,taper plug welding and friction stir welding.
One very important characteristic of friction welding is its ability to weldalloys and combinations of alloys previously regarded as unweldable. It ispossible to make dissimilar metal joints, joining steel, copper and aluminiumto themselves and to each other and to successfully weld alloys such as the2.5% copper–Al 2618 and the AlZnMgCu alloy 7075 without hot cracking.The primary reason for this is that no melting takes place and thus no brittleintermetallic phases are formed.
8.5.1 Rotary/relative motion friction welding
The rotary/relative motion friction welding process (Fig. 8.11) is suited tothe joining of fairly regular shaped components, one of them ideally beingcircular in cross-section. Equal diameter tubes or bars are the best examplesince equal heating can take place over the whole contact area. There area couple of disadvantages to this process. The first is that one of the com-ponents must be rotated and this places a restriction on the shape and sizeof the items to be welded, the second is that items to be welded cannot bepresented to the mating part at an angle.
The welding parameters comprise the rotational speed which determinesthe peripheral speed, the pressure applied during the welding process andthe duration of the weld cycle. The metal extruded from the joint forms aflash on the outside of the weld and this is generally machined off to givea flat surface.
8.5.2 Friction stir welding
The most significant process for the welding of aluminium to be developedwithin the last decade of the twentieth century was the friction stir process,an adaptation of the friction welding process. This process was invented atTWI in the UK in 1991 and, unlike the conventional rotary or linear motionprocesses, is capable of welding longitudinal seams in flat plate. Despitebeing such a new process friction stir welds have already been launchedinto space in 1999 in the form of seams in the fuel tanks of a Boeing Delta
Other welding processes 161
II rocket (Fig. 8.12). It will soon be used for non-structural components inconventional commercial aircraft and is being actively considered for struc-tural use. Friction stir welding has also been introduced into shipyards withgreat success and is being actively investigated for applications in therailway rolling stock and automotive industries.
The process utilises a bar-like tool in a wear-resistant material, for alu-minium generally tool steel, a tool lasting in the region of 1–2 km of weldingbefore requiring replacement. The end of the bar is machined to form acentral probe and a shoulder, the probe length being slightly less than thedepth of the weld required. The bar is rotated and the probe plunged intothe weld line until the shoulder contacts the surface. The rotating probewithin the workpiece heats and plasticises the surrounding metal. Movingthe tool along the joint line results in the metal flowing from the front tothe back of the probe, being prevented from extruding from the joint bythe shoulders (Fig. 8.13). This also applies a substantial forging force whichconsolidates the plasticised metal to form a high-quality weld.
162 The welding of aluminium and its alloys
8.12 Launch of a Boeing Delta II Rocket in August 1999 containingfriction stir welded joints. Courtesy of TWI Ltd.
To provide support and to prevent the plasticised metal extruding fromthe underside of the weld a non-fusible backing bar must be used.A groovein the backing bar may be used to form a positive root bead – a simplemethod of determining that full penetration has been achieved (Fig. 8.14).
The technique enables long lengths of weld to be made without anymelting taking place (Fig. 8.15). This provides some important metallurgi-cal advantages compared with fusion welding. Firstly, no melting means thatsolidification and liquation cracking are eliminated; secondly, dissimilar and
Other welding processes 163
Sufficient downward force tomaintain registered contact
Advancingside of weld Joint
Leadingedge of therotating tool
Retreating sideof weld
Trailing edge ofthe rotating tool
8.13 Principle of the friction stir welding process. Courtesy of TWI Ltd.
8.14 Macro-section of 75mm thick A6082 double sided friction stir weld also illustrating a WhorlTM tool tip. Courtesy of TWI Ltd.
incompatible alloys that cannot be fusion welded together can be success-fully joined; thirdly, the stirring and forging action produces a fine-grainstructure with properties better than can be achieved in a fusion weld and,lastly, low boiling point alloying elements are not lost by evaporation. Otheradvantages are low distortion, no edge preparation, no porosity, no weldconsumables such as shield gas or filler metal and some tolerance to thepresence of an oxide layer.
One disadvantage to the process is that the ‘keyhole’ remains when thetool is retracted at the end of the joint. While this may not be a problemwith longitudinal seams where the weld may be ended in a run-off tab thatcan be removed, it restricts the use of the process for circumferential seams.This disadvantage has been overcome by the use of friction taper plugwelding. Tools with a retractable pin are also being investigated and havegiven some promising results.
Alloys that have been welded include the easily weldable alloys 5083,5454, 6061 and 6082 and the less weldable alloys 2014, 2219 and 7075. Inthe case of alloys in the ‘O’ condition tensile failures occur in the parentmaterial away from the weld. As far as the effect on the HAZ is concernedheat input is less than that of a conventional arc fusion weld. This results innarrow heat affected zones and a smaller loss of strength in those alloysthat have been hardened by cold-working or ageing. Table 8.3 lists the
164 The welding of aluminium and its alloys
8.15 2 metre long friction stir weld in 10mm thick A6082 alloy.Courtesy of TWI Ltd.
results of mechanical tests carried out by TWI Ltd as part of the investiga-tory programme. The results show that the ‘softening factor’, the ratiobetween the parent metal strength and that of the weld, in both the cold-worked and age-hardened alloys, is close to 1, implying that there is alimited loss of strength.
The softening factors of 0.83 for the 6082-T6 alloy can be compared withthe softening factor of 0.50 in Table 4.5 of BS 8118 for an arc weld in thesame alloy and condition. The design benefits once this reduction instrength loss can be taken advantage of in the design specifications areobvious.
Plate of 75mm thickness has been welded using a double sided techniqueat a welding speed of 60mm per minute. Plates in the thickness range 1.2–50mm have been welded in a single pass and at speeds of up to 1800mm/min. The process is completely mechanical and can be carried outwith simple machine tool equipment that requires very little maintenance.The conventional non-destructive testing techniques of radiography andultrasonic examination do not lend themselves to the interrogation of friction welds. However, the welding parameters are machine tool settingsand can be easily monitored and used to determine weld quality, any deviation from the required settings being cause for rejection.
Although this development is relatively recent it has been enthusiasti-cally adopted by the rail rolling stock manufacturers and a number of ship-yards in addition to its use in the aerospace industry.
Other welding processes 165
Table 8.3 Tensile test results for a range of friction stir welded alloys
Material 0.2% proof strength UTS Elongation Softening factor(N/mm2) (N/mm2) (%)
Resistance welding is a fusion welding process that requires the applicationof both heat and pressure to achieve a sound joint. The simplest form of the process is spot welding where the pressure is provided by clampingtwo or more overlapping sheets between two electrodes (Fig. 9.1).A currentis then passed between the electrodes, sufficient heat being generated at the interface by resistance to the flow of the current that melting occurs,a weld nugget is formed and an autogenous fusion weld is made betweenthe plates. The heat generated depends upon the current, the time thecurrent is passed and the resistance at the interface.The resistance is a func-tion of the resistivity and surface condition of the parent material, the size,shape and material of the electrodes and the pressure applied by the electrodes.
There are a number of variants of the resistance welding process includ-ing spot, seam, projection and butt welding. It is an economical processideally suited to producing large numbers of joints on a mass productionbasis. Spot welding in particular has been used extensively in the automo-tive industry, albeit mostly for the joining of steel and in the aerospaceindustry for airframe components in aluminium alloys. Seam welding isused in the production of thin sheet, leak-tight containers such as fuel tanks.Projection welding is generally used for welding items such as captive nutsonto plate. This variation is not normally used on aluminium and is notcovered in this chapter. Flash welding, unlike spot and seam welding thatrequire a lap joint, is capable of making butt welds.This is achieved by resis-tance heating the abutting faces and then forging them together.
There are a couple of characteristics of aluminium that make it more dif-ficult to resistance weld than steel. The most significant is its high electricalconductivity, requiring high welding currents and large capacity equip-ment. Secondly, the electrodes are made from copper which alloys withaluminium, resulting in rapid wear and a short electrode life.
9Resistance welding processes
As with conventional fusion welding, resistance welding suffers fromsimilar problems of oxide entrapment and hot cracking, the latter not beinghelped by the lack of a more crack-resistant filler metal, and porosity.
9.2 Power sources
The power sources are normally rated in kV A at 50% duty cycle so, if themaximum primary input power available is known, it is possible to calcu-late the maximum power output from the welding machine. There are fivetypes of power source commonly used for the welding of aluminium. Thesecomprise single phase AC or DC machines; three phase DC machines witheither primary or secondary rectification and inverter units with secondaryrectification. The choice of equipment depends on a number of factors suchas the primary current available, the output current required, the amountof space required between and around the electrodes, whether the equip-ment is required to be portable and the equipment cost.
9.2.1 Single phase AC units
The power source is simple, robust, relatively inexpensive and maintenancefree, comprising little more than a transformer and a suitable timer. Forthese reasons this form of power source has been popular for low-volumeapplications. However, the equipment is not very energy efficient as the secondary circuit suffers from substantial inductive losses. Demand on theprimary supply is also high and unbalanced between the phases: weldingcurrent can be high but the voltage is normally low, between about 3 and20 volts.
Resistance welding processes 167
Lap joint Welding current
9.1 Principles of spot welding process.
The spot welder may be pedestal mounted (Fig. 9.2) or portable. Withportable equipment the transformer may be remote from or incorporatedinto the welding gun. With portable equipment the weight of the trans-former makes the gun with the built-in transformer difficult to manipulateeven with counterweights to ease manual handling. The gun weight mayalso exceed the carrying capacity of welding robots. Using a power sourceremote from the gun requires heavy, stiff cables to deliver the weldingcurrent, again making the gun difficult to manipulate.
9.2.2 Single phase DC units
Single phase DC units are rather more energy efficient than the single phaseAC units as rectification of the current in the secondary circuit reduceslosses due to inductance. Power demand across the phases is also more bal-anced than the single phase units. Although the rectifier adds to the weightthe increased efficiency enables a lighter transformer to be used, giving anoverall reduction in weight. The equipment cost is greater than the simple
168 The welding of aluminium and its alloys
9.2 Modern pedestal mounted spot welder for aerospace applications.Courtesy of British Federal.
transformer AC unit but an improvement in weld quality can be used tojustify this increase.
As with the AC unit the welding gun may be pedestal mounted orportable. The limitations in cables apply when the power source is remotefrom the gun but the potential for a lighter transformer on gun weldinghead eases the manipulation problems apparent with the AC units.
9.2.3 Primary rectified three phase units
Primary rectified three phase units predate the advent of solid state elec-tronics, using ignitron or thyratron tubes for current control. They werewidely used in high-quality applications in industries such as aerospace.Half wave rectification of the primary current is used to provide the trans-former with DC to give a high-current, low-voltage output. It is possible toweld a wider range of materials and thicknesses with these more efficientunits. The length of the current pulse that these units are capable of pro-viding is limited before saturation of the transformer core occurs. Alternatespot welds are generally made with alternate polarities.
9.2.4 Secondary rectified three phase DC units
Secondary rectified three phase DC units are very energy efficient and arecapable of delivering very high welding currents, making them ideally suitedto the welding of aluminium alloys. They do, however, use very large andheavy transformers and diodes, making the equipment bulky and bestsuited for fixed and pedestal machines.
9.2.5 Secondary rectification inverter units
As mentioned in other chapters the development of solid state electronics,particularly inverter technology, has resulted in highly energy efficient,compact and light power units with weight savings of up to 50% comparedwith an AC unit of equivalent output. At high current output there is a riskof overheating and up until perhaps 1997 the maximum output was limitedto some 20kA but this value has now been increased to over 50kA. Thisenables these units to be used in high utilisation activities such as thoserequired in the automotive industry and to be mounted on robots for continuous operation (Fig. 9.3).
9.3 Surface condition and preparation
The surface condition of the aluminium sheets is one of the most impor-tant deciding factors in achieving consistent quality of resistance spot and
Resistance welding processes 169
seam welds.Variations in the thickness of the oxide film will affect the resis-tance between both the electrodes and the plates and at the plate interface.The resistance may be measured by clamping a single plate between twoelectrodes and applying a set current of some 10–15 A, measuring thevoltage and calculating the resistance by the use of Ohm’s Law. Material asdelivered may have a resistance of between 300 and several millionmicrohms, cleaned and prepared plate should have a resistance of 10–100microhms. For the highest and most consistent quality this range should betightened to some 10–30 microhms.
To achieve this low level of resistance the cleaning and storage recom-mendations in Section 4.7 should be followed. Mechanical abraded surfacesgenerally provide longer electrode lives than chemically cleaned surfaces,with mill finished sheets giving the shortest lives. Special lubricating oilssuch as polybutene have been used to extend electrode life by reducing the
170 The welding of aluminium and its alloys
9.3 Modern robotic resistance spot welding cell. The robot welds onone jig while the operator unloads/loads the second jig. Courtesy ofBritish Federal.
friction between electrode tip and the sheet but care needs to be taken toensure that there is not excessive oil present.
9.4 Spot welding
9.4.1 Spot welding principles and parameters
Spot welding is by far the most widely used variant of the resistance weldingprocess. The basic principles of the technique are illustrated in Fig. 9.1. Asmany as five overlapping sheets of aluminium may be welded together ina single operation. The weld nugget extends through the sheets but withoutmelting the surfaces of the outer plates. The main welding parameters arecurrent, pressure and time – typical parameters are given in Tables 9.1 and9.2. It is recommended that when developing a welding procedure the elec-trode sizes, the welding time and the welding force should be selected firstand the welding current increased until the desired nugget size is achieved.Minimum recommended nugget sizes for the thinner of two sheets beingwelded are as given in Table 9.3.
The welding force required by three phase frequency converter equip-ment is some 2 to 5 times that of the single phase AC units and for threephase secondary rectified machines somewhere in the region of 0.5 to 2times. Note that excessive forging force will result in indentation of thesheets, increased distortion and sheet separation. Too low a forging force
Resistance welding processes 171
Table 9.1 Typical welding parameters for 50Hz equipment single phase ACunits. Valid for 1XXX, 3XXX, 5XXX and 6XXX alloys
Sheet Electrode Dome Dome Electrode Welding Weldingthickness diameter radius radius force current time(mm) (mm) (top) (bottom) (kN) (kA) (cycles)
results in metal expulsion, surface burning because of poor contact, tip pick-up or contamination and internal defects of porosity and cracking.
If a forging force is required to assist in consolidating the weld, particu-larly for the crack-sensitive alloys this should be in the region of 2.5 to 3times the welding force. Welding current for three phase frequency con-verter units should be some 30% higher than for the single phase AC units.
A controlled up-slope on the welding current, say over two or threecycles, enables the electrodes to seat on the surface reducing metal expul-sion and surface overheating. A down-slope or current decay reduces therate of solidification and assists in consolidation of the weld nugget if a post-weld forge is used.
9.4.2 Welding head requirements
The welding head may be mounted on a pedestal, a bench, a dedicatedmachine, a manually operated boom or a robot.The simplest machine is themanually operated pedestal machine but even this may be supplementedwith automatic feed and ejection.The pedestal machines are capable of pro-
172 The welding of aluminium and its alloys
Table 9.2 Typical welding parameters for 50Hz equipment single phase DCunits. Valid for 1XXX, 3XXX, 5XXX and 6XXX alloys
Sheet thickness Electrode Dome Welding Welding Welding (mm) diameter radius force current time
viding the highest power output, with capacities ranging from 5 to400kVA. The portable guns such as those used on robots in the automo-tive industry generally range in capacity from 10 to 150kVA. The design ofthe welding head is important in reducing electrode tip wear, assisting inreducing porosity and cracking and enabling high production rates to beachieved. The head characteristics that affect electrode wear comprise thespeed at which the head approaches the job – larger equipment may havea two-speed head that applies the full force only after the initial electrodecontact is made. Although tip life is extended the slow approach speed willincrease the weld cycle time and reduce production rates. The inertia of thehead affects the speed of acceleration and deceleration and ideally the headshould be designed to be as light as possible consistent with rigidity. Toomuch flexure of the arms will result in accelerated electrode wear due tomovement between the electrode and the workpiece and unacceptableelectrode alignment.
Low inertia is also required during weld pool solidification.As the moltenweld metal cools and solidifies, the weld nugget contracts. The electrodemust be able to respond rapidly and be capable of following this slightdeformation if sound and high-quality welds are to be produced. A‘squeeze’ is therefore often applied, which assists in consolidating the weld,reducing shrinkage porosity and hot cracking.
9.4.3 Welding electrodes
The bulk of the cost of a spot weld is the cost of dressing or replacing theelectrode, the life being defined as the number of spot welds that can bemade with a pair of electrodes while maintaining a minimum weld nuggetdiameter. Pick-up of aluminium on to the tip and rapid wear are the twomain reasons for the short life of spot welding electrodes. High welding currents, surface finish and electrode forces further assist in shortening theelectrode life. It is not uncommon in very high-quality applications such asaerospace for the electrode to require cleaning after as few as 20 spot welds.
Electrode life may be extended by the use of replaceable caps on theelectrode tips or, it is claimed, by the use of copper alloys with increasedhardness which reduces mushrooming of the tip. Increases in hardness canbe achieved by alloying with zirconium or cadmium–chromium and dis-persion hardened with aluminium oxide. Of these the 1% Cd-Cu are usedfor the softer alloys with the harder 1% Cr-Cu or 21% Cr-Zr-Cu alloys forthe welding of the cold-worked or age-hardened alloys.
The profile of the electrode tip is important with respect to both the tiplife and weld quality. Tips may be conical, truncated conical, flat, domed orcylindrical. Of these types the truncated cone and the dome predominate.The most commonly recommended shape is the domed tip, the shape of
Resistance welding processes 173
which is more easily maintained in production than the truncated cone.Alignment is also less of an issue and is favoured particularly for portableequipment. The truncated cone tends to be used for commercial qualityapplications, mainly because electrode alignment is more critical and diffi-cult to maintain consistently in production. Tip life, however, is markedlybetter, by a factor of two to three, than can be achieved with the domedelectrode. Cone angles vary from 60° to 150° including an angle with a slightradius on the tip which aids in alignment and reduces marking of the sheet.The tip profile may be maintained by grinding, filing or by the use of abrasive cloth in a shaped former. While this dressing operation may beperformed manually it is difficult to maintain the correct tip shapeand electrode alignment. The use of automatic tip dressing tools or spe-cially designed hand-held manual or pneumatic tip dressers is stronglyrecommended.
Efficient electrode cooling is also necessary to maintain tip life. Largediameter electrodes will provide a greater heat sink but efficient watercooling is imperative. The cooling channel should be carried as close to thetip as possible, a distance of between 12 and 20mm being usual with waterflow rates of 5–10 litres/min. Water inlet temperature should be in theregion of 20°C and the outlet temperature in the region of 30°C.
9.4.4 Quality control
There is no specification available for the quality control of aluminium spotwelds within the UK although ASME IX includes rules for procedureapproval of spot welds.There is, however, a British Specification for the spotwelding of steel, BS 1140, which contains a multitude of recommendationsthat may also be applied to aluminium. The main method of demonstrat-ing acceptable quality is by means of the peel test, a simple, inexpensivetest, but this may be replaced or supplemented by a tension shear test or atwist test. The test piece for all three tests is essentially the same – two overlapping plates welded together with a single spot. An acceptable resultin the peel test is when the weld nugget is pulled out of the parent plate.
Monitoring of the welding parameters is an effective method of assuringquality during production welding. This monitoring may be very simple,detecting only the absence of a weld, or may be a sophisticated electroni-cally based monitor which will both monitor and record current, number ofcycles, pressure and time. This recording can be augmented by audible orvisual warning of out-of-range welding parameters. Finally, one of the mosteffective quality control methods is visual inspection where surface melting,adhesion of the electrodes, pits, cracks, asymmetry of the weld spot and
174 The welding of aluminium and its alloys
surface indentation can be readily identified. These features may be usedto assess the quality of production batches.
9.5 Seam welding
Seam welding uses a wheel-shaped electrode (Fig. 9.4) to make either aseries of overlapping spot welds to form a continuously welded and leaktight seam or a number of spot welds spaced apart – roll-spot welding. Therequirements on electrodes and surface finish are the same as for spotwelding. The shunt effect of the closely spaced nuggets and the short weldtimes mean that higher currents are necessary than for spot welds. Typicalwelding parameters are given in Table 9.4.
Higher welding forces will be needed for harder alloys and lower valuesfor softer alloys. Welding parameters for three phase frequency converter
Resistance welding processes 175
9.4 Typical resistance seam welder showing the copper wheelelectrodes. Courtesy of British Federal.
units are similar to those in Table 9.4 except that welding current needs tobe increased by between 0.5 and 2.5 times, the higher values for the thickermaterials.
Pick-up on the electrode wheel can be a problem and may require thewheel to be cleaned after only one revolution. Mechanised cleaning systemsthat remove the contamination in-process by wire brushing or abrasivemeans have been successful in maintaining continuous production.
9.6 Flash butt welding
9.6.1 Process principles
As the name suggests flash butt welding is capable of making butt joints inbar-like or tubular components, L,T and X-shaped extrusions, etc.The weldis a solid phase joint where the two ends of the component are forgedtogether at high temperature, any molten metal being expelled frombetween the two faces (Fig. 9.5). The process takes place in two phases, a‘flashing’ and an upsetting phase. The two components to be joined areclamped in electrodes, at least one of which is movable.A low-voltage, high-amperage current is applied without the two components being in contact.The parts are then brought together at a controlled rate, resulting in a seriesof brief short-circuits as the asperities on the faying faces melt and burn off.This continuous series of short-circuits raises the temperature of the endsand expels some of the molten metal, giving the ‘flashes’ that give theprocess its name.
The heating melts and plasticises the metal and, once sufficient heat hasbeen built up, the ends of the components are forged together, forcing outany melted metal, oxides and contaminants and some of the plasticisedmaterial, forming a ‘flash’ or ‘upset’. The expulsion of contaminants and
176 The welding of aluminium and its alloys
Table 9.4 Seam welding conditions. Single phase AC units. Hardened 5XXXseries alloy
Sheet Travel Spots/ On plus On time Welding Welding Weldthickness speed metre off time (cycles) current force(mm) (m/min) (cycles) (kA) (kN)
9.5 Principles of flash butt welding. Courtesy of TWI Ltd.
oxides means that pre-weld cleanliness is not as important as the conven-tional fusion welding processes. The weld is consolidated by this forgingaction, giving a high-strength joint even in heat-treatable alloys.The forgingaction also eliminates any cast structure and reduces the width of the HAZ.A monitor chart from a typical weld sequence is illustrated in Fig. 9.6.
9.6.2 Welding machines
The basis of the flash welding machine is an AC transformer, the majorityof production equipment being single phase machines. The electrodes orclamps are mounted on two rigid platens, at least one of which is movableand powered by a pneumatic or hydraulic system (Fig. 9.7). The capacity ofthe machine is limited by the current requirements of the joint and the upsetpressure available. The power demanded of the transformer is based on the cross-sectional area of the faying faces as a critical current density isrequired. The varying electrical conductivity of the different alloys also hasan effect on power requirements and the range of yield strengths placevarying demands on the upset pressure mechanism. As an approximation amachine capable of flash butt welding 65cm2 of steel can weld only some35cm2 of aluminium.
The current requirements for flash butt welding range from around12500 to 15500A/cm2 during the upset phase of welding. Current
requirements during the flashing stage will be some 30–50% less than theupset current. Voltages vary from 2 volts at a low cross-sectional area to 20volts for the thicker sections. The lowest voltage possible should be usedconsistent with stable flashing for the best results.
178 The welding of aluminium and its alloys
9.7 Schematic of a typical tube or bar flash welding machine. 1 = current sensing circuit 2 = upset control 3 = pressure transducer.
For the welding of steel copper alloys are generally used for the manufac-ture of the electrode clamps. For aluminium, however, steel, sometimescopper plated, has been found to give better results, conducting less heataway from the weld, providing a longer life and more positive clamping. Bydrawing the weld back through one of the clamps fitted with a knife edgeit is also possible to shear off the upset as part of the removal process. Abroach may be inserted into the bore of hollow components to remove anyinternal flash. To achieve a clean cut and to prevent smearing of the upsetduring removal the cutting edges must be kept sharp. The clamps aremachined to match the outside shape of the components and are split toenable rapid insertion. They are also designed to clamp around 80% of thecircumference and to be of a sufficient length that slippage does not occurduring upsetting.
To prevent crushing or deformation of hollow components removableinserts or backing devices may be used beneath the clamp area. Sufficientdistance must be left between the ends of the inserts to ensure that they donot take part in the welding operation.
9.6.4 Quality control
Provided that the equipment is correctly set-up and maintained, flash buttwelding is a trouble-free process. Alignment of the components is vital toachieve low rates of weld rejects. Failure to align the components can resultin ‘shelving’ where one component rides up over its partner and in unevenflashing, producing lack of fusion defects. Insufficient heat and/or inade-quate upset may both result in lack of fusion type defects or oxide entrap-ment. Both of these defects can be readily detected by the use of a bendtest such as those required by the procedure approval specification BS EN288 Part 4 – see Chapter 10, Table 10.3. Bend testing is a relatively inex-pensive method of assuring weld quality. Those non-destructive test tech-niques that are commonly used for interrogating arc-welded butt joints,such as radiography or ultrasonic examination, are not suitable for flashbutt welding and the engineer is forced to consider destructive tests. Bendtesting of pre-production test pieces prior to the start and at the end of aproduction period of some 8 hours is one of the most cost-effective andeasily performed techniques. When this testing is supplemented by in-process monitoring of the welding parameters (Fig. 9.6) then it is possibleto demonstrate a 100% acceptable weld quality. While it is written for thecontrol of steel flash butt welding the specification BS 4204 ‘Flash ButtWelding of Steel Tubes for Pressure Applications’ is an extremely usefulreference, full of information that may be applied to aluminium alloys. It
Resistance welding processes 179
gives recommendations on equipment choice, welding sequence control,procedure approval testing and production control testing. In addition thereis an example of a flash welding weld procedure record form and a list ofinformation required on a weld procedure specification.
180 The welding of aluminium and its alloys
Very often the decisions on how a weld should be made, filler metal andwelding parameter selection are left to the welder. While this may beacceptable in those situations where the weld quality is only incidental tothe integrity of the fabrication it is not acceptable where the weld is crucialto the performance of the component. The need for approved welders towork to approved welding procedures is also often a requirement of eitherthe application standard to which the fabrication is designed and con-structed or a contract specification requirement. Aside from these specifi-cation requirements it may be necessary for the fabricator to be able todemonstrate to clients, to regulatory authorities or, should a failure leadingto loss or damage occur, to a court of law that the welds have been madeto an acceptable quality.To specify how both the welds and the welders maybe shown to be acceptable there are a number of standards available to theengineer. The requirements of some of these standards are covered in thischapter.
It cannot be emphasised too strongly that the detail below is only asummary of the specification requirements and must be treated withcaution. Although best efforts have been made to ensure that the abstractsare accurate, they are only abstracts and accurate at the time of writing.Where compliance is a standard or contract requirement the latest editionof the approval standards must be consulted.
10.2 Welding procedures
A welding procedure or weld procedure specification (WPS) is a writteninstruction that specifies materials, consumables and edge preparations fora given joint. It lists the pre- and post-weld operations including heat treat-ments; machining, grinding and dressing of the weld; details the weldingvariables and the run sequence; and may specify the acceptance criteria and
10Welding procedure and welder approval
inspection methods. The purpose of the WPS is to ensure that acceptancecriteria can be met consistently, including mechanical properties and defectlevels. It is also useful in enforcing quality control procedures, in standard-ising on welding methods, production times and costs and in controlling pro-duction schedules. Its prime purpose, however, is to give the welder clear,unequivocal instructions on how a weld is to be made. A typical WPS isshown in Fig. 10.1.
In order to confirm that the welding procedure, if followed, is capable of providing the required strength and freedom from defects, the WPS isapproved or qualified. This approval is achieved by welding and testing a test piece representative of the production welds, the welding details and the test results being recorded in a weld procedure approval record(WPAR). In the American ASME specifications this is known as a proce-dure qualification record (PQR). Within the WPAR a number of essentialvariables are identified. These essential variables are those features of theprocedure that, if changed outside a range of approval, will result in anunacceptable change in the mechanical properties or defect level of theweld, invalidating the WPS and making re-approval necessary.
The procedure approval specifications detail the acceptable forms of testpieces, the essential variables and their ranges of approval, test methodsand acceptance standards. The most commonly encountered specificationsare the European specifications, the EN 288 series and the American specifications, the ASME codes.
10.2.1 The BS EN 288 specifications for arc welding approval
The EN series are all entitled ‘Specification and Approval of Welding Procedures for Metallic Materials’.
There are currently 9 parts of the EN specifications as follows:
• Part 1 General Rules for Fusion Welding.• Part 2 Welding Procedure Specification for Arc Welding.• Part 3 Welding Procedure Tests for the Arc Welding of Steel.• Part 4 Welding Procedure Tests for the Arc Welding of Aluminium and
its Alloys.• Part 5 Welding Approval by Using Approved Welding Consumables for
Arc Welding.• Part 6 Approval Related to Previous Experience.• Part 7 Approval by a Standard Welding Procedure for Arc Welding.• Part 8 Approval by a Pre-production Welding Test.• Part 9 Welding Procedure Test for Pipeline Welding on Land and Off-
shore Site Butt Welding of Transmission Pipelines.
182 The welding of aluminium and its alloys
Welding procedure and welder approval 183
Manufacturer’s WPS number
WPAR numberLocationManufacturerMain welding processRoot welding processJoint typeWelding position
IN ACCORDANCE WITH CLEANINGPROCEDURE CP015/AL
AIMg4, 5mNo.7BS EN 573 PI2 AW5083
From 12 To 25From >500 To
005/AL /82/PLWORKSALWELD SERVICES LTD131-MIG131-MIGButt-plate ss mbFLAT (PA)
Weldspec 4.01.161 (c) Copyright 2002 C-spec/TWI Software. All rights reserved worldwide.Page 1 of 1Catalog n° WPS00019
ALWELD SERVICES LTDGranta Park, Great Abington, Cambridge, CB1 6AL
EN288 – Manufacturer’s Welding Procedure Specification (WPS)Weldspec for Windows
10.1 Example of welding procedure specification (WPS) prepared inaccordance with BS-EN 288 Part 4.
Of the 9 parts of the EN 288 specification only Parts 1, 2 and 4 are dealtwith in this review.
Part 1 contains definitions and discusses briefly the methods of approvalcontained in Parts 3 to 8. It also requires WPSs to be prepared in accor-dance with Part 2.
Part 2 specifies the requirements for the contents of welding procedurespecifications for arc welding, listing all of the variables that need to beincluded and giving instructions as to how the weld shall be made. There isalso in Appendix A of the specification a copy of a suggested form for aWPS. See also Fig. 10.1.
Part 4 is the most important part within the series with respect to aluminium. It specifies how a WPS for the welding of aluminium or its alloysshall be approved. It gives the limits of validity of the WPS within the range of variables and includes an example of a WPAR and the accom-panying approval certificate. Copies of these are included in Appendix A of the specification. It lists the size and shape of the test pieces and thenon-destructive and mechanical tests required to prove the properties of the weld. It covers TIG, MIG and plasma-arc welding processes only,although it may be used as the basis for approving other processes by agreement.
In order to reduce the number of tests required the alloys are formedinto groups, each group having similar characteristics as listed in Table 10.1.The test pieces are representative of the joints to be welded in produc-tion, comprising plate and pipe butt welds, branch welds and fillets. Testpiece sizes are illustrated in Fig. 10.2. The test piece form, type of test and methods and extent of examination of the test pieces are detailed inTable 10.2.
184 The welding of aluminium and its alloys
Table 10.1 Aluminium alloy grouping system
Group Type of alloy
21 Pure aluminiumAluminium with less than 1.5% impurities, e.g. 1050, 1080, 1200, 1350Aluminium with less than 1.5% alloy additions, e.g. 3103
22 Non-heat-treatable alloys divided into two groups:22.1 Aluminium–magnesium alloys with 3.5% Mg or less, e.g. 3105, 5005,
5052, 5154, 545422.2 Aluminium–magnesium alloys with between 4% and 5.6% Mg, e.g.
5083, 5182, 508623 Heat-treatable alloys. These include the Al-Mg-Si and the Al-Zn-Mg
alloys, e.g. 6060, 6063, 6082, 6463, 7020, 7022, 7075
The range of approval for dissimilar metal joints is also covered. This isnot included in this chapter – for details reference should be made to clause188.8.131.52 of the specification. The position of the specimens within the testpiece is also illustrated in Fig. 10.2. Note that the bend coupon radius variesdepending upon the material group and the condition or temper of the testpiece as given in Table 10.3. Note also that allowance for strength loss inthe cross joint tensile test in cold worked or age hardened alloys is allowedfor in Table 2 of the specification.
Welding procedure and welder approval 185
Table 10.2 Test regime to BS EN 288 Part 4
Test piece Type of Extent of testingform test
1 Butt Visual examination to EN 970 100%Radiography or ultrasonics 100%Penetrant examination to EN 571-1 100%Transverse tensile test to EN 895 2 specimensTransverse bend test to EN 910 2 root
2 face at and over 12mm thick
4 side bend coupons may be substituted for the root and face bends
Macro-examination to EN 1321 1 sectionMicro-examination to EN 1321 1 section (only for
material groups22 and 23)
2 Branch Visual examination to EN 970 100%Penetrant examination to EN 571-1 100%Radiography or ultrasonics 100%
At and below50mm diameter radiography or ultrasonics is not mandatory
Macro-examination to EN 1321 2 sectionsMicro-examination to EN 1321 1 section (only for
material groups 22 and 23)
3 Fillet Visual examination to EN 970 100%Penetrant examination to EN 571-1 100%Macro-examination to EN 1321 2 sectionsMicro-examination to EN 1321 1 section (only for
material groups 22 and 23)
186 The welding of aluminium and its alloys
6 timesthickness –150 mm min.
6 times thickness–150 mm min.
25 mm min. discard
25 mm min. discard
Archive material fore.g. impact tests,additional tensiles, etc.
Macro/microsection Cross joint
tensile 2 off bendcoupons
2 off bendcoupons Cross joint
Minimum test plate size and test piece position – plate butt weld approval test
Minimum specimen length600 mm, irrespective ofdiameter. Weld in centre
2 off bendcoupons
2 off bendcoupons
Cross jointtensile 1 off
Archive material for, e.g.impact specimens, all weldtensile, etc.
Pipe top dead centre
Minimum test pipe size and test piece position – pipe butt weld approval test
10.2 Test piece positions for approval testing to BS EN 288 Part 4.
The ranges of approval of the essential variables are given in Clause 8 ofthe specification and comprise the following:
• The manufacturer. The approval is restricted to the manufacturer andworkshops or sites under his technical and quality control. Procedureapproval cannot be sub-contracted to a third party or transferred betweenfabricators.
• The parent metal. In order to reduce the number of tests required thealloys have been formed into groups with similar characteristics, asshown in Table 10.1.
• Parent metal thickness is approved over a range dependent upon the testpiece thickness. For the purposes of this the thickness is regarded (1) asthe thinner of the two materials when dissimilar thicknesses are weldedin a butt joint; (2) as the thinner of the two materials in a fillet weld; (3)as the thickness of the branch for a set-on branch; and (4) as the thick-ness of the main pipe for a set-in or set-through branch (Table 10.4).
Welding procedure and welder approval 187
Table 10.3 Bend coupon testing requirements – BS EN 288 Part 4
Material Former diametergroup
Temper or O F H14 H16 H18 H19 T4 T5 T7condition H112 H24 H26 H28 H29 T6
Butt, T-butt, branches, Butt, T-butt, branches,single run, one or multi-run, all filletsboth sides
t £ 3 0.8t to 1.1t t to 2t3 < t £ 12 0.8t to 1.1t 3 to 2t12 < t £ 100 0.8t to 1.1t 0.5t to 2t (max. 150)t > 100 0.8t to 1.1t 0.5t to 1.5t
All dimensions in millimetres.
There is a footnote to the table in the specification that infers that, wherea multi-process procedure is used to make the joint, the approval range ofthickness of weld metal from the individual processes should be based onthe approval range given in the table.The range of approval for a fillet weldis based on the throat thickness of the test piece and is given as 0.75a to1.5a where a is the throat. A test piece throat thickness of 10mm or moreapproves all fillet welds over 10mm throat.
An important point to remember is that a fillet weld approval providesno information on the mechanical properties of a joint.Where the fillet weldis to be load carrying it is necessary to perform a butt weld approval so thattensile data are available for design purposes.
• Test piece diameter is also an essential variable when welding pipes,tubes or hollow sections. Below 168.3mm outside diameter the approvalrange is 0.5D to 2D where D is the test piece diameter. At and above168.3mm OD the range is 0.5D to flat plates.
• Welding position has a range of approval based on the ease of makingthe joint. For example, a pipe butt weld made in the vertical-up (PF)position approves for all positions except vertical-down (PG). Similarlythere is a range of approval for joint type with an unbacked butt jointin pipe approving for all other butt and fillet welds. For full details ofthese ranges reference should be made to Tables 8 and 9 in the specifi-cation. A sketch explaining the welding positions and how they are designated is included as Fig. 10.3.
• Other essential variables comprise the welding process; filler metal classification; type of current; heat input when specified; preheat andinterpass temperature; post-weld heat treatment or ageing; the type ofboth shielding and backing gases; and the number of filler wires in MIGwelding.
Once the procedure is approved and the WPAR is written the approvalremains valid indefinitely provided that none of the essential variables are changed outside of their range of approval. This approval enables anynumber of welding procedures or work instructions to be written, providedthat the variables specified in the WPS are within the range of approval ofthe WPAR.
While the best effort has been made to provide an accurate summary ofBS EN 288 Part 4 and the information is correct at the time of writing it isrecommended that the specification is referred to when there is a require-ment to comply in the application standard or in contractual documents.
10.2.2 ASME IX welding and brazing qualifications
The principles of approval testing in this ASME code are very similar tothose adopted for the EN specifications. There are testing requirements for
188 The welding of aluminium and its alloys
standard test pieces, a list of essential and non-essential variables and the corresponding ranges of approval. ASME IX, however, covers a widerrange of welding processes, including all of the arc welding processes,laser and electron beam welding, electro-slag and electro-gas welding,stud welding, friction welding and oxy-gas welding. It also covers brazingapprovals, brazing operator and welder approvals.
The essential variables in the ASME code are as follows:
• The alloys are grouped under ‘P’ numbers, the members of a P-numbergroup having similar characteristics as listed in Table 10.5. Approval ofone alloy in the group approves for all the others in the group, a changein the P-number requires re-approval.Alloys not listed are ‘unassigned’.This means that the alloy has not been grouped and the specific alloyhas to be individually approved.
• Filler metals are grouped under ‘F’ numbers in a similar manner to theparent metals. The groups are given in Table 10.6.
• Thickness and joint type are essential variables. A butt weld approves a fillet weld but not vice versa, the approval range on thickness
Welding procedure and welder approval 189
10.3 Welding position designations in accordance with EN 288.
depending upon the test piece thickness as in Table 10.7. Fillet welds canbe approved by fillet test pieces sectioned to provide macro sectionsonly. The thickness range approved is unlimited.
• The welding position and the welding preparation are not essential variables.
• The addition or deletion of or a change in the shielding gas in the gasshielded processes requires a re-approval.
• The approval is limited to the manufacturer and sites under his or herdirect control.
Test piece Range of Range of weld Test specimensthickness thickness ‘T ’ metal thickness tapproved approved
<1.6mm T to 2T 2t 2 cross jointtensiles 2 root 2 face bends
1.6–9.6mm 1.6mm to 2T 2t 2 cross joint tensiles2 root 2 face bends
>9.6–19.2mm 4.8mm to 2T 2t (t < 19.2mm) 2 cross joint tensiles2T (t ≥ 19.2mm) 4 side bends
38.1mm and over 4.8mm to 2t (t < 19.2mm) 2 cross joint tensiles203.2mm 203.2mm 4 side bends
(t ≥ 19.2mm)
10.3 Welder approval
While the procedure approval test is performed to demonstrate acceptablemechanical properties, the welder approval test is carried out to demon-strate that the welder has a sufficient level of skill to deposit weld metal ofan acceptable quality. A similar philosophy to that for procedure approvalis adopted – a number of standard tests are called up in the standards, suc-cessful completion of which gives a range of approval for a number of essen-tial variables. Since the purpose of the test is to assess the skill of the welderthe essential variables are different from those of the procedure approvaltest. The specifications most frequently encountered are BS EN 287 Part 2and ASME IX.
10.3.1 BS EN 287 Part 2
BS EN 287 Part 2 complements the procedure approval specification BSEN 288 Part 4. The specification regards the welding process as an essen-tial variable and restricts the processes covered by the specification to MIG,TIG and plasma-arc welding although other processes may be approved byagreement (Table 10.8).
Materials are grouped for the purposes of approval as follows:
• Group W21, pure aluminium and aluminium–manganese alloys with lessthan 1.55Mn;
• Group W22 non-heat-treatable alloys;• Group W23 heat-treatable alloys.
Dissimilar metal joints are treated in a similar manner with a test piecemade in one group conferring approval to weld a number of combinationsas shown in Table 10.9.
Welding procedure and welder approval 191
Table 10.8 Material groups for which the welder isapproved
Test piece material group Range of approval
W21 W22 W23
W21 * X —W22 X * —W23 X X *
* Approved group.X Group also approved.— Not approved.
An approval test on wrought material gives approval to weld both castand wrought alloys within the same group and combinations of wroughtand cast material.Any alloys not contained within the grouping system mustbe approved individually.
The approval range for the filler metal and the shield gas is not perhapsas clear as that with the parent metal groups. A test made with a specificfiller metal and shielding gas gives approval to weld with any other fillermetal compatible with the parent metal group provided that there is nochange in the process or shield gas and that this does not require a changein the welder’s technique. This last variable is unfortunately not quantified.
Thickness and pipe diameter are both essential variables; the ranges ofapproval are given in Tables 10.10 and 10.11.
Joint type is an essential variable. An approval test on a pipe alsoapproves the welder for welding plate; a plate approval for welding pipe ofover 500mm; a plate butt weld made in the flat (PA) or horizontal–verticalposition (PC) position approves for butt joints in pipes of 150 mm or morein diameter welded in similar positions. A butt weld approves a fillet weld.Welding a backed test piece approves a double sided joint with a back-gouge but not for unbacked joints.
An approval test with a specific filler metal and gas combination approvesthe welder to weld with any filler metal and gas that are compatible with
192 The welding of aluminium and its alloys
Table 10.9 Range of approval for dissimilar metaljoints
Test piece material group Range of approval
W21 W21 welded to W22W22 W22 welded to W21W23 W22 welded to W21
W23 welded to W21W23 welded to W22
The filler metal must correspond to one of theparent metal groups.
Table 10.10 Range of approval on thickness
Test piece thickness t (mm) Range of approval
t £ 6 0.7t to 2.5t6 < t £ 15 6mm < t £ 40mm
Over 40mm thick a test at the specific thickness isrequired.
the parent metal, provided that this does not require a change in thewelder’s technique.
The last and perhaps the most important variable from the welder’s pointof view is the welding position as shown in Table 10.12, the principle beingthat a test carried out in a more difficult position approves for welding inthe easier positions. The specification requires that the test is carried outwith conditions similar to those to be used in production such as edgepreparation, position, welding time, preheat and heat input. The test piecemust have at least one stop and start in both the root run and in the cappingpass.
The test regimes for the various types of joint are given in Table 10.13.The acceptance standard is specified in EN 30042 ‘Guidance on Quality
Levels for Imperfections’ and is specified as defect level ‘C’ for excess weldmetal, excess convexity, excess throat thickness and penetration and level‘B’ for the remaining defects.
The welder may submit a second test piece if the first fails to achieve therequired standard. If this test piece also fails and the failure can be attrib-uted to a lack of skill then the welder is required to be re-trained beforebeing permitted to attempt the test once more. Successful completion of atest approves the welder for a period of two years although the approvalcertificate must be endorsed at six monthly intervals by the employer. Thiscan be done provided that the welder is engaged on work within the rangeof approval and that the work is of an acceptable quality. The period ofapproval can be extended beyond two years by the examining body pro-vided that the employer can produce documentary evidence such as sixmonthly radiographic, ultrasonic or fracture test reports.
10.3.2 ASME IX welder approval
The ASME code covers both procedure approval (qualification) and welderapproval. Welders are divided into two categories, those who performmanual or semi-automatic (MIG) welding and those who operate machineor automatic welding equipment. As with EN 287 Part 2 the welder must
Welding procedure and welder approval 193
Table 10.11 Range of approval on diameter
Test piece diameter D (mm) Range of approval
D £ 125 0.5D to 2DD > 125 ≥0.5D
For structural hollow sections ‘D ’ is the dimension of the smaller side.
Table 10.12 Approval related to test weld position
Welding position of approval test piece Range of approval
1) PB for pipes may be welded in two versions.(1) pipe: rotating; axis: horizontal; weld: horizontal vertical.(2) pipe: fixed; axis: vertical; weld: horizontal vertical.
2) This is an approved position and is covered by the other related tests.Key* indicates the welding position for which the welder is approved in the approval test.¥ indicates those welding positions for which the welder is also approved.— indicates those welding positions for which the welder is not approved.Reproduced with the permission of BSI under licence no. 2002 SK/0151. British Standards can be obtained from BSI Customer Services, 389 Chiswick High Road, London W4 4AL.
welds Butt welds Fillet welds
Pipe-axis and -angle
rotating fixed rotating 1) fixed
0° 90° 45° 45° 0° 90°
PG PF PD PA PG PF PC H-L045 PA PB PG PF PD2)
— — — ¥ — — — — ¥ ¥ — — —
— — — ¥ — — ¥ — ¥ ¥ — — —
¥ — — — — — — — — — — — —
— ¥ — ¥ — — — — ¥ ¥ — ¥ —
— ¥ ¥ ¥ — — — — ¥ ¥ — ¥ ¥
— — — — — — — — ¥ — — — —
— — — — — — — — ¥ ¥ — — —
* — — — — — — — — — — — —
— * — — — — — — ¥ ¥ — — —
— ¥ * — — — — — ¥ ¥ — — ¥
— — — * — — — — ¥ ¥ — — —
¥ — — — * — — — — — ¥ — —
— ¥ ¥ ¥ — * — — ¥ ¥ — ¥ ¥
— — — ¥ — — * — ¥ ¥ — — —
— ¥ ¥ ¥ — ¥ ¥ * ¥ ¥ — ¥ ¥
— — — — — — — — * — — — —
— — — — — — — — ¥ * — — —
¥ — — — — — — — — — * — —
— ¥ ¥ — — — — — ¥ ¥ — * ¥
be provided with a written welding procedure.There are a number of essen-tial variables for three of the processes relevant to aluminium as shown inTable 10.14. For information on the range of approval of the essential vari-ables reference should be made to the clause listed in Table 10.14, to befound in ASME IX.
196 The welding of aluminium and its alloys
Table 10.14 List of variables for welder approval to ASME IX
Main variable Clause Variables GMAW GTAW PAWnumber
Joint detail QW402.4 Delete backing Yes Yes YesQW402.7 Add backing No No No
Base metal QW403.2 Thickness No limit No limit No limitQW403.16 Pipe diameter Yes Yes YesQW403.18 P material group Yes Yes Yes
Filler metal QW404.14 ± Filler NA Yes YesQW404.15 Change F No. Yes Yes YesQW404.22 ± Inserts NA Yes YesQW404.30 Change in t Yes Yes Yes
Weld position QW405.1 Add position Yes Yes YesQW405.3 Vup vs Vdown Yes Yes Yes
Gas QW408.8 Delete backing Yes Yes YesElectrical QW409.2 Change transfer Yes NA NA
modeQW409.4 AC to DC NA Yes NAQW409.4 DC+ to DC- NA Yes NA
t is the weld deposit thickness.
Table 10.13 Test regime for welder approval
Test method Butt weld plate Butt weld pipe Fillet weld
Visual Yes Yes YesRadiography Yes1 Yes1 Not mandatoryBend or tensile Yes2 Yes2 Not mandatoryFracture Yes1 Yes1 Yes3,4
Macro (unpolished) Not mandatory Not mandatory Not mandatory4
Penetrant Not mandatory Not mandatory Not mandatory
1 Radiography or fracture test, not both.2 A tensile test may be used instead of a bend test for alloys with low ductility.A bend or tensile test must be carried out if the MIG welding process (131) isused.3 The examining body may request additional macro-testing and penetrantexamination.4 The fracture test may be replaced by at least 4 macro-sections.
Approval testing for a butt (groove) weld is by bend testing although thismay be replaced by radiography – it is permitted to use the first productionweld made by the welder for this approval. Qualification for a fillet weld isby macro-examination and fracture testing.
The approval is valid for a period of six months. Provided that the welderwelds with the relevant process within this six month period the approvalcan be extended indefinitely unless there is any reason to question thewelder’s competence.
10.3.3 BS EN 1418 welding personnel – approval testing
BS EN 287 Part 2 covers the approval of manual welders – BS EN 1418 has been produced to specify how operators of mechanised or automatedequipment should be approved.The full title of the specification is ‘WeldingPersonnel – Approval testing of welding operators for fusion welding and resistance weld setters for fully mechanized and automatic welding ofmetallic materials’. The specification makes it clear that only those opera-tors responsible for setting up and adjusting operating parameters duringwelding need to be approved. Programmers of equipment who do not actually operate the equipment in production are not required to beapproved, nor are resistance welding operators.
Definitions are given in clause 3 where:
• Automatic welding is defined as welding operations where all parame-ters are pre-set and cannot be adjusted during welding.
• Mechanised welding is where all of the activities are performed auto-matically but the welding variables can be changed during welding.
• Robotic welding is defined as automatic welding using a pre-programmed manipulator.
The welding operators or resistance weld setters may be approved by oneof four methods:
• By performing the welding procedure test specified in EN 288 Part 3 or 4.
• By performing a pre-production or production welding test. This testmay be carried out on non-standard test pieces, on test pieces simulat-ing production or on actual production items that have been identifiedas test pieces prior to welding. Testing is to the requirements of EN 288Part 8.
• By taking actual production items for testing. As in the point abovetesting is to the requirements of EN 288 Part 8.
• By performing a function test. In this the operator/resistance weld setteris required to know the relationship between parameter deviations and
Welding procedure and welder approval 197
welding results, to set and control the parameters in accordance with anapproved welding procedure, to test the operation of the welding unitand to be capable of recognising and reporting any malfunctions.AnnexB of the specification gives information of what knowledge the opera-tor/resistance weld setter would typically be expected to have.
Provided that the operator/resistance weld setter successfully completesone of the above tests then there is no limit to their range of approval. Thisis provided that they continue to work with the same type of welding unit,the welding process is not changed and they work in accordance with anapproved procedure.Automatic and robotic welding approval using a multi-run technique gives approval for welding with a single run but not viceversa; approval to weld without a sensor gives approval for welding with asensor but not vice versa; changing the robot type, system or control unitrequires re-approval as does any change to the other essential variables.
Provided that the operator/resistance weld setter works with reasonablecontinuity, i.e. no break is longer than six months, and there is no reason toquestion their competence then the approval is valid for a period of twoyears.The employer must endorse on the approval certificate at six monthlyintervals that this is so. If the employer keeps records of non-destructive ormechanical tests carried out at a maximum of six month periods and theseconfirm that the required quality is being maintained then the examiningbody can endorse the approval certificate at the end of the two year valid-ity period for further periods of two years.
198 The welding of aluminium and its alloys
Previous chapters have covered those defects and losses in strength thatmay be described as arising from metallurgical effects. This chapter coversthose defects that may be described as defects of geometry, their causes andthe non-destructive testing techniques that may be used to detect them.Many of these defects are caused by the welder, because of either a lack of care or a lack of skill, and emphasise the need for adequate training.Similarly, if non-destructive testing is to be correctly performed and defects accurately identified and sized, well-trained and experienced non-destructive evaluation (NDE) operatives are needed. A simple and inexpensive non-destructive examination technique that is sometimes overlooked is that of a thorough visual examination by a suitably trainedand experienced welding inspector. Such an examination will identify manydefects, particularly those of shape as listed in Section 11.2 below.
11.2 Defects in arc welding
A list of weld defects and their causes is given in Table 11.1. Other defectsnot listed are mainly those of geometry and include misshapen and incor-rectly sized welds,variable cap width and height,weld face roughness, incom-plete weld fill and asymmetry of fillet welds. These are all welder-inducedproblems,requiring improved shop-floor discipline and/or welder retraining.
If the required acceptance level for the defects listed above is not con-tained within a relevant application standard then it is the responsibility ofthe designer to select the appropriate quality level. A readily available specification to which the designer may refer for guidance is BS EN 30042‘Arc Welded Joints in Weldable Alloys, Guidance on Quality Levels forImperfections’. This document contains three quality levels, B stringent, Cintermediate and D moderate, the choice of which depends upon designconsiderations, subsequent fabrication activities such as rolling or pressing,
11Weld defects and quality control
Table 11.1 Weld defects, description and causes
ISO 6520 Defect Name Description CausesDefect no.
4011 Lack of side wall fusion Failure of weld metal to fuse to Current too low, travel speed too high, (Fig. 11.1) weld preparation incorrect torch angle, oxide film on prep.
surfaces, inadequate joint cleaning, weld preparation too narrow
4012 Lack of inter-run fusion Failure of weld metal to fuse to Current too low, travel speed too high, (Fig. 11.1) preceding run incorrect torch angle, inadequate
4013 Lack of root fusion Root bead fully penetrated but not Current too low, voltage too low, travel (Fig. 11.1) fused to root face speed too high, root face too thick, root
gap too wide, incorrect torch angle,inadequate cleaning
517 Poor restart (cold start) Lack of fusion beneath weld start Incorrect welder technique (see Section position 7.4.1), poor earthing
402 Lack of penetration Failure to achieve the minimum Current too low, travel speed too high, penetration specified by design incorrect torch angle, incorrect weld prep.
4021 Insufficient (lack of) root Failure of weld metal to penetrate Current too low, travel speed too fast, root (Fig. 11.2) penetration fully root faces face too thick, root gap too small,
incorrect torch angle, misalignment
504 Excess penetration Unacceptable protrusion of the root Current too high, travel speed too slow, (Fig. 11.3) bead root gap too wide, root face too thin
501 Root or face undercut Notch parallel to weld at weld toe. Current too high, travel speed too fast, (Fig. 11.4) Prevalent at top edge of PB fillet incorrect torch angle, inadequate cleaning
502 (butt) Excess convexity Excess weld metal on the face of a Current too high, travel speed too low,
503 (fillet) Excess weld metal butt or fillet weld incorrect torch manipulation(Fig. 11.5) (excess cap height)
511 Incomplete fill (face Insufficient weld metal fill giving Poor welder technique, travel speed too (Fig. 11.6) concavity or missed groove on weld face resulting in fast, current too low, incorrect torch
edge). Insufficient insufficient throat positioningthroat in fillet welds
515 Root concavity Root pass ‘sucked back’ to give a Current too high, root gap too wide, root (Fig. 11.7) shallow groove face too thin
510 Burn-through Localised loss of weld pool in root Current too high, travel speed too slow, root face too thin, root gap too large
506 Overlap (roll-over) Weld metal that has rolled over at Weld bead too large, current too high, (Fig. 11.8) the edges and not fused to the travel speed too slow, prevalent in horiz.–
parent metal. May be face or root vert. welds, inadequate cleaning
201 Porosity Gas entrapped in weld metal giving Dirty consumables, poorly cleaned or dirty a cavity. May be localised, weld preparations, contaminated shield uniformly distributed or aligned gas, contaminated (hydrogen containing)
parent metal – especially castings, oxide film on parent metal, porous gas hoses, leaks in gas delivery system, condensation, poor joint design trapping gas (see Chapter 2)
2016 Worm-hole (piping) Elongated gas cavity formed by Excessive current, travel speed too slowsolidification of large weld pool
2024 Crater pipe Elongated cavity in the weld finish Incorrect welder technique – lack of crater crater fill
100 Solidification cracking Cracks in weld produced during Incorrect choice of filler metal, failure to welding control dilution, incorrect edge
preparation, crack susceptible parent
Table 11.1 (cont.)
ISO 6520 Defect Name Description CausesDefect no.
metal, high restraint, high heat input (seeChapter 2)
104 Crater cracking Short longitudinal or star-shaped Incorrect welder technique, lack of crater crack in finish crater fill
100 Liquation cracking Cracking in the HAZ or in Incorrect filler metal, crack sensitive previously deposited weld metal parent metal, high restraint, high heat
input (see Chapter 2)
303 Oxide entrapment Oxide films trapped within the Oxide films in or on parent metal, oxide weld metal films in or on filler metal, oxygen in shield
gas, poor gas shielding, inadequate cathodic cleaning
3034 Puckering Excessive oxide entrapment from Poor gas cover, very high weld currentweld pool turbulence
3041 (tungsten) Tungsten or copper Accidental contact of the electrode Poor welder technique, incorrect 3042 (copper) inclusions (TIG) or contact tip (MIG) mechanised set-up
11.1 Defects 4011 lack of side wall fusion, 4012 lack of inter-runfusion, 4013 root fusion.
11.2 Defect 4021.
Excessive penetration (EP)
11.3 Defect 504.
11.4 Defect 501.
11.5 (a) Defect 502. (b) Defect 503.
Incomplete filling or underfill
11.6 Defect 511.
Root concavity (RC)RC
11.7 Defect 515.
11.8 Defect 506.
static or dynamic loading, temperature and corrosive conditions and theconsequences of failure.
11.3 Non-destructive testing methods
NDE may be used to reveal defects that would be difficult or impossible todetect by visual examination. The techniques are used during manufactureas a quality control tool to determine the quality of the work. The extentof NDE depends upon the application and the criticality of the joint and isgenerally specified in the relevant application standards or contract speci-fication. It is important for NDE to be included in the planning of the fabrication process as it can require substantial time and resources. Fullaccount of this must be taken if disruption of production and delays to theprogramme are to be avoided.
The requirement to perform NDE must also be taken into account duringthe design phase. As with welding, access for NDE must be planned intothe component. The implication of this is that both welding engineers anddesigners must be conversant with the techniques and their limitations ifthe processes are to be used effectively.
11.3.1 Penetrant examination
This is a technique that is capable of detecting surface breaking defects only.It relies upon a coloured or fluorescent dye, sprayed upon the surface,penetrating these defects. After cleaning the excess from the surface, thedye within the defect is drawn to the surface by spraying on a developer inthe case of the colour contrast dye or by exposing the surface to ultra-violetlight. The defect is revealed by the dye staining the developer or by fluorescing (Fig. 11.9).
Figure 11.10 is a photograph of a typical penetrant examination indica-tion. The fluorescent dye gives greater sensitivity than the colour contrastdye and does not require the use of a colour contrast developer but doesrequire the use of an ultra-violet light and preferably a darkened room.Thecleaners, penetrant dyes and developers can all be obtained in aerosol cans,making the process extremely portable and ideal for site use.
The dye used as a penetrant must be capable of penetrating narrowcracks but must not be removed from more open defects during the clean-ing operation carried out before the application of the developer. The dyemust have a high contrast with the developer. It is important that the testpiece is thoroughly pre-cleaned – any dirt, oil or water in the crack mayprevent the penetrant from entering. Degreasing should be carried out byswabbing or immersing the item in one of the proprietary cleaners, acetoneor methanol. Immersion in an ultrasonic cleaning bath is probably the best
Weld defects and quality control 205
method. Wire brushing or grinding should not be used unless it can be fol-lowed by an acid etch as mechanical methods of cleaning can smear overdefects and prevent the dye from penetrating.
Inspection in other than the flat position is difficult but penetrants havebeen developed with a jelly-like consistency that can be used to carry outinspections in the vertical and overhead positions.Automated methods maybe used, with the components loaded into baskets and processed on a con-
206 The welding of aluminium and its alloys
Beam of fluorescent light
Defect open to surfacePenetrant
Penetrant drawn intodefect
Penetrant cleaned offbut retained in defect
Penetrant drawn outand staining developer
Developer sprayed on
Fluorescent dye retainedin defect
11.9 Penetrant examination principles.
11.10 Liquid penetrant test result illustrating staining of the spray-ondeveloper by a defect in the HAZ. Courtesy of TWI Ltd.
veyor line. The fluorescent dyes are better in this application than colourcontrast dyes because of their greater sensitivity.
Sensitivity of the process can be checked using standard test blocks. Forthe examination of aluminium components, these are available in 2024 alloyheat treated to give real cracks of a standard size. These blocks should bescrupulously cleaned after each check to ensure that the cracks do notbecome clogged with debris.
Although the technique is simple to use, interpretation of the results canbe difficult, particularly if the surface is ‘naturally’ rough or if the dye istrapped in acceptable geometric features. Operatives should therefore betrained and, for many tasks, a qualification in penetrant examination iseither an application standard or contract requirement. Both the BritishInstitute of NDT (BINDT) and the American Welding Society (AWS) runaccreditation schemes.
There are few health and safety risks involved in using the technique.Thecleaners and some of the solvents in which the dye and developer are dis-solved will cause skin irritation if used with unprotected hands, and glovesare strongly recommended. The cleaners and solvent vapours will also needto be controlled if the process is used in confined spaces. Some of thesematerials are also flammable, so there are fire and explosion risks.
• It can be used on both ferrous and non-ferrous metals.• It is very portable.• Large areas can be examined very quickly.• It can be used on small parts with complex geometry.• It is simple, cheap and easy to use and interpret.
• It will only detect defects open to the surface.• Careful surface preparation and cleanliness are required.• It is not possible to retest a component indefinitely.• There may be health and safety problems with some of the chemicals.• There are health and safety problems with fumes in confined spaces.
11.3.2 Eddy current examination
Eddy current examination is a process that may be used on any materialthat will pass an electric current. A coil carrying an alternating current isplaced close to the item to be examined, inducing an eddy current in thespecimen. Defects in the specimen will interrupt this eddy current flow andthese perturbations can be detected by a second, search coil. The coils can
Weld defects and quality control 207
be placed either side of a thin plate-like sample or can be wound to giveside-by-side coils in a single probe. These may be shaped to fit in the boreor around the outside of pipes and tubes and in these applications the processlends itself to automation. The equipment is calibrated using a defect-freespecimen. The accuracy can be affected by metallurgical condition, stand-off and coil dimensions. For these reasons eddy current testing is used onlyrarely on welded components, although it is excellent in examining contin-uously welded tube from pipe mills. The process has been developed overrecent years to make it more portable and simpler to use. Microprocessor-based control and recording units, improved and more tolerant probes andlight-weight electronics have enabled the technique to be used on-site forthe examination of structures in service, where it is an effective tool for thedetection of cracking and corrosion problems. It is also possible for thedepth of surface cracks to be determined. It is of limited use for interro-gating welds, however, being most commonly used in the examination ofcontinuously welded tube, and is not covered further in this chapter.
11.3.3 Ultrasonic examination
The ultrasonic examination of welds uses the same principles as when sonaris used for the detection of submarines. A ‘sound’ wave emitted from atransmitter is bounced off an object and this reflection captured by areceiver. The direction and distance of the object can be determined bymeasuring the elapsed time between transmission and detection of the‘echo’. In welded components this is usually done by moving a small probe,containing both transmitter and receiver, over the item to be examined anddisplaying the echo on an oscilloscope screen. The probe transmits a beamof ultrasound that passes through the metal and is reflected back from anydefects, much like shining a torch at a mirror, in principle with the samerules applying to the reflection of the beam. This is illustrated in Fig. 11.11.Deeply buried defects such as lack of fusion, lack of penetration and cracksin addition to volumetric defects such as slag entrapment and porosity areall easily detected.
The success of the technique depends upon the use of trained, experi-enced operators who know precisely the characteristics of the metal beingexamined, the beam direction, its amplitude and frequency and the weldgeometry. It is recommended that operators should be approved to one ofthe certification schemes such as those operated by the BINDT or theASNT.
The frequency of the ultrasonic waves is generally in the range of 2–5MHz, the lower frequencies being used for the examination of coarse-grained material and on rough surfaces. The higher-frequency probes areused for the detection of fine defects such as cracks, non-metallic inclusions,
208 The welding of aluminium and its alloys
lack of fusion and voids. The beams are transmitted as either compressionwaves or shear waves and, ideally, a defect should be oriented normal tothe wave to give the maximum reflection. Projecting the beam at a glanc-ing angle at a planar defect can result in the beam being reflected awayfrom the receiver and lost – remember the analogy of the torch and themirror. The probe angle should be selected to optimise the reflection of thesound beam. Probes that project the beam into the test piece at an anglenormal to the plate surface are ideally suited to the detection of laminardefects, i.e. those lying parallel to the plate surface and for determining theplate thickness (Fig. 11.12).
Probes can be obtained that project the beam into the test piece at anangle, the most common being 45°, 60° and 70°. The angled probes are bestsuited for the detection of defects at an angle to the plate surface such as lack of sidewall fusion. Here the defect is at the angle of the original weld preparation and as illustrated in Fig. 11.13 is easiest to detect by aprobe of an appropriate angle. Note that the beam may be ‘skipped’ alongthe interior of a plate, enabling defects a long distance from the probe tobe found.
Before commencing the examination some preparation work is neces-sary. Data on material and heat treatment, welding process and procedureand weld preparation design are necessary if accurate determinations ofdefect types, orientations and sizes are to be made. The normal inspection
Weld defects and quality control 209
Horizontal CRT beamdeflection
Cathode Ray Tube(CRT) DISPLAYSCREEN
Vertical CRTbeam deflection
Electrical impulsefor pulse initiation
Signal from reflectedpulse (echo signal)
Reflected pulsesfrom defects
Signal base from time
Ultrasonic Test Set
11.11 Principles of ultrasonic testing of metals. Courtesy of TWI Ltd.
method is to scan the probe on the surface of the parent metal adjacent tothe weld. To do this the surface must be free of scale, spatter and roughnessand the parent metal should ideally be free of laminations and excessiveinclusions. A couplant, generally water, oil, grease or glycerine, is applied toform a film on the surface of the test piece. This aids the transmission ofthe beam into the sample.
210 The welding of aluminium and its alloys
Probe on specimen
Cathode ray screen
11.12 Compression wave examination. Courtesy of TWI Ltd.
Thin layerof couplant
Centre line ofultrasonic beam
Probe angle, α Probe index mark
11.13 Angle probe examination of a weld. Courtesy of TWI Ltd.
To ensure that all of the defects in both the weld and the HAZ aredetected the probe must be scanned over the full cross-section and the fulllength of the weld. Accurate sizing and positioning of any defects reliesupon accurate marking out of the weld. Flaws that lie parallel to the beammay be missed and to ensure that this does not occur it is necessary to scanin two directions at 90° to each other. Interpretation of the reflections fromregions such as root penetration beads, backing straps and fillet weld rootscan be very difficult, leading to incorrect defect sizing and sentencing. Forthis reason the root area is frequently excluded from the area to be ultra-sonically examined.
• It is very good for the detection of planar defects and cracks.• It can easily determine defect depth.• It is readily portable.• Access is required to one side only.• There are none of the health and safety problems associated with the
• Very skilled operators are required.• Surface breaking defects are difficult to detect.• Accurate sizing of small (<3mm) defects is difficult or impossible.• The geometry of the joint can restrict the scanning pattern and prevent
accurate interpretation.• No permanent objective record is available.• The process can be slow and laborious.
11.3.4 Radiographic examination
Electromagnetic radiation has properties that are useful for industrial radi-ography purposes. The rays travel in straight lines and cannot be deflectedor reflected by mirrors or lenses; they have wavelengths that enable theradiation to penetrate many materials, including most metals. They will,however, damage living tissue and therefore present some health and safetyproblems.
The radiation, either X-rays from a suitable source or gamma rays froma radioactive isotope, is absorbed as it passes through the material. Thisabsorption increases as the density of the material increases so that if a pho-tographic film is placed on the side opposite the radiation source, any lessdense areas will appear as darker areas on the film (Figs. 11.14 and 11.15),to give a shadow picture of the internal features of the test sample once thefilm has been processed. Thus voids, porosity, slag, cracks and defects of
Weld defects and quality control 211
212 The welding of aluminium and its alloys
Source of radiation
Image of cavity on film
11.14 Principles of radiographic examination of a weld. Courtesy ofTWI Ltd.
11.15 Radiograph of aluminium welds.(a) Longitudinal cracking at the weld start. Close square TIG butt weldin 7000 series alloy. (b) Gross porosity in TIG butt weld in 4000 seriesalloy.
geometry can all be identified, although planar defects normal to the beammay not be detected.
To radiograph a welded joint a suitable source of radiation, a film in alight-proof cassette and some method of processing the film are required.This latter generally requires a dark room where the film can be developed,fixed, washed, dried and viewed. The radiation can be produced from an X-ray tube, the energy generally being described by the voltage and currentat which the tube is operated. These may vary from 20kV to 30MV and 10to 30mA, although the normal limit for the commonly available industrialunits is around 400kV. A 400kV unit is capable of penetrating up to 100mm of steel and 200mm of aluminium. Gamma radiation is producedby the decay of a naturally occurring or manufactured radioactive isotope.The isotopes decay over a period of time, a measure of the longevity of thesource being the half life, the length of time taken for the source to decayto half of its initial intensity. The most common isotopes are cobalt-60, halflife 5.3 years; caesium-137, half life 30 years; iridium-192, half life 74 days;thulium-170, half life 127 days and ytterbium-169, half life 31 days. Thestrength of the source is expressed as curies or becquerels. As a gamma raysource cannot be switched off the isotope is stored in a special containerequipped with either a port that can be opened remotely to expose thesource or from which it can be wound out when required (Fig. 11.16).
Weld defects and quality control 213
11.16 Radioactive isotope projection system. Courtesy of TWI Ltd.
Neutron and electron guns are also used to produce high-energy beams.These can be used for interrogating materials in the same way as X- andgamma radiation. This equipment is not as readily available but has its usesin industry, particularly for very thick components where long exposuretimes would be required using conventional lower energy sources.
The quality of the radiograph is affected by the source to film distance – the greater this is the sharper the image; the size of the radiation source– the smaller the source the sharper the image; the beam energy – the higherthe energy the less sharp the image; the film grain size and quality and thecorrect film processing.To enable the radiographic quality to be determinedan image quality indicator (IQI) is used. This comprises a number of wiresof different diameters or a stepped wedge with varying diameters of holesdrilled in the steps. The IQI is placed on the source side of the test pieceand adjacent to or across the weld so that its image can be seen on the radi-ograph after processing. The diameter of the thinnest wire or the smallestdiameter hole that can be seen is then expressed as a percentage of thespecimen thickness – the percentage sensitivity of the radiograph.The otherquality control measure is the density of the radiograph which may be mea-sured easily with a densitometer. Ideally the density should be between 1.8and 2.5. Radiographs produced using X-radiation are generally of betterquality than those produced using gamma radiation. Variations in samplethickness will result in variations in density which may make parts of thefilm either too dark or insufficiently dense for accurate defect detection.
Real time radiographic equipment is now being more widely used. Thisuses a fluoroscopic screen and a video camera, enabling the image to bestored, retrieved, and automatically judged almost instantly. This hasobvious benefits with respect to the speed of identifying and correctingwelding faults.
Radiographic interpretation should be entrusted to well-trained experi-enced radiographers and should be performed in a darkened viewing roomon a viewer designed for the task.
• A permanent record is available.• Both buried and surface defects can be detected and the technique
is particularly good for finding volumetric defects such as slag andporosity.
• The equipment is portable, particularly the gamma ray sources.• All materials can be examined.
• The capital cost of equipment, which will need to include the process-ing and viewing facilities.
214 The welding of aluminium and its alloys
• Health and safety considerations – large areas may need to be closedoff during radiography or enclosures must be provided in which theradiography is carried out. Radiographers must also be monitored forexposure to radiation.
• Access is required to both sides of the component, the source on oneside, the film on the other.
• There are problems in detecting planar defects and fine cracks if theseare normal to the beam.
• There is a limitation on the thickness that can be radiographed anddefects easily detected.
• Skilled and experienced radiographers are required.• The depth and through thickness dimension of a defect is very difficult
Weld defects and quality control 215
Listed below are all of the European and ISO standards that are related tothe properties, composition and product forms of aluminium and its alloys.The list also includes design codes, welding specifications, procedure andwelder approval specifications, welding guides and health and safety speci-fications. The list is up to date at the time of writing – May 2002 – but itshould not be regarded as a definitive up-to-date listing as specifications, inparticular the EN and ISO standards, are being introduced on an on-goingbasis and the equivalent BS specifications withdrawn.
Appendix ABritish and ISO standards related to
welding and aluminium
No. Std source Number Part Year Title Key: Wholly or partially replaced byWithdrawnObsolescentReplaces
1 British BS 499 1991 Welding terms and symbols2 British BS 499 Part 1 1992 Welding brazing and thermal cutting glossary3 British BS 499 Part 2 1980 Specification for symbols for welding4 British BS 499 Part 2C 1992 Welding symbols BSEN 24063, BSEN
225535 British BS 499 Part 3 1992 Specification for symbols for welding BSEN 225536 British BS 638 Arc welding power sources, equipment and
accessories7 British BS 638 Part 4 1996 Specifications for welding cables8 British BS 638 Part 5 1988 Specifications for accessories BSEN 60974-129 British BS 638 Part 7 1984 Specifications for safety requirements for
installation and use10 British BS 638 Part 8 1984 BSEN 50078, BSEN
60974-1111 British BS 638 Part 9 1990 Specifications for power sources for
manual arc welding with limited power12 British BS 638 Part 10 1990 Specifications for safety requirements BSEN 60974-1:1990
for arc welding equipment: welding power sources
13 British BS 679 Specification for filters, cover lenses and BSEN 166:1996,backing lenses for use during welding BSEN 167:1995,and similar operations BSEN 168:1995,
Table A.1 (cont.)
No. Std source Number Part Year Title Key: Wholly or partially replaced byWithdrawnObsolescentReplaces
14 British BS 1470 1987 Specification for wrought aluminium and BSEN 485-1-4, BSENaluminium alloys for general engineering 515, BSEN 573 1-4purposes – drawn tube
15 British BS 1471 1972 Specification for wrought aluminium andaluminium alloys for general engineeringpurposes: drawn tube
16 British BS 1472 1972 Specification for wrought aluminium and ISO 209-1, ISO 209-2,aluminium alloys for general engineering BSEN 586 1&2,purposes: forging stock and forgings BSEN 604-1, BSEN
603 1&217 British BS 1473 1972 Specification for wrought aluminium and ISO 209-, ISO 209-2
aluminium alloys for general engineeringpurposes: rivet, bolt and screw stock
18 British BS 1474 Specification for wrought aluminium and ISO 6362, ISO 209-,aluminium alloys for general engineering ISO 209-2, BSEN purposes: bars, extruded round tubes 755 1-6and sections
19 British BS 1475 1972 Specification for wrought aluminium and BSEN 1301 1 to 3aluminium alloys for general engineering purposes – wire
20 British BS 1490 1988 Specification for aluminium and aluminium ISO 3522, ISO 7722,alloy. Ingots and castings for general BSEN 1676engineering purposes
21 British BS 2653 1955 Specification for protective clothing for BSEN 470-1welders
22 British BS 2901 Filler rods and wires for gas-shielded arcwelding
23 British BS 2901 Part 4 1990 Specification for aluminium and aluminiumalloys and magnesium alloys
24 British BS 3019 TIG welding25 British BS 3019 Part 1 Specification for TIG welding of aluminium, BSEN 1011-4
magnesium and their alloys26 British BS 3451 1981 Methods of testing fusion welds in BSEN 895,
aluminium and aluminium alloys BSEN 910, BSEN1320, BSEN 1321
27 British BS 3571 MIG welding28 British BS 3571 Part 1 1985 Specification for MIG welding of aluminium
and aluminium alloys29 British BS 4300 Specification for wrought aluminium and alloys
for general engineering purposes30 British BS 4300 Part 1 Part 1 Longitudinally welded tube31 British BS 4300 Part 4 Part 4 Solid extruded bars and sections32 British BS 4300 Part 10 Part 10 Drawn tube33 British BS 4300 Part 11 Part 11 Forging stock and forgings34 British BS 4300 Part 12 Part 12 Bars, extruded round tube and
sections35 British BS 4300 Part 13 Part 13 Welding wire36 British BS 4300 Part 15 Part 15 Bar, extruded round tube and sections37 British BS 7570 1992 Code of practice for validation of arc welding
equipment38 British BS 8118 Structural use of aluminium39 British BS 8118 Part 1 1991 Code of practice for design40 British BS 8118 Part 2 1991 Specification for materials, workmanship and
Table A.1 (cont.)
No. Std source Number Part Year Title Key: Wholly or partially replaced byWithdrawnObsolescentReplaces
41 European BS EN 166 1996 Personal eye-protection. Specifications42 European BS EN 167 1996 Personal eye-protection. Optical test methods43 European BS EN 168 1996 Personal eye-protection. Non-optical test
methods44 European BS EN 169 1992 Specification for filters for personal eye-
protection equipment used in welding andsimilar operations
45 European BS EN 287 Approval testing of welders for fusion welding46 European BS EN 287 Part 2 1992 Aluminium and aluminium alloys47 European BS EN 288 Specification and approval of welding
procedures for metallic materials48 European BS EN 288 Part 1 1992 General rules for fusion welding49 European BS EN 288 Part 2 1992 Welding procedure specification for arc welding50 European BS EN 288 Part 4 1992 Welding procedure tests for the arc welding of
aluminium and its alloys51 European BS EN 470 Protective clothing for use in welding and allied
processes52 European BS EN 470 Part 1 1995 General Requirements53 European BS EN 485 Aluminium and aluminium alloys. Sheet, strip
and plate54 European BS EN 485 Part 1 Part 1 Inspection and delivery conditions55 European BS EN 485 Part 2 Part 2 Mechanical properties56 European BS EN 485 Part 3 Part 3 Tolerance on shape and dimensions –
hot rolled products
57 European BS EN 485 Part 4 Part 4 Tolerance on shape and dimensions –cold rolled products
58 European BS EN 486 Aluminium and aluminium alloys. Extrusioningots
59 European BS EN 487 Aluminium and aluminium alloys. Rollingingots
60 European BS EN 515 1993 Aluminium and aluminium alloys. Wroughtproducts. Temper designations
61 European BS EN 573 Aluminium and aluminium alloys. Chemicalcomposition and form of wrought products
62 European BS EN 573 Part 1 Numerical designation system63 European BS EN 573 Part 2 Chemical symbol based designation system64 European BS EN 573 Part 3 Chemical composition65 European BS EN 573 Part 4 Forms of products66 European BS EN 575 Aluminium and aluminium alloys. Master
alloys produced by melting67 European BS EN 576 Aluminium and aluminium alloys. Unalloyed
aluminium alloys for remelting68 European BS EN 586 Aluminium and aluminium alloys. Forgings69 European BS EN 586 Part 1 Part 1 Inspection and delivery conditions70 European BS EN 586 Part 2 Part 2 Mechanical properties and additional
requirements71 European BS EN 601 Aluminium and aluminium alloys. Chemical
composition of castings in contact with food72 European BS EN 602 Aluminium and aluminium alloys. Wrought
products. Chemical composition of semi-products in contact with food
73 European BS EN 603 Aluminium and aluminium alloys. Wroughtforging stock
74 European BS EN 603 Part 1 Part 1 Inspection and delivery conditions75 European BS EN 603 Part 2 Part 2 Mechanical properties76 European BS EN 604 Aluminium and aluminium alloys. Cast forging
Table A.1 (cont.)
No. Std source Number Part Year Title Key: Wholly or partially replaced byWithdrawnObsolescentReplaces
77 European BS EN 604 Part 1 Part 1 Inspection and delivery conditions78 European BS EN 604 Part 2 Part 2 Tolerances on dimensions and form79 European BS EN 719 1994 Welding co-ordination. Tasks and
responsibilities80 European BS EN 729 Quality requirements for welding. Fusion
welding of metallic materials81 European BS EN 729 Part 1 1995 Guidelines for selection and use82 European BS EN 729 Part 2 1995 Comprehensive quality requirements83 European BS EN 729 Part 3 1995 Standard quality requirements84 European BS EN 729 Part 4 1995 Elementary quality requirements85 European BS EN 755 Aluminium and aluminium alloys. Extruded
rod/bar, tube and profiles86 European BS EN 755 Part 1 1997 Technical conditions for inspection and delivery87 European BS EN 755 Part 2 1997 Mechanical properties88 European BS EN 755 Part 3 1996 Round bars, tolerances on dimensions and form89 European BS EN 755 Part 4 1996 Square bars, tolerances on dimensions and
form90 European BS EN 755 Part 5 1996 Rectangular bars, tolerances on dimensions
and form91 European BS EN 755 Part 6 1996 Hexagonal bars, tolerances on dimensions and
form92 European BS EN 895 1995 Destructive tests on welds in metallic materials.
Transverse tensile test
93 European BS EN 910 1996 Destructive tests on welds in metallic materials.Bend tests
94 European BS EN 1301 Aluminium and aluminium alloys. Drawn wire95 European BS EN 1301 Part 1 1997 Technical conditions for inspection and delivery96 European BS EN 1301 Part 2 1997 Mechanical properties97 European BS EN 1301 Part 3 1997 Tolerances on dimensions98 European BS EN 1320 1997 Destructive tests on welds in metallic materials.
Fracture tests99 European BS EN 1321 1997 Destructive tests on welds in metallic materials.
Macroscopic and microscopic examination ofwelds
100 BS EN 1418 1998 Welding personnel – Approval testing of weldingoperators for fusion welding and resistanceweld setters for fully mechanised and automatic welding of metallic materials
101 European BS EN 1676 Aluminium and aluminium alloys. Alloyed ingots for remelting
102 European BS EN 1715 Aluminium and aluminium alloys. Drawingstock
103 European BS EN 1715 Part 1 Part 1 General requirements and technicalconditions for inspection and delivery
104 European BS EN 1715 Part 2 Part 2 Specific requirements for electricalapplications
105 European BS EN 1715 Part 3 Part 3 Specific requirements for mechanicaluses
106 European BS EN 1715 Part 4 Part 4 Specific requirements for weldingapplications
107 European BS EN 1780 Aluminium and aluminium alloys. Designationof unalloyed and alloyed aluminium ingots for remelting, master alloys and castings
108 European BS EN 1011 Welding recommendations for welding ofmetallic materials
Table A.1 (cont.)
No. Std source Number Part Year Title Key: Wholly or partially replaced byWithdrawnObsolescentReplaces
109 European BS EN 1011 Part 1 1998 General guidance for arc welding110 European BS EN 1011 Part 4 Arc welding of aluminium and aluminium alloys111 European BS EN 22553 1995 Welded, brazed and soldered joints. Symbolic
representations on drawings.112 European BS EN 24063 1992 Welded brazing, soldering and braze welding BS EN ISO 4063
of metals. Nomenclature of process and reference numbers for symbolic representation on drawings
113 European BS EN 50078 1994 Torches and guns for arc welding BS EN 60947-7114 BS EN 60974 Arc welding equipment115 BS EN 60974 Part 1 1998 Torches116 European BS EN 60974 Part 11 1996 Electrode holders117 European BS EN 60974 Part 12 1996 Coupling devices for welding cables
118 International BS EN ISO 4063 Welding and allied processes. Nomenclature ofprocess and reference numbers
119 International ISO 209 Part 1 1989 Wrought aluminium and aluminium alloys.Chemical composition and forms of products – Part 1 Chemical composition. 1st edition
120 International ISO 209 Part 2 1989 Wrought aluminium and aluminium alloys.Chemical composition and forms of products – Part 2 Forms of products. 1st edition
121 International ISO 3522 1984 Cast aluminium alloys. Chemical compositionand mechnanical properties, 2nd edition
122 International ISO 6362 Part 1 Wrought aluminium and aluminium alloys. Supersedes ISOExtruded rods/bars, tubes and profiles – 5191Technical conditions for inspection and delivery
123 International ISO 6362 Part 2 Wrought aluminium and aluminium alloys.Extruded rods/bars, tubes and profiles –mechanical properties
124 International ISO 6362 Part 3 Wrought aluminium and aluminium alloys.Extruded rods/bars, tubes and profiles.Extruded rectangular bars – tolerances ondimensions and form
125 International ISO 6362 Part 4 Wrought aluminium and aluminium alloysextruded rods/bars, tubes and profiles.Extruded profiles – Tolerances on shape anddimensions
126 International ISO 6362 Part 5 Wrought aluminium and aluminium alloys Replaces ISO 7273extruded rods/bars, tubes and profiles. Extruded round, square and hexagonal bars– tolerances on shape and dimensions
127 International ISO 7722 1985 Aluminium and aluminium alloy castingsproduced by gravity or chill sand casting or by related processes. General conditions forinspection and delivery
128 British BS.CP 119 The structural use of aluminium
129 Chemical CS 3039 Chromated marine glue144 prENV 1999-2 1997 Design of aluminium structures – structures
susceptible to fatigue
BSI British Standards Institution Sales Department, 389 Chiswick High Road, www.bsi.org.uk Tel:London W4 4AL 0208 996 7000
Al 99.99 1 660 660 0AW-1080A Al 99.8 1AAW-1070A Al 99.7AW-1050A Al 99.5 1B 635 659 24AW-1200 Al 99.0 1C 645 658 13AW-1350 Al 99.5 1EAW-2014 Al Cu4SiMg H15 510 635 125AW-2017(A) Al Cu4SiMg(A)AW-2024 Al Cu4Mg1 2L97/2L98AW-3003 Al Mn1Cu N3AW-3103 Al Mn1 N3 645 655 10AW-3004 Al Mn1Mg1AW-3005 Al Mn1Mg0.5AW-3105 Al Mn0.5Mg0.5 N31AW-4006 Al Si1FeAW-4007 Al Si1.5MnAW-4043a Al Si5 N21 577 630 53AW-4047A Al Si12 N2 577 585 8AW-5005 Al Mg1(B) N41AW-5040 Al Mg1.5MnAW-5049 Al Mg2Mn0.8AW-5050 Al Mg1.5(C)AW-5251 Al Mg2 N4 625 650 25AW-5052 Al Mg2.5AW-5056A Al Mg5 N6 575 630 55AW-5154A Al Mg3.5(A) N5 595 640 45AW-5454 Al Mg3Mn N51AW-5554 Al Mg3Mn N51AW-5356A Al Mg5AW-5556A Al Mg5.2MnCr N61AW-5754 Al Mg3
Alloy designations: wrought products 229
Table A.4 (cont.)
BS EN BS EN Old BS/DTD Temperature (°C)numerical chemical number
AW-5182 Al Mg4.5Mn0.4AW-5083 Al Mg4.5Mn0.7 N8AW-5086 Al Mg4AW-6061 Al Mg1SiCu H20 575 640 45AW-6063 Al MgSi H9 605 655 50AW-6082 Al SiMgMn H30 600 650 50AW-7005 Al ZnAW-7020 Al Zn4.5Mg1 H17AW-7021 Al Zn5.5Mg1.5AW-7022 Al Zn5Mg3CuAW-7075 Al Zn5.5MgCu DTD5074AAW-8011(A) Al FeSi(A)
age hardening see precipitation hardeningalloy elements 35–36alloying interstitial and substitutional 14alloy metallurgy 40–46
alloy grouping 184range of approval 187–188test regime 185–187
In compiling this book the author has drawn freely on a large number of textbooksand published papers, none of which are referenced in the text. Listed below aresome of the sources of information that have been used and other useful referencescontaining more information than it has been possible to include in this practicalguide to welding. Some of these references include specific information on the par-ticular topic, others are included for those who wish to gain a more general under-standing of the principles of metallurgy, the uses of aluminium and the weldingprocesses covered in the main text.
It has been attempted to list the books and papers under the relevant chapternumbers when they are specific to the topic, for example most of the books refer-enced under Chapter 2 are texts on general metallurgy, Chapter 6 contains a list ofreferences specific to TIG welding. This has not always been possible, hence theinclusion of General textbooks on welding which contains a listing of books thatcover more than one process. It may surprise some readers to see that specificationshave been referenced as useful sources of information. As mentioned elsewhere,specifications are documents that have been written by experts in their field andgenerally contain recommendations and requirements that are a summary of bestpractice. The shop floor engineer ignores these recommendations at his or her peril!
Included at the end of this listing are the web sites and/or addresses of a numberof organisations that can provide many of the books referenced.
Chapter 1Aluminium and its Applications, M. Conseva et al., Edimet Spa. ISBN 88-86259-
01-8.American Society for Materials Handbook Vol. 20 – Materials Selection and Design,
A.S.M. ISBN 0-87170-386-6.Science and Use of Engineering Materials, E. Crane et al., Butterworths Ltd. ISBN
Chapter 2An Introduction to Metallurgy, A.H. Cottrell, Edward Arnold Ltd. ISBN 7131-
2044-4.Elements of Materials Science and Engineering, L.H. Van Vlack, Addison-Wesley
Pub. Co. ISBN 0-201-52822-3.
Mechanical Metallurgy, G.E. Dieter, McGraw-Hill Book Co. ISBN 0-07-100406-8.Metallurgy for the Non-Metallurgist, Author and publisher American Society of
Metals. ISBN 0-87170-652-0.Metallurgy of Welding, J.F. Lancaster,Woodhead Publishing Limited, ISBN 1-85573-
428-1.Modern Physical Metallurgy, R.E. Smallman, Butterworth and Co.Welding Metallurgy, Sindo Kou, John Wiley and Sons. ISBN 0-471-84090-4.
Chapter 3Aluminium and Its Alloys, F. King, Ellis Horwood Ltd. ISBN 0-7458-0013-0.Corrosion of Aluminium and Aluminium Alloys, Author and publisher American
Society of Metals. ISBN 0-87170-629-6.Introduction to Aluminium Alloys and Tempers, Author and publisher American
Society of Metals. ISBN 0-87170-689-X.Light Alloys – Metallurgy of the Light Metals, I. Polmear, Edward Arnold Ltd. ISBN
0-7131-2819-4.Properties of Aluminium Alloys – Tensile, Creep and Fatigue Data at High and Low
Temperatures, J.G. Kaufman, Aluminium Association. ISBN 0-87170-632-6.Weldability of Al-Zn-Mg Alloys, Tao Ma, Delft University of Technology. ISBN
Chapter 4Recommended Practices for Plasma Arc Cutting, Author and publisher American
Welding Society. ISBN 0-87171-219-9.
Chapter 5Fatigue Design of Welded Joints and Components (Recommendations of IIW
Working Group XIII–XV), A. Hobbacher et al., Woodhead Publishing Limited.ISBN 1-85573-315-3.
Fatigue Strength of Welded Structures, S.J. Maddox, Abington Publishing. ISBN 1-85573-013-8.
Welded Design – Theory and Practice, J. Hicks, Abington Publishing. ISBN 1-85573-537-7.
General textbooks on welding (includes both TIG and MIG welding)Advanced Welding Systems – Vol. 1 Fundamentals of Fusion Welding Technology,
Jean Cornu, IFS (Publications) ISBN 0-948507-69-1.ANSI/AWS D8.14M Specification for Automotive and Light Truck Components
Weld Quality – Aluminium Arc Welding,Author and Publisher American WeldingSociety. ISBN 0-87171-591-0.
Arc Welding Automation, H.B. Cary, Marcel Decker Inc. ISBN 0-8247-9645-4.ASM Handbook Vol. 6. Welding, Brazing and Soldering, Author and publisher
American Society of Materials. ISBN 0-87170-382-3.AWS D 3.7. Guide for Aluminium Hull Welding. Author and publisher American
Welding Society. ISBN 0-67171-320-9.AWS D 10.7. Aluminium and Aluminium Alloy Pipe. Recommended Practices for
Gas Shielded Arc Welding. Author and publisher American Welding Society.ISBN 0-87171-260-1.
Health and Safety in Welding and Allied Processes, 5th edition, J. Blunt and N. Balchin, Woodhead Publishing Limited. ISBN 1-85573-538-5.
Joints in Aluminium – INALCO ’98. Conference Proceedings edited by M.H. Ogleet al., Woodhead Publishing Limited. ISBN 1-85573-417-6.
Process Pipe and Tube Welding, ed. by W. Lucas,Abington Publishing. ISBN 1-85573-012-X.
The Science and Practice of Welding, 2 volumes. A.C. Davies, Cambridge UniversityPress. ISBN 0-521-43565-X and 0-521-43566-8.
Welding and Cutting, P. Houldcroft, Woodhead Publishing Limited. ISBN 1-85573-578-4.
Welding Handbook, Vols. 1 and 2. Author and publisher American Welding Society.ISBN 0-87171-281-4 and 0-87171-354-3.
Welding Kaiser Aluminium, Author and publisher Kaiser Aluminium and ChemicalSales. ISBN No.
Chapter 6Advanced Welding Systems – Vol. 3. TIG and Related Processes, Jean Cornu, IFS
(Publications). ISBN 0-948507-71-3.AWS B2.1.015. GTAW of Aluminium M-22 or P22. 10 to 18 gauge as welded with
or without backing. Author and publisher American Welding Society. ISBN 0-87171-369-1.
BS 3019 TIG Welding Part 1 Specification for TIG Welding of Aluminium and Magnesium Alloys. Author and publisher British Standards Institution. ISBN 0-580-14124-1.
Practical TIG (GTA) Welding, P.W. Muncaster, Abington Publishing. ISBN 1-85573-020-0.
TIG and Plasma Welding, W. Lucas, Abington Publishing. ISBN 1-85573-005-7.
Chapter 7Advanced Welding Systems – Vol. 2. Consumable Electrode Processes, Jean Cornu,
IFS (Publications) ISBN 0-948507-70-5.BS 3571 MIG Welding. Part 1 Specification for MIG Welding of Aluminium and
Aluminium Alloys. Author and publisher British Standards Institution. ISBN 0-580-14260-4.
Chapter 8AWS C 6.1 Recommended Practices for Friction Welding. Author and publisher
American Welding Society. ISBN 0-87171-309-8.ANSI/AWS C 7.1 Recommended Practices for Electron Beam Welding. Author and
publisher American Welding Society. ISBN 0-87171-580-5.ANSI/AWS C 7.2 Recommended Practice for Laser Beam Welding, Cutting and
Drilling. American Society of Welding. ISBN 0-87171-562-7.Electron Beam Welding, H. Schultz, Woodhead Publishing Limited. ISBN 1-85573-
050-2.Europe Follows Japan into Friction Stir Welding, J. Davenport et al., TWI Ltd.Industrialisation of Friction Stir Welding for Aerospace Structures, S.W. Kallee et al.,
Laser Welding, P.A. Hilton et al., Woodhead Publishing Limited. ISBN 1-85573-518-0.